
#=======================================================================
data_global
#=======================================================================

_audit_creation_method                   'Jana2006 Version : 01/05/2018'


# 1. PROCESSING SUMMARY (IUCr Office Use Only)

_journal_date_recd_electronic            ?
_journal_date_to_coeditor                ?
_journal_date_from_coeditor              ?
_journal_date_accepted                   ?
_journal_date_printers_first             ?
_journal_date_printers_final             ?
_journal_date_proofs_out                 ?
_journal_date_proofs_in                  ?
_journal_coeditor_name                   ?
_journal_coeditor_code                   ?
_journal_coeditor_notes
; ?
;
_journal_techeditor_code                 ?
_journal_paper_category                  ?
_journal_techeditor_notes
; ?
;
_journal_coden_ASTM                      ?
_journal_name_full                       'Acta Crystallographica Section C'
_journal_year                            ?
_journal_volume                          ?
_journal_issue                           ?
_journal_page_first                      ?
_journal_page_last                       ?
_journal_suppl_publ_number               ?
_journal_suppl_publ_pages                ?

#=======================================================================

# 2. SUBMISSION DETAILS

_publ_contact_author_name                ?
_publ_contact_author_address
; ?
;
_publ_contact_author_email               ?
_publ_contact_author_fax                 ?
_publ_contact_author_phone               ?

_publ_requested_journal                  'Acta Crystallographica Section C'
_publ_requested_category                 ?

_publ_contact_letter
; ?
;

#=======================================================================

# 3. TITLE AND AUTHOR LIST

_publ_section_title
; ?
;
_publ_section_title_footnote
; ?
;
loop_
 _publ_author_name
 _publ_author_footnote
 _publ_author_address
; ?      # name
;
; ?      # footnote
;
; ?      # address
;

#=======================================================================

# 4. TEXT

_publ_section_synopsis
; ?
;
_publ_section_abstract
; ?
;
_publ_section_comment
; ?
;
_publ_section_introduction
; ?
;
_publ_section_experimental
; ?
;
_publ_section_exptl_prep
; ?
;
_publ_section_exptl_refinement
; ?
;
_publ_section_exptl_solution
; ?
;
_publ_section_discussion
; ?
;
_publ_section_acknowledgements
; ?
;
_publ_section_references
;
Petricek, V., Dusek, M. & Palatinus L. (2014). Z. Kristallogr. 229(5), 345-352.

Palatinus L. & Chapuis G. (2007). J. Appl. Cryst. 40, 786-790.

# enable this reference if Diamond ver. 2 was used for visualization
#Brandenburg, K. (1999). DIAMOND. Version. 2.1c.
#Crystal Impact GbR, Bonn, Germany.

# enable this reference if Diamond ver. 3 was used for visualization
#Brandenburg, K. & Putz, H. (2005). DIAMOND Version 3.
#Crystal Impact GbR, Postfach 1251, D-53002 Bonn, Germany.

# enable this reference if SIR97 was used for solving of the structure
#Altomare, A., Burla, M. C., Camalli, M., Cascarano, G., Giacovazzo, C.,
#Guagliardi, A., Moliterni, A. G. G., Polidori, G., Spagna, R. (1997).
#SIR97. A Package for Crystal Structure Solution by Direct Methods
#and Refinement, Bari, Rome, Italy.

# use this reference if SIR2002 was used for solving of the structure
#Burla, M.C., Camalli, M., Carrozzini, B., Cascarano, G., Giacovazzo, C.,
#Polidori, G., Spagna, R.
#SIR2002: the program, J. Appl. Cryst, (2003). 36, 1103


# use this reference if SIR2011 was used for solving of the structure
#Burla, M.C., Caliandro, R., Camalli, M., Carrozzini, B., Cascarano,
#G.L., Giacovazzo, C., Mallamo. M., Mazzone, A., Polidori, G., Spagna, R.
#SIR2011: a new package for crystal structure determination and refinement,
#J.Appl.Cryst. (2012) 45, 357-361

# enable this reference if bond valences were calculated
#Brown, I. D. (1996). J. Appl. Cryst. 29, 479-480.

# enable this reference if Xshape wase used for crystal shape refinement
#Stoe & Cie (1998). X-SHAPE. Stoe & Cie, Darmstadt, Germany.


# enable this reference if Flack coefficient was refined
#Flack, H. D. (1983). Acta Cryst. A39, 876-881.
;
_publ_section_figure_captions
; ?
;
_publ_section_table_legends
; ?
;

#=======================================================================
data_I
#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic
; ?
;
_chemical_name_common                    alcantarillaite
_chemical_formula_moiety                 ?
_chemical_formula_structural             ?
_chemical_formula_analytical             ?
_chemical_formula_iupac                  ?
_chemical_formula_sum
'As3.13 Ca0.44 Fe3.3 H8.9 K0.11 Mg0 Na0.05 O19 P0.7 W0.43'
_chemical_formula_weight                 855.6
_chemical_melting_point                  ?
_chemical_compound_source                ?
_chemical_absolute_configuration         .

#=======================================================================

# 6. CRYSTAL DATA

_symmetry_cell_setting                   orthorhombic
_symmetry_space_group_name_H-M           'I m m a'
_symmetry_space_group_name_Hall          '-I -2x;-2yb;-2zb'
_symmetry_Int_Tables_number              74

loop_
 _space_group_symop_id
 _space_group_symop_operation_xyz
 1   x,y,z
 2   -x,-y+1/2,z
 3   -x,y+1/2,-z
 4   x,-y,-z
 5   -x,-y,-z
 6   x,y+1/2,-z
 7   x,-y+1/2,z
 8   -x,y,z
 9   x+1/2,y+1/2,z+1/2
 10  -x+1/2,-y,z+1/2
 11  -x+1/2,y,-z+1/2
 12  x+1/2,-y+1/2,-z+1/2
 13  -x+1/2,-y+1/2,-z+1/2
 14  x+1/2,y,-z+1/2
 15  x+1/2,-y,z+1/2
 16  -x+1/2,y+1/2,z+1/2

_cell_length_a                           24.038(8)
_cell_length_b                           7.444(3)
_cell_length_c                           10.387(3)
_cell_angle_alpha                        90
_cell_angle_beta                         90
_cell_angle_gamma                        90
_cell_volume                             1858.6(11)

loop_
 _twin_individual_id
 _twin_individual_mass_fraction_refined
 _twin_individual_twin_matrix_11
 _twin_individual_twin_matrix_12
 _twin_individual_twin_matrix_13
 _twin_individual_twin_matrix_21
 _twin_individual_twin_matrix_22
 _twin_individual_twin_matrix_23
 _twin_individual_twin_matrix_31
 _twin_individual_twin_matrix_32
 _twin_individual_twin_matrix_33
 ? ? ? ? ? ? ? ? ? ? ?

_cell_formula_units_Z                    4

_cell_measurement_reflns_used            3061
_cell_measurement_theta_min              1.7
_cell_measurement_theta_max              31.2
_cell_measurement_temperature            100
_cell_special_details
; ?
;

_exptl_crystal_density_diffrn            3.0575
_exptl_crystal_density_meas              ?
_exptl_crystal_density_method            ?
_exptl_crystal_F_000                     1607

_exptl_absorpt_coefficient_mu            11.006
_exptl_crystal_description               blade
_exptl_crystal_size_max                  0.10
_exptl_crystal_size_mid                  0.02
_exptl_crystal_size_min                  0.002
_exptl_crystal_size_rad                  ?
_exptl_crystal_colour                    colorless
_exptl_absorpt_correction_type           empirical
_exptl_absorpt_process_details           ?
_exptl_absorpt_correction_T_min          0.40
_exptl_absorpt_correction_T_max          0.75
loop_
 _exptl_crystal_face_index_h
 _exptl_crystal_face_index_k
 _exptl_crystal_face_index_l
 _exptl_crystal_face_perp_dist
 ? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details                   ?

_diffrn_ambient_temperature              100
_diffrn_source                           synchrotron
_diffrn_source_power                     ?
_diffrn_source_voltage                   ?
_diffrn_source_current                   ?
_diffrn_radiation_type                   synchrotron
_diffrn_radiation_source                 synchrotron
_diffrn_radiation_wavelength             0.7107
_diffrn_radiation_monochromator          ?
_diffrn_measurement_device               ?
_diffrn_measurement_device_type          "area detector"
_diffrn_detector                         "area detector"
_diffrn_detector_area_resol_mean         ?
_diffrn_measurement_method               ?
_diffrn_measurement_specimen_support     ?

_diffrn_reflns_number                    15140
_diffrn_reflns_theta_min                 1.69
_diffrn_reflns_theta_max                 31.19
_diffrn_reflns_theta_full                29.25
_diffrn_measured_fraction_theta_max      0.9
_diffrn_measured_fraction_theta_full     0.98
_diffrn_reflns_av_R_equivalents          0.1007
_diffrn_reflns_av_unetI/netI             0.0368
_diffrn_reflns_limit_h_min               -33
_diffrn_reflns_limit_h_max               33
_diffrn_reflns_limit_k_min               -9
_diffrn_reflns_limit_k_max               9
_diffrn_reflns_limit_l_min               -13
_diffrn_reflns_limit_l_max               13
_diffrn_reflns_reduction_process         ?

_diffrn_standards_number                 ?
_diffrn_standards_interval_count         ?
_diffrn_standards_interval_time          ?
_diffrn_standards_decay_%                ?
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
  ? ? ?

_diffrn_radiation_probe                  X-ray

#=======================================================================

# 8. REFINEMENT DATA

_refine_special_details
; ?
;

_reflns_number_total                     651
_reflns_number_gt                        528
_reflns_threshold_expression             'I>2σ(I)'

_refine_ls_structure_factor_coef         F
_refine_ls_R_factor_gt                   0.0748
_refine_ls_wR_factor_gt                  0.0767
_refine_ls_R_factor_all                  0.0885
_refine_ls_wR_factor_ref                 0.0776
_refine_ls_goodness_of_fit_ref           3.54
_refine_ls_goodness_of_fit_gt            3.95
_refine_ls_restrained_S_gt               ?
_refine_ls_restrained_S_all              ?
_refine_ls_number_reflns                 651
_refine_ls_number_parameters             89
_refine_ls_number_restraints             0
_refine_ls_number_constraints            5
_refine_ls_weighting_scheme              sigma
_refine_ls_weighting_details             'w=1/(σ²(F)+0.0001F²)'
_refine_ls_hydrogen_treatment            'constr'
_refine_ls_shift/su_max                  0.0398
_refine_ls_shift/su_mean                 0.0078
_refine_diff_density_max                 1.27
_refine_diff_density_min                 -1.32
_refine_ls_extinction_method             'none'
_refine_ls_extinction_coef               ?
_refine_ls_extinction_expression         ?
_refine_ls_abs_structure_details         ?
_refine_ls_abs_structure_Flack           ?
_refine_ls_abs_structure_Rogers          ?

loop_
 _atom_type_symbol
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 As   0.0499  2.0058
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 Ca   0.2262  0.3064
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 Fe   0.3463  0.8444
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 H    0.0000  0.0000
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 K    0.2009  0.2494
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 Mg   0.0486  0.0363
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 Na   0.0362  0.0249
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 O    0.0106  0.0060
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 P    0.1023  0.0942
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 W   -0.8490  6.8722
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection               ?
_computing_cell_refinement               ?
_computing_data_reduction                ?
_computing_structure_solution            ?
_computing_structure_refinement          ?
_computing_molecular_graphics            ?
_computing_publication_material          ?

loop_
 _restr_distance_atom_site_label_1
 _restr_distance_site_symmetry_1
 _restr_distance_atom_site_label_2
 _restr_distance_site_symmetry_2
 _restr_distance_target
 _restr_distance_target_weight_param
 ? ? ? ? ? ?

loop_
 _restr_angle_atom_site_label_1
 _restr_angle_site_symmetry_1
 _restr_angle_atom_site_label_2
 _restr_angle_site_symmetry_2
 _restr_angle_atom_site_label_3
 _restr_angle_site_symmetry_3
 _restr_angle_target
 _restr_angle_target_weight_param
 ? ? ? ? ? ? ? ?

loop_
 _restr_torsion_atom_site_label_1
 _restr_torsion_site_symmetry_1
 _restr_torsion_atom_site_label_2
 _restr_torsion_site_symmetry_2
 _restr_torsion_atom_site_label_3
 _restr_torsion_site_symmetry_3
 _restr_torsion_atom_site_label_4
 _restr_torsion_site_symmetry_4
 _restr_torsion_angle_target
 _restr_torsion_weight_param
 ? ? ? ? ? ? ? ? ? ?

loop_
 _restr_equal_distance_atom_site_label_1
 _restr_equal_distance_site_symmetry_1
 _restr_equal_distance_atom_site_label_2
 _restr_equal_distance_site_symmetry_2
 _restr_equal_distance_class_class_id
 _restr_equal_distance_class_target_weight_param
 ? ? ? ? ? ?

loop_
 _restr_equal_angle_atom_site_label_1
 _restr_equal_angle_site_symmetry_1
 _restr_equal_angle_atom_site_label_2
 _restr_equal_angle_site_symmetry_2
 _restr_equal_angle_atom_site_label_3
 _restr_equal_angle_site_symmetry_3
 _restr_equal_angle_class_class_id
 _restr_equal_angle_class_target_weight_param
 ? ? ? ? ? ? ? ?

loop_
 _restr_equal_torsion_atom_site_label_1
 _restr_equal_torsion_site_symmetry_1
 _restr_equal_torsion_atom_site_label_2
 _restr_equal_torsion_site_symmetry_2
 _restr_equal_torsion_atom_site_label_3
 _restr_equal_torsion_site_symmetry_3
 _restr_equal_torsion_atom_site_label_4
 _restr_equal_torsion_site_symmetry_4
 _restr_equal_torsion_class_class_id
 _restr_equal_torsion_class_target_weight_param
 ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_adp_type
 _atom_site_U_iso_or_equiv
 _atom_site_site_symmetry_multiplicity
 _atom_site_occupancy
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
  Fe1 Fe 0.25 0.25 0.25 Uani 0.0593(15) 4 1 d . . .
  Fe2 Fe 0.3339(7) 0.5 0.5 Uani 0.060(4) 8 0.775(9) d . . .
  W2 W 0.3155(8) 0.519(3) 0.495(2) Uani 0.060(4) 16 0.112(4) d . . .
  As1 As 0.38593(11) 0.25 0.2800(2) Uani 0.0626(10) 8 0.76(2) d . . .
  P1 P 0.38593(11) 0.25 0.2800(2) Uani 0.0626(10) 8 0.24(2) d . . .
  O1 O 0.4419(6) 0.25 0.1872(16) Uani 0.095(6) 8 1 d . . .
  O2 O 0.3279(6) 0.25 0.1939(12) Uani 0.070(5) 8 1 d . . .
  O3 O 0.3856(4) 0.4315(11) 0.3727(7) Uani 0.073(4) 16 1 d . . .
  O4a O 0.2762(8) 0.559(2) 0.6217(17) Uiso 0.052(3) 16 0.5 d . . .
  O4b O 0.2556(7) 0.562(3) 0.6186(19) Uiso 0.052(3) 16 0.5 d . . .
  O5 O 0.3274(5) 0.25 0.5719(11) Uani 0.063(4) 8 1 d . . .
  As2 As 0.2123(3) 0.0261(9) 0.5131(7) Uiso 0.059(3) 16 0.264(7) d . . .
  As3 As 0.2716(3) 0.3076(7) 0.6920(6) Uiso 0.067(4) 16 0.216(7) d . . .
  Ca Ca 0.1759(9) 0 0.5 Uiso 0.084(8) 8 0.34(2) d . . .
  Fe3 Fe 0.5 0.3608(14) 0.1082(9) Uiso 0.063(4) 8 0.258(10) d . . .
  O6 O 0.2056(8) 0.25 0.6063(18) Uiso 0.0611 8 0.59(3) d . . .
  Ow1 O 0.5 0.554(6) 0.261(4) Uiso 0.063(4) 8 0.258(10) d . . .
  Ow2 O 0.5581(9) 0.5 0 Uiso 0.063(4) 8 0.52(2) d . . .
  Ow3 O 0.086(3) 0.25 0.697(7) Uiso 0.139(18) 8 0.36(5) d . . .
  Ow4 O 0.059(2) 0.25 0.891(5) Uiso 0.139(18) 8 0.36(5) d . . .
  Ow5 O 0 0.088(19) 0.014(13) Uiso 0.139(18) 8 0.15(4) d . . .
  Ow6 O 0.060549 0.25 0.759908 Uiso 0.139(18) 8 0.44(6) d . . .


loop_
 _jana_atom_site_ADP_C_label
 _jana_atom_site_ADP_C_type_symbol
 _jana_atom_site_ADP_C_111
 _jana_atom_site_ADP_C_112
 _jana_atom_site_ADP_C_113
 _jana_atom_site_ADP_C_122
 _jana_atom_site_ADP_C_123
 _jana_atom_site_ADP_C_133
 _jana_atom_site_ADP_C_222
 _jana_atom_site_ADP_C_223
 _jana_atom_site_ADP_C_233
 _jana_atom_site_ADP_C_333
 ? ? ? ? ? ? ? ? ? ? ? ?

loop_
 _jana_atom_site_ADP_D_label
 _jana_atom_site_ADP_D_type_symbol
 _jana_atom_site_ADP_D_1111
 _jana_atom_site_ADP_D_1112
 _jana_atom_site_ADP_D_1113
 _jana_atom_site_ADP_D_1122
 _jana_atom_site_ADP_D_1123
 _jana_atom_site_ADP_D_1133
 _jana_atom_site_ADP_D_1222
 _jana_atom_site_ADP_D_1223
 _jana_atom_site_ADP_D_1233
 _jana_atom_site_ADP_D_1333
 _jana_atom_site_ADP_D_2222
 _jana_atom_site_ADP_D_2223
 _jana_atom_site_ADP_D_2233
 _jana_atom_site_ADP_D_2333
 _jana_atom_site_ADP_D_3333
 ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
 _jana_atom_site_ADP_E_label
 _jana_atom_site_ADP_E_type_symbol
 _jana_atom_site_ADP_E_11111
 _jana_atom_site_ADP_E_11112
 _jana_atom_site_ADP_E_11113
 _jana_atom_site_ADP_E_11122
 _jana_atom_site_ADP_E_11123
 _jana_atom_site_ADP_E_11133
 _jana_atom_site_ADP_E_11222
 _jana_atom_site_ADP_E_11223
 _jana_atom_site_ADP_E_11233
 _jana_atom_site_ADP_E_11333
 _jana_atom_site_ADP_E_12222
 _jana_atom_site_ADP_E_12223
 _jana_atom_site_ADP_E_12233
 _jana_atom_site_ADP_E_12333
 _jana_atom_site_ADP_E_13333
 _jana_atom_site_ADP_E_22222
 _jana_atom_site_ADP_E_22223
 _jana_atom_site_ADP_E_22233
 _jana_atom_site_ADP_E_22333
 _jana_atom_site_ADP_E_23333
 _jana_atom_site_ADP_E_33333
 ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
 _jana_atom_site_ADP_F_label
 _jana_atom_site_ADP_F_type_symbol
 _jana_atom_site_ADP_F_111111
 _jana_atom_site_ADP_F_111112
 _jana_atom_site_ADP_F_111113
 _jana_atom_site_ADP_F_111122
 _jana_atom_site_ADP_F_111123
 _jana_atom_site_ADP_F_111133
 _jana_atom_site_ADP_F_111222
 _jana_atom_site_ADP_F_111223
 _jana_atom_site_ADP_F_111233
 _jana_atom_site_ADP_F_111333
 _jana_atom_site_ADP_F_112222
 _jana_atom_site_ADP_F_112223
 _jana_atom_site_ADP_F_112233
 _jana_atom_site_ADP_F_112333
 _jana_atom_site_ADP_F_113333
 _jana_atom_site_ADP_F_122222
 _jana_atom_site_ADP_F_122223
 _jana_atom_site_ADP_F_122233
 _jana_atom_site_ADP_F_122333
 _jana_atom_site_ADP_F_123333
 _jana_atom_site_ADP_F_133333
 _jana_atom_site_ADP_F_222222
 _jana_atom_site_ADP_F_222223
 _jana_atom_site_ADP_F_222233
 _jana_atom_site_ADP_F_222333
 _jana_atom_site_ADP_F_223333
 _jana_atom_site_ADP_F_233333
 _jana_atom_site_ADP_F_333333
 ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 10. MOLECULAR GEOMETRY


loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_site_symmetry_1
 _geom_bond_site_symmetry_2
 _geom_bond_distance
 _geom_bond_publ_flag
  Fe1 Fe2 . . 3.778(9) ?
  Fe1 Fe2 . 10_564 3.778(9) ?
  Fe1 Fe2 . 13_555 3.778(9) ?
  Fe1 Fe2 . 6_546 3.778(9) ?
  Fe1 W2 . . 3.60(2) ?
  Fe1 W2 . 10_564 3.53(2) ?
  Fe1 W2 . 11_555 3.60(2) ?
  Fe1 W2 . 4_566 3.53(2) ?
  Fe1 W2 . 13_555 3.60(2) ?
  Fe1 W2 . 6_546 3.53(2) ?
  Fe1 W2 . 7_555 3.60(2) ?
  Fe1 W2 . 16_544 3.53(2) ?
  Fe1 As1 . . 3.282(3) ?
  Fe1 As1 . 11_555 3.282(3) ?
  Fe1 P1 . . 3.282(3) ?
  Fe1 P1 . 11_555 3.282(3) ?
  Fe1 O2 . . 1.961(14) ?
  Fe1 O2 . 11_555 1.961(14) ?
  Fe1 O4a . 10_564 2.048(18) ?
  Fe1 O4a . 4_566 2.048(18) ?
  Fe1 O4a . 6_546 2.048(18) ?
  Fe1 O4a . 16_544 2.048(18) ?
  Fe1 O4b . 10_564 1.960(19) ?
  Fe1 O4b . 4_566 1.960(19) ?
  Fe1 O4b . 6_546 1.960(19) ?
  Fe1 O4b . 16_544 1.960(19) ?
  Fe1 As2 . . 3.327(7) ?
  Fe1 As2 . 10_554 3.332(7) ?
  Fe1 As2 . 11_555 3.327(7) ?
  Fe1 As2 . 4_556 3.332(7) ?
  Fe1 As2 . 13_555 3.327(7) ?
  Fe1 As2 . 6_556 3.332(7) ?
  Fe1 As2 . 7_555 3.327(7) ?
  Fe1 As2 . 16_554 3.332(7) ?
  Fe1 As3 . 10_564 3.388(6) ?
  Fe1 As3 . 4_566 3.388(6) ?
  Fe1 As3 . 6_546 3.388(6) ?
  Fe1 As3 . 16_544 3.388(6) ?
  Fe1 Ca . . 3.657(11) ?
  Fe1 Ca . 10_554 3.657(11) ?
  Fe1 Ca . 13_555 3.657(11) ?
  Fe1 Ca . 6_556 3.657(11) ?
  Fe2 Fe2 . 6_546 3.722(3) ?
  Fe2 Fe2 . 6_556 3.722(3) ?
  Fe2 W2 . . 0.47(3) ?
  Fe2 W2 . 4_566 0.47(3) ?
  Fe2 W2 . 6_546 3.605(19) ?
  Fe2 W2 . 6_556 3.893(19) ?
  Fe2 W2 . 7_555 3.893(19) ?
  Fe2 W2 . 7_565 3.605(19) ?
  Fe2 As1 . . 3.202(7) ?
  Fe2 As1 . 4_566 3.202(7) ?
  Fe2 P1 . . 3.202(7) ?
  Fe2 P1 . 4_566 3.202(7) ?
  Fe2 O3 . . 1.886(15) ?
  Fe2 O3 . 4_566 1.886(15) ?
  Fe2 O4a . . 1.93(2) ?
  Fe2 O4a . 4_566 1.93(2) ?
  Fe2 O4b . . 2.30(2) ?
  Fe2 O4b . 4_566 2.30(2) ?
  Fe2 O5 . . 2.011(5) ?
  Fe2 O5 . 4_566 2.011(5) ?
  Fe2 As2 . 6_556 2.932(19) ?
  Fe2 As2 . 7_555 2.932(19) ?
  Fe2 As3 . . 2.876(11) ?
  Fe2 As3 . 4_566 2.876(11) ?
  Fe2 As3 . 6_556 3.386(10) ?
  Fe2 As3 . 7_555 3.386(10) ?
  Fe2 Ca . 6_556 3.80(3) ?
  W2 W2 . 4_566 0.31(3) ?
  W2 W2 . 6_546 3.72(3) ?
  W2 W2 . 6_556 3.72(3) ?
  W2 W2 . 7_555 4.01(3) ?
  W2 W2 . 7_565 3.43(3) ?
  W2 As1 . . 3.45(2) ?
  W2 As1 . 4_566 3.36(2) ?
  W2 P1 . . 3.45(2) ?
  W2 P1 . 4_566 3.36(2) ?
  W2 O3 . . 2.21(2) ?
  W2 O3 . 4_566 2.21(2) ?
  W2 O4a . . 1.65(3) ?
  W2 O4a . 4_566 1.64(3) ?
  W2 O4b . . 1.96(3) ?
  W2 O4b . 4_566 1.96(3) ?
  W2 O5 . . 2.18(2) ?
  W2 O5 . 4_566 1.87(2) ?
  W2 As2 . 6_556 2.48(2) ?
  W2 As2 . 7_555 2.51(2) ?
  W2 As3 . . 2.79(2) ?
  W2 As3 . 4_566 2.56(2) ?
  W2 As3 . 6_556 3.08(2) ?
  W2 As3 . 7_555 3.35(2) ?
  W2 Ca . 1_565 4.90(2) ?
  W2 Ca . 6_556 3.36(3) ?
  As1 P1 . . 0 ?
  As1 O1 . . 1.654(16) ?
  As1 O2 . . 1.657(14) ?
  As1 O3 . . 1.659(8) ?
  As1 O3 . 7_555 1.659(8) ?
  As1 Ca . 10_554 3.759(9) ?
  As1 Ca . 13_555 3.759(9) ?
  As1 Fe3 . . 3.374(6) ?
  As1 Fe3 . 2_655 3.374(6) ?
  P1 O1 . . 1.654(16) ?
  P1 O2 . . 1.657(14) ?
  P1 O3 . . 1.659(8) ?
  P1 O3 . 7_555 1.659(8) ?
  P1 Ca . 10_554 3.759(9) ?
  P1 Ca . 13_555 3.759(9) ?
  P1 Fe3 . . 3.374(6) ?
  P1 Fe3 . 2_655 3.374(6) ?
  O1 Fe3 . . 1.819(15) ?
  O1 Fe3 . 2_655 1.819(15) ?
  O2 Ca . 10_554 2.744(9) ?
  O2 Ca . 13_555 2.744(9) ?
  O4a O4b . . 0.50(2) ?
  O4a As2 . 6_556 2.092(19) ?
  O4a As2 . 7_555 2.007(19) ?
  O4a As3 . . 2.011(19) ?
  O4a Ca . 6_556 2.76(3) ?
  O4b As2 . 6_556 1.74(2) ?
  O4b As2 . 7_555 1.648(19) ?
  O4b As3 . . 2.08(2) ?
  O4b Ca . 6_556 2.32(3) ?
  O5 As3 . . 1.881(13) ?
  O5 As3 . 7_555 1.881(13) ?
  As2 As2 . 4_556 0.474(10) ?
  As2 As2 . 7_555 3.334(10) ?
  As2 As3 . . 3.143(9) ?
  As2 As3 . 4_556 3.570(9) ?
  As2 As3 . 13_556 3.326(9) ?
  As2 As3 . 6_546 3.036(9) ?
  As2 As3 . 7_555 2.650(9) ?
  As2 Ca . . 0.91(2) ?
  As2 Ca . 6_546 4.015(9) ?
  As2 Ca . 6_556 3.637(9) ?
  As2 O6 . . 1.934(12) ?
  As2 O6 . 4_556 2.406(12) ?
  As3 As3 . 11_556 1.590(9) ?
  As3 As3 . 13_556 1.806(9) ?
  As3 As3 . 7_555 0.857(8) ?
  As3 Ca . . 3.809(15) ?
  As3 Ca . 10_555 4.131(9) ?
  As3 Ca . 13_556 3.725(10) ?
  As3 Ca . 6_556 3.365(17) ?
  As3 O6 . . 1.87(2) ?
  As3 O6 . 11_556 2.207(19) ?
  Ca Ca . 6_546 3.722(3) ?
  Ca Ca . 6_556 3.722(3) ?
  Ca Fe3 . 9_445 4.50(2) ?
  Ca Fe3 . 12_455 4.50(2) ?
  Ca O6 . . 2.278(13) ?
  Ca O6 . 4_556 2.278(13) ?
  Ca Ow2 . 9_445 2.83(3) ?
  Fe3 Fe3 . 2_655 1.650(14) ?
  Fe3 Fe3 . 4_565 3.057(14) ?
  Fe3 Ow1 . . 2.14(4) ?
  Fe3 Ow2 . . 2.070(17) ?
  Fe3 Ow2 . 5_665 2.070(17) ?
  Ow1 Ow6 . 9_554 2.06(3) ?
  Ow1 Ow6 . 10_564 2.06(3) ?
  Ow3 Ow4 . . 2.11(9) ?
  Ow3 Ow6 . . 0.89(7) ?
  Ow4 Ow6 . . 1.36(6) ?
  Ow5 Ow5 . 4_555 1.3(2) ?

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_2
 _geom_angle_site_symmetry_3
 _geom_angle
 _geom_angle_publ_flag
  Fe2 Fe1 Fe2 . . 10_564 120.97(12) ?
  Fe2 Fe1 Fe2 . . 13_555 180.0(5) ?
  Fe2 Fe1 Fe2 . . 6_546 59.03(12) ?
  Fe2 Fe1 W2 . . . 6.7(4) ?
  Fe2 Fe1 W2 . . 10_564 121.0(3) ?
  Fe2 Fe1 W2 . . 11_555 116.4(3) ?
  Fe2 Fe1 W2 . . 4_566 6.2(4) ?
  Fe2 Fe1 W2 . . 13_555 173.3(4) ?
  Fe2 Fe1 W2 . . 6_546 59.0(3) ?
  Fe2 Fe1 W2 . . 7_555 63.6(3) ?
  Fe2 Fe1 W2 . . 16_544 173.8(4) ?
  Fe2 Fe1 As1 . . . 53.4(2) ?
  Fe2 Fe1 As1 . . 11_555 126.6(2) ?
  Fe2 Fe1 P1 . . . 53.4(2) ?
  Fe2 Fe1 P1 . . 11_555 126.6(2) ?
  Fe2 Fe1 O2 . . . 72.2(4) ?
  Fe2 Fe1 O2 . . 11_555 107.8(4) ?
  Fe2 Fe1 O4a . . 10_564 105.6(5) ?
  Fe2 Fe1 O4a . . 4_566 17.6(5) ?
  Fe2 Fe1 O4a . . 6_546 74.4(5) ?
  Fe2 Fe1 O4a . . 16_544 162.4(5) ?
  Fe2 Fe1 O4b . . 10_564 99.4(5) ?
  Fe2 Fe1 O4b . . 4_566 29.8(5) ?
  Fe2 Fe1 O4b . . 6_546 80.6(5) ?
  Fe2 Fe1 O4b . . 16_544 150.2(5) ?
  Fe2 Fe1 As2 . . . 80.07(15) ?
  Fe2 Fe1 As2 . . 10_554 131.8(3) ?
  Fe2 Fe1 As2 . . 11_555 131.8(3) ?
  Fe2 Fe1 As2 . . 4_556 86.64(14) ?
  Fe2 Fe1 As2 . . 13_555 99.93(15) ?
  Fe2 Fe1 As2 . . 6_556 48.2(3) ?
  Fe2 Fe1 As2 . . 7_555 48.2(3) ?
  Fe2 Fe1 As2 . . 16_554 93.36(14) ?
  Fe2 Fe1 As3 . . 10_564 74.04(14) ?
  Fe2 Fe1 As3 . . 4_566 46.94(13) ?
  Fe2 Fe1 As3 . . 6_546 105.96(14) ?
  Fe2 Fe1 As3 . . 16_544 133.06(13) ?
  Fe2 Fe1 Ca . . . 91.3(2) ?
  Fe2 Fe1 Ca . . 10_554 118.6(4) ?
  Fe2 Fe1 Ca . . 13_555 88.7(2) ?
  Fe2 Fe1 Ca . . 6_556 61.4(4) ?
  Fe2 Fe1 Fe2 10_564 . 13_555 59.03(12) ?
  Fe2 Fe1 Fe2 10_564 . 6_546 180.0(5) ?
  Fe2 Fe1 W2 10_564 . . 116.4(3) ?
  Fe2 Fe1 W2 10_564 . 10_564 6.2(4) ?
  Fe2 Fe1 W2 10_564 . 11_555 6.7(4) ?
  Fe2 Fe1 W2 10_564 . 4_566 121.0(3) ?
  Fe2 Fe1 W2 10_564 . 13_555 63.6(3) ?
  Fe2 Fe1 W2 10_564 . 6_546 173.8(4) ?
  Fe2 Fe1 W2 10_564 . 7_555 173.3(4) ?
  Fe2 Fe1 W2 10_564 . 16_544 59.0(3) ?
  Fe2 Fe1 As1 10_564 . . 126.6(2) ?
  Fe2 Fe1 As1 10_564 . 11_555 53.4(2) ?
  Fe2 Fe1 P1 10_564 . . 126.6(2) ?
  Fe2 Fe1 P1 10_564 . 11_555 53.4(2) ?
  Fe2 Fe1 O2 10_564 . . 107.8(4) ?
  Fe2 Fe1 O2 10_564 . 11_555 72.2(4) ?
  Fe2 Fe1 O4a 10_564 . 10_564 17.6(5) ?
  Fe2 Fe1 O4a 10_564 . 4_566 105.6(5) ?
  Fe2 Fe1 O4a 10_564 . 6_546 162.4(5) ?
  Fe2 Fe1 O4a 10_564 . 16_544 74.4(5) ?
  Fe2 Fe1 O4b 10_564 . 10_564 29.8(5) ?
  Fe2 Fe1 O4b 10_564 . 4_566 99.4(5) ?
  Fe2 Fe1 O4b 10_564 . 6_546 150.2(5) ?
  Fe2 Fe1 O4b 10_564 . 16_544 80.6(5) ?
  Fe2 Fe1 As2 10_564 . . 131.8(3) ?
  Fe2 Fe1 As2 10_564 . 10_554 86.64(14) ?
  Fe2 Fe1 As2 10_564 . 11_555 80.07(15) ?
  Fe2 Fe1 As2 10_564 . 4_556 131.8(3) ?
  Fe2 Fe1 As2 10_564 . 13_555 48.2(3) ?
  Fe2 Fe1 As2 10_564 . 6_556 93.36(14) ?
  Fe2 Fe1 As2 10_564 . 7_555 99.93(15) ?
  Fe2 Fe1 As2 10_564 . 16_554 48.2(3) ?
  Fe2 Fe1 As3 10_564 . 10_564 46.94(13) ?
  Fe2 Fe1 As3 10_564 . 4_566 74.04(14) ?
  Fe2 Fe1 As3 10_564 . 6_546 133.06(13) ?
  Fe2 Fe1 As3 10_564 . 16_544 105.96(14) ?
  Fe2 Fe1 Ca 10_564 . . 118.6(4) ?
  Fe2 Fe1 Ca 10_564 . 10_554 91.3(2) ?
  Fe2 Fe1 Ca 10_564 . 13_555 61.4(4) ?
  Fe2 Fe1 Ca 10_564 . 6_556 88.7(2) ?
  Fe2 Fe1 Fe2 13_555 . 6_546 120.97(12) ?
  Fe2 Fe1 W2 13_555 . . 173.3(4) ?
  Fe2 Fe1 W2 13_555 . 10_564 59.0(3) ?
  Fe2 Fe1 W2 13_555 . 11_555 63.6(3) ?
  Fe2 Fe1 W2 13_555 . 4_566 173.8(4) ?
  Fe2 Fe1 W2 13_555 . 13_555 6.7(4) ?
  Fe2 Fe1 W2 13_555 . 6_546 121.0(3) ?
  Fe2 Fe1 W2 13_555 . 7_555 116.4(3) ?
  Fe2 Fe1 W2 13_555 . 16_544 6.2(4) ?
  Fe2 Fe1 As1 13_555 . . 126.6(2) ?
  Fe2 Fe1 As1 13_555 . 11_555 53.4(2) ?
  Fe2 Fe1 P1 13_555 . . 126.6(2) ?
  Fe2 Fe1 P1 13_555 . 11_555 53.4(2) ?
  Fe2 Fe1 O2 13_555 . . 107.8(4) ?
  Fe2 Fe1 O2 13_555 . 11_555 72.2(4) ?
  Fe2 Fe1 O4a 13_555 . 10_564 74.4(5) ?
  Fe2 Fe1 O4a 13_555 . 4_566 162.4(5) ?
  Fe2 Fe1 O4a 13_555 . 6_546 105.6(5) ?
  Fe2 Fe1 O4a 13_555 . 16_544 17.6(5) ?
  Fe2 Fe1 O4b 13_555 . 10_564 80.6(5) ?
  Fe2 Fe1 O4b 13_555 . 4_566 150.2(5) ?
  Fe2 Fe1 O4b 13_555 . 6_546 99.4(5) ?
  Fe2 Fe1 O4b 13_555 . 16_544 29.8(5) ?
  Fe2 Fe1 As2 13_555 . . 99.93(15) ?
  Fe2 Fe1 As2 13_555 . 10_554 48.2(3) ?
  Fe2 Fe1 As2 13_555 . 11_555 48.2(3) ?
  Fe2 Fe1 As2 13_555 . 4_556 93.36(14) ?
  Fe2 Fe1 As2 13_555 . 13_555 80.07(15) ?
  Fe2 Fe1 As2 13_555 . 6_556 131.8(3) ?
  Fe2 Fe1 As2 13_555 . 7_555 131.8(3) ?
  Fe2 Fe1 As2 13_555 . 16_554 86.64(14) ?
  Fe2 Fe1 As3 13_555 . 10_564 105.96(14) ?
  Fe2 Fe1 As3 13_555 . 4_566 133.06(13) ?
  Fe2 Fe1 As3 13_555 . 6_546 74.04(14) ?
  Fe2 Fe1 As3 13_555 . 16_544 46.94(13) ?
  Fe2 Fe1 Ca 13_555 . . 88.7(2) ?
  Fe2 Fe1 Ca 13_555 . 10_554 61.4(4) ?
  Fe2 Fe1 Ca 13_555 . 13_555 91.3(2) ?
  Fe2 Fe1 Ca 13_555 . 6_556 118.6(4) ?
  Fe2 Fe1 W2 6_546 . . 63.6(3) ?
  Fe2 Fe1 W2 6_546 . 10_564 173.8(4) ?
  Fe2 Fe1 W2 6_546 . 11_555 173.3(4) ?
  Fe2 Fe1 W2 6_546 . 4_566 59.0(3) ?
  Fe2 Fe1 W2 6_546 . 13_555 116.4(3) ?
  Fe2 Fe1 W2 6_546 . 6_546 6.2(4) ?
  Fe2 Fe1 W2 6_546 . 7_555 6.7(4) ?
  Fe2 Fe1 W2 6_546 . 16_544 121.0(3) ?
  Fe2 Fe1 As1 6_546 . . 53.4(2) ?
  Fe2 Fe1 As1 6_546 . 11_555 126.6(2) ?
  Fe2 Fe1 P1 6_546 . . 53.4(2) ?
  Fe2 Fe1 P1 6_546 . 11_555 126.6(2) ?
  Fe2 Fe1 O2 6_546 . . 72.2(4) ?
  Fe2 Fe1 O2 6_546 . 11_555 107.8(4) ?
  Fe2 Fe1 O4a 6_546 . 10_564 162.4(5) ?
  Fe2 Fe1 O4a 6_546 . 4_566 74.4(5) ?
  Fe2 Fe1 O4a 6_546 . 6_546 17.6(5) ?
  Fe2 Fe1 O4a 6_546 . 16_544 105.6(5) ?
  Fe2 Fe1 O4b 6_546 . 10_564 150.2(5) ?
  Fe2 Fe1 O4b 6_546 . 4_566 80.6(5) ?
  Fe2 Fe1 O4b 6_546 . 6_546 29.8(5) ?
  Fe2 Fe1 O4b 6_546 . 16_544 99.4(5) ?
  Fe2 Fe1 As2 6_546 . . 48.2(3) ?
  Fe2 Fe1 As2 6_546 . 10_554 93.36(14) ?
  Fe2 Fe1 As2 6_546 . 11_555 99.93(15) ?
  Fe2 Fe1 As2 6_546 . 4_556 48.2(3) ?
  Fe2 Fe1 As2 6_546 . 13_555 131.8(3) ?
  Fe2 Fe1 As2 6_546 . 6_556 86.64(14) ?
  Fe2 Fe1 As2 6_546 . 7_555 80.07(15) ?
  Fe2 Fe1 As2 6_546 . 16_554 131.8(3) ?
  Fe2 Fe1 As3 6_546 . 10_564 133.06(13) ?
  Fe2 Fe1 As3 6_546 . 4_566 105.96(14) ?
  Fe2 Fe1 As3 6_546 . 6_546 46.94(13) ?
  Fe2 Fe1 As3 6_546 . 16_544 74.04(14) ?
  Fe2 Fe1 Ca 6_546 . . 61.4(4) ?
  Fe2 Fe1 Ca 6_546 . 10_554 88.7(2) ?
  Fe2 Fe1 Ca 6_546 . 13_555 118.6(4) ?
  Fe2 Fe1 Ca 6_546 . 6_556 91.3(2) ?
  W2 Fe1 W2 . . 10_564 117.0(5) ?
  W2 Fe1 W2 . . 11_555 112.3(5) ?
  W2 Fe1 W2 . . 4_566 4.8(5) ?
  W2 Fe1 W2 . . 13_555 180.0(5) ?
  W2 Fe1 W2 . . 6_546 63.0(5) ?
  W2 Fe1 W2 . . 7_555 67.7(5) ?
  W2 Fe1 W2 . . 16_544 175.2(5) ?
  W2 Fe1 As1 . . . 59.9(3) ?
  W2 Fe1 As1 . . 11_555 120.1(3) ?
  W2 Fe1 P1 . . . 59.9(3) ?
  W2 Fe1 P1 . . 11_555 120.1(3) ?
  W2 Fe1 O2 . . . 78.0(4) ?
  W2 Fe1 O2 . . 11_555 102.0(4) ?
  W2 Fe1 O4a . . 10_564 101.9(6) ?
  W2 Fe1 O4a . . 4_566 11.3(6) ?
  W2 Fe1 O4a . . 6_546 78.1(6) ?
  W2 Fe1 O4a . . 16_544 168.7(6) ?
  W2 Fe1 O4b . . 10_564 97.1(6) ?
  W2 Fe1 O4b . . 4_566 23.1(6) ?
  W2 Fe1 O4b . . 6_546 82.9(6) ?
  W2 Fe1 O4b . . 16_544 156.9(6) ?
  W2 Fe1 As2 . . . 79.5(4) ?
  W2 Fe1 As2 . . 10_554 138.3(3) ?
  W2 Fe1 As2 . . 11_555 137.7(3) ?
  W2 Fe1 As2 . . 4_556 86.6(4) ?
  W2 Fe1 As2 . . 13_555 100.5(4) ?
  W2 Fe1 As2 . . 6_556 41.7(3) ?
  W2 Fe1 As2 . . 7_555 42.3(3) ?
  W2 Fe1 As2 . . 16_554 93.4(4) ?
  W2 Fe1 As3 . . 10_564 69.6(3) ?
  W2 Fe1 As3 . . 4_566 42.8(3) ?
  W2 Fe1 As3 . . 6_546 110.4(3) ?
  W2 Fe1 As3 . . 16_544 137.2(3) ?
  W2 Fe1 Ca . . . 89.7(4) ?
  W2 Fe1 Ca . . 10_554 124.9(4) ?
  W2 Fe1 Ca . . 13_555 90.3(4) ?
  W2 Fe1 Ca . . 6_556 55.1(4) ?
  W2 Fe1 W2 10_564 . 11_555 4.8(5) ?
  W2 Fe1 W2 10_564 . 4_566 121.8(5) ?
  W2 Fe1 W2 10_564 . 13_555 63.0(5) ?
  W2 Fe1 W2 10_564 . 6_546 180.0(5) ?
  W2 Fe1 W2 10_564 . 7_555 175.2(5) ?
  W2 Fe1 W2 10_564 . 16_544 58.2(5) ?
  W2 Fe1 As1 10_564 . . 121.0(3) ?
  W2 Fe1 As1 10_564 . 11_555 59.0(3) ?
  W2 Fe1 P1 10_564 . . 121.0(3) ?
  W2 Fe1 P1 10_564 . 11_555 59.0(3) ?
  W2 Fe1 O2 10_564 . . 101.7(5) ?
  W2 Fe1 O2 10_564 . 11_555 78.3(5) ?
  W2 Fe1 O4a 10_564 . 10_564 15.5(6) ?
  W2 Fe1 O4a 10_564 . 4_566 106.7(6) ?
  W2 Fe1 O4a 10_564 . 6_546 164.5(6) ?
  W2 Fe1 O4a 10_564 . 16_544 73.3(6) ?
  W2 Fe1 O4b 10_564 . 10_564 25.7(6) ?
  W2 Fe1 O4b 10_564 . 4_566 101.9(6) ?
  W2 Fe1 O4b 10_564 . 6_546 154.3(6) ?
  W2 Fe1 O4b 10_564 . 16_544 78.1(6) ?
  W2 Fe1 As2 10_564 . . 137.7(4) ?
  W2 Fe1 As2 10_564 . 10_554 82.3(4) ?
  W2 Fe1 As2 10_564 . 11_555 75.4(4) ?
  W2 Fe1 As2 10_564 . 4_556 137.2(3) ?
  W2 Fe1 As2 10_564 . 13_555 42.3(4) ?
  W2 Fe1 As2 10_564 . 6_556 97.7(4) ?
  W2 Fe1 As2 10_564 . 7_555 104.6(4) ?
  W2 Fe1 As2 10_564 . 16_554 42.8(3) ?
  W2 Fe1 As3 10_564 . 10_564 47.6(3) ?
  W2 Fe1 As3 10_564 . 4_566 74.3(3) ?
  W2 Fe1 As3 10_564 . 6_546 132.4(3) ?
  W2 Fe1 As3 10_564 . 16_544 105.7(3) ?
  W2 Fe1 Ca 10_564 . . 124.3(4) ?
  W2 Fe1 Ca 10_564 . 10_554 86.1(4) ?
  W2 Fe1 Ca 10_564 . 13_555 55.7(4) ?
  W2 Fe1 Ca 10_564 . 6_556 93.9(4) ?
  W2 Fe1 W2 11_555 . 4_566 117.0(5) ?
  W2 Fe1 W2 11_555 . 13_555 67.7(5) ?
  W2 Fe1 W2 11_555 . 6_546 175.2(5) ?
  W2 Fe1 W2 11_555 . 7_555 180.0(5) ?
  W2 Fe1 W2 11_555 . 16_544 63.0(5) ?
  W2 Fe1 As1 11_555 . . 120.1(3) ?
  W2 Fe1 As1 11_555 . 11_555 59.9(3) ?
  W2 Fe1 P1 11_555 . . 120.1(3) ?
  W2 Fe1 P1 11_555 . 11_555 59.9(3) ?
  W2 Fe1 O2 11_555 . . 102.0(4) ?
  W2 Fe1 O2 11_555 . 11_555 78.0(4) ?
  W2 Fe1 O4a 11_555 . 10_564 11.3(6) ?
  W2 Fe1 O4a 11_555 . 4_566 101.9(6) ?
  W2 Fe1 O4a 11_555 . 6_546 168.7(6) ?
  W2 Fe1 O4a 11_555 . 16_544 78.1(6) ?
  W2 Fe1 O4b 11_555 . 10_564 23.1(6) ?
  W2 Fe1 O4b 11_555 . 4_566 97.1(6) ?
  W2 Fe1 O4b 11_555 . 6_546 156.9(6) ?
  W2 Fe1 O4b 11_555 . 16_544 82.9(6) ?
  W2 Fe1 As2 11_555 . . 137.7(3) ?
  W2 Fe1 As2 11_555 . 10_554 86.6(4) ?
  W2 Fe1 As2 11_555 . 11_555 79.5(4) ?
  W2 Fe1 As2 11_555 . 4_556 138.3(3) ?
  W2 Fe1 As2 11_555 . 13_555 42.3(3) ?
  W2 Fe1 As2 11_555 . 6_556 93.4(4) ?
  W2 Fe1 As2 11_555 . 7_555 100.5(4) ?
  W2 Fe1 As2 11_555 . 16_554 41.7(3) ?
  W2 Fe1 As3 11_555 . 10_564 42.8(3) ?
  W2 Fe1 As3 11_555 . 4_566 69.6(3) ?
  W2 Fe1 As3 11_555 . 6_546 137.2(3) ?
  W2 Fe1 As3 11_555 . 16_544 110.4(3) ?
  W2 Fe1 Ca 11_555 . . 124.9(4) ?
  W2 Fe1 Ca 11_555 . 10_554 89.7(4) ?
  W2 Fe1 Ca 11_555 . 13_555 55.1(4) ?
  W2 Fe1 Ca 11_555 . 6_556 90.3(4) ?
  W2 Fe1 W2 4_566 . 13_555 175.2(5) ?
  W2 Fe1 W2 4_566 . 6_546 58.2(5) ?
  W2 Fe1 W2 4_566 . 7_555 63.0(5) ?
  W2 Fe1 W2 4_566 . 16_544 180.0(5) ?
  W2 Fe1 As1 4_566 . . 59.0(3) ?
  W2 Fe1 As1 4_566 . 11_555 121.0(3) ?
  W2 Fe1 P1 4_566 . . 59.0(3) ?
  W2 Fe1 P1 4_566 . 11_555 121.0(3) ?
  W2 Fe1 O2 4_566 . . 78.3(5) ?
  W2 Fe1 O2 4_566 . 11_555 101.7(5) ?
  W2 Fe1 O4a 4_566 . 10_564 106.7(6) ?
  W2 Fe1 O4a 4_566 . 4_566 15.5(6) ?
  W2 Fe1 O4a 4_566 . 6_546 73.3(6) ?
  W2 Fe1 O4a 4_566 . 16_544 164.5(6) ?
  W2 Fe1 O4b 4_566 . 10_564 101.9(6) ?
  W2 Fe1 O4b 4_566 . 4_566 25.7(6) ?
  W2 Fe1 O4b 4_566 . 6_546 78.1(6) ?
  W2 Fe1 O4b 4_566 . 16_544 154.3(6) ?
  W2 Fe1 As2 4_566 . . 75.4(4) ?
  W2 Fe1 As2 4_566 . 10_554 137.2(3) ?
  W2 Fe1 As2 4_566 . 11_555 137.7(4) ?
  W2 Fe1 As2 4_566 . 4_556 82.3(4) ?
  W2 Fe1 As2 4_566 . 13_555 104.6(4) ?
  W2 Fe1 As2 4_566 . 6_556 42.8(3) ?
  W2 Fe1 As2 4_566 . 7_555 42.3(4) ?
  W2 Fe1 As2 4_566 . 16_554 97.7(4) ?
  W2 Fe1 As3 4_566 . 10_564 74.3(3) ?
  W2 Fe1 As3 4_566 . 4_566 47.6(3) ?
  W2 Fe1 As3 4_566 . 6_546 105.7(3) ?
  W2 Fe1 As3 4_566 . 16_544 132.4(3) ?
  W2 Fe1 Ca 4_566 . . 86.1(4) ?
  W2 Fe1 Ca 4_566 . 10_554 124.3(4) ?
  W2 Fe1 Ca 4_566 . 13_555 93.9(4) ?
  W2 Fe1 Ca 4_566 . 6_556 55.7(4) ?
  W2 Fe1 W2 13_555 . 6_546 117.0(5) ?
  W2 Fe1 W2 13_555 . 7_555 112.3(5) ?
  W2 Fe1 W2 13_555 . 16_544 4.8(5) ?
  W2 Fe1 As1 13_555 . . 120.1(3) ?
  W2 Fe1 As1 13_555 . 11_555 59.9(3) ?
  W2 Fe1 P1 13_555 . . 120.1(3) ?
  W2 Fe1 P1 13_555 . 11_555 59.9(3) ?
  W2 Fe1 O2 13_555 . . 102.0(4) ?
  W2 Fe1 O2 13_555 . 11_555 78.0(4) ?
  W2 Fe1 O4a 13_555 . 10_564 78.1(6) ?
  W2 Fe1 O4a 13_555 . 4_566 168.7(6) ?
  W2 Fe1 O4a 13_555 . 6_546 101.9(6) ?
  W2 Fe1 O4a 13_555 . 16_544 11.3(6) ?
  W2 Fe1 O4b 13_555 . 10_564 82.9(6) ?
  W2 Fe1 O4b 13_555 . 4_566 156.9(6) ?
  W2 Fe1 O4b 13_555 . 6_546 97.1(6) ?
  W2 Fe1 O4b 13_555 . 16_544 23.1(6) ?
  W2 Fe1 As2 13_555 . . 100.5(4) ?
  W2 Fe1 As2 13_555 . 10_554 41.7(3) ?
  W2 Fe1 As2 13_555 . 11_555 42.3(3) ?
  W2 Fe1 As2 13_555 . 4_556 93.4(4) ?
  W2 Fe1 As2 13_555 . 13_555 79.5(4) ?
  W2 Fe1 As2 13_555 . 6_556 138.3(3) ?
  W2 Fe1 As2 13_555 . 7_555 137.7(3) ?
  W2 Fe1 As2 13_555 . 16_554 86.6(4) ?
  W2 Fe1 As3 13_555 . 10_564 110.4(3) ?
  W2 Fe1 As3 13_555 . 4_566 137.2(3) ?
  W2 Fe1 As3 13_555 . 6_546 69.6(3) ?
  W2 Fe1 As3 13_555 . 16_544 42.8(3) ?
  W2 Fe1 Ca 13_555 . . 90.3(4) ?
  W2 Fe1 Ca 13_555 . 10_554 55.1(4) ?
  W2 Fe1 Ca 13_555 . 13_555 89.7(4) ?
  W2 Fe1 Ca 13_555 . 6_556 124.9(4) ?
  W2 Fe1 W2 6_546 . 7_555 4.8(5) ?
  W2 Fe1 W2 6_546 . 16_544 121.8(5) ?
  W2 Fe1 As1 6_546 . . 59.0(3) ?
  W2 Fe1 As1 6_546 . 11_555 121.0(3) ?
  W2 Fe1 P1 6_546 . . 59.0(3) ?
  W2 Fe1 P1 6_546 . 11_555 121.0(3) ?
  W2 Fe1 O2 6_546 . . 78.3(5) ?
  W2 Fe1 O2 6_546 . 11_555 101.7(5) ?
  W2 Fe1 O4a 6_546 . 10_564 164.5(6) ?
  W2 Fe1 O4a 6_546 . 4_566 73.3(6) ?
  W2 Fe1 O4a 6_546 . 6_546 15.5(6) ?
  W2 Fe1 O4a 6_546 . 16_544 106.7(6) ?
  W2 Fe1 O4b 6_546 . 10_564 154.3(6) ?
  W2 Fe1 O4b 6_546 . 4_566 78.1(6) ?
  W2 Fe1 O4b 6_546 . 6_546 25.7(6) ?
  W2 Fe1 O4b 6_546 . 16_544 101.9(6) ?
  W2 Fe1 As2 6_546 . . 42.3(4) ?
  W2 Fe1 As2 6_546 . 10_554 97.7(4) ?
  W2 Fe1 As2 6_546 . 11_555 104.6(4) ?
  W2 Fe1 As2 6_546 . 4_556 42.8(3) ?
  W2 Fe1 As2 6_546 . 13_555 137.7(4) ?
  W2 Fe1 As2 6_546 . 6_556 82.3(4) ?
  W2 Fe1 As2 6_546 . 7_555 75.4(4) ?
  W2 Fe1 As2 6_546 . 16_554 137.2(3) ?
  W2 Fe1 As3 6_546 . 10_564 132.4(3) ?
  W2 Fe1 As3 6_546 . 4_566 105.7(3) ?
  W2 Fe1 As3 6_546 . 6_546 47.6(3) ?
  W2 Fe1 As3 6_546 . 16_544 74.3(3) ?
  W2 Fe1 Ca 6_546 . . 55.7(4) ?
  W2 Fe1 Ca 6_546 . 10_554 93.9(4) ?
  W2 Fe1 Ca 6_546 . 13_555 124.3(4) ?
  W2 Fe1 Ca 6_546 . 6_556 86.1(4) ?
  W2 Fe1 W2 7_555 . 16_544 117.0(5) ?
  W2 Fe1 As1 7_555 . . 59.9(3) ?
  W2 Fe1 As1 7_555 . 11_555 120.1(3) ?
  W2 Fe1 P1 7_555 . . 59.9(3) ?
  W2 Fe1 P1 7_555 . 11_555 120.1(3) ?
  W2 Fe1 O2 7_555 . . 78.0(4) ?
  W2 Fe1 O2 7_555 . 11_555 102.0(4) ?
  W2 Fe1 O4a 7_555 . 10_564 168.7(6) ?
  W2 Fe1 O4a 7_555 . 4_566 78.1(6) ?
  W2 Fe1 O4a 7_555 . 6_546 11.3(6) ?
  W2 Fe1 O4a 7_555 . 16_544 101.9(6) ?
  W2 Fe1 O4b 7_555 . 10_564 156.9(6) ?
  W2 Fe1 O4b 7_555 . 4_566 82.9(6) ?
  W2 Fe1 O4b 7_555 . 6_546 23.1(6) ?
  W2 Fe1 O4b 7_555 . 16_544 97.1(6) ?
  W2 Fe1 As2 7_555 . . 42.3(3) ?
  W2 Fe1 As2 7_555 . 10_554 93.4(4) ?
  W2 Fe1 As2 7_555 . 11_555 100.5(4) ?
  W2 Fe1 As2 7_555 . 4_556 41.7(3) ?
  W2 Fe1 As2 7_555 . 13_555 137.7(3) ?
  W2 Fe1 As2 7_555 . 6_556 86.6(4) ?
  W2 Fe1 As2 7_555 . 7_555 79.5(4) ?
  W2 Fe1 As2 7_555 . 16_554 138.3(3) ?
  W2 Fe1 As3 7_555 . 10_564 137.2(3) ?
  W2 Fe1 As3 7_555 . 4_566 110.4(3) ?
  W2 Fe1 As3 7_555 . 6_546 42.8(3) ?
  W2 Fe1 As3 7_555 . 16_544 69.6(3) ?
  W2 Fe1 Ca 7_555 . . 55.1(4) ?
  W2 Fe1 Ca 7_555 . 10_554 90.3(4) ?
  W2 Fe1 Ca 7_555 . 13_555 124.9(4) ?
  W2 Fe1 Ca 7_555 . 6_556 89.7(4) ?
  W2 Fe1 As1 16_544 . . 121.0(3) ?
  W2 Fe1 As1 16_544 . 11_555 59.0(3) ?
  W2 Fe1 P1 16_544 . . 121.0(3) ?
  W2 Fe1 P1 16_544 . 11_555 59.0(3) ?
  W2 Fe1 O2 16_544 . . 101.7(5) ?
  W2 Fe1 O2 16_544 . 11_555 78.3(5) ?
  W2 Fe1 O4a 16_544 . 10_564 73.3(6) ?
  W2 Fe1 O4a 16_544 . 4_566 164.5(6) ?
  W2 Fe1 O4a 16_544 . 6_546 106.7(6) ?
  W2 Fe1 O4a 16_544 . 16_544 15.5(6) ?
  W2 Fe1 O4b 16_544 . 10_564 78.1(6) ?
  W2 Fe1 O4b 16_544 . 4_566 154.3(6) ?
  W2 Fe1 O4b 16_544 . 6_546 101.9(6) ?
  W2 Fe1 O4b 16_544 . 16_544 25.7(6) ?
  W2 Fe1 As2 16_544 . . 104.6(4) ?
  W2 Fe1 As2 16_544 . 10_554 42.8(3) ?
  W2 Fe1 As2 16_544 . 11_555 42.3(4) ?
  W2 Fe1 As2 16_544 . 4_556 97.7(4) ?
  W2 Fe1 As2 16_544 . 13_555 75.4(4) ?
  W2 Fe1 As2 16_544 . 6_556 137.2(3) ?
  W2 Fe1 As2 16_544 . 7_555 137.7(4) ?
  W2 Fe1 As2 16_544 . 16_554 82.3(4) ?
  W2 Fe1 As3 16_544 . 10_564 105.7(3) ?
  W2 Fe1 As3 16_544 . 4_566 132.4(3) ?
  W2 Fe1 As3 16_544 . 6_546 74.3(3) ?
  W2 Fe1 As3 16_544 . 16_544 47.6(3) ?
  W2 Fe1 Ca 16_544 . . 93.9(4) ?
  W2 Fe1 Ca 16_544 . 10_554 55.7(4) ?
  W2 Fe1 Ca 16_544 . 13_555 86.1(4) ?
  W2 Fe1 Ca 16_544 . 6_556 124.3(4) ?
  As1 Fe1 As1 . . 11_555 180.0(5) ?
  As1 Fe1 P1 . . . 0.0(5) ?
  As1 Fe1 P1 . . 11_555 180.0(5) ?
  As1 Fe1 O2 . . . 22.7(4) ?
  As1 Fe1 O2 . . 11_555 157.3(4) ?
  As1 Fe1 O4a . . 10_564 111.6(5) ?
  As1 Fe1 O4a . . 4_566 68.4(5) ?
  As1 Fe1 O4a . . 6_546 68.4(5) ?
  As1 Fe1 O4a . . 16_544 111.6(5) ?
  As1 Fe1 O4b . . 10_564 97.7(5) ?
  As1 Fe1 O4b . . 4_566 82.3(5) ?
  As1 Fe1 O4b . . 6_546 82.3(5) ?
  As1 Fe1 O4b . . 16_544 97.7(5) ?
  As1 Fe1 As2 . . . 101.15(12) ?
  As1 Fe1 As2 . . 10_554 78.42(12) ?
  As1 Fe1 As2 . . 11_555 78.85(12) ?
  As1 Fe1 As2 . . 4_556 101.58(12) ?
  As1 Fe1 As2 . . 13_555 78.85(12) ?
  As1 Fe1 As2 . . 6_556 101.58(12) ?
  As1 Fe1 As2 . . 7_555 101.15(12) ?
  As1 Fe1 As2 . . 16_554 78.42(12) ?
  As1 Fe1 As3 . . 10_564 99.76(12) ?
  As1 Fe1 As3 . . 4_566 80.24(12) ?
  As1 Fe1 As3 . . 6_546 80.24(12) ?
  As1 Fe1 As3 . . 16_544 99.76(12) ?
  As1 Fe1 Ca . . . 114.7(3) ?
  As1 Fe1 Ca . . 10_554 65.3(3) ?
  As1 Fe1 Ca . . 13_555 65.3(3) ?
  As1 Fe1 Ca . . 6_556 114.7(3) ?
  As1 Fe1 P1 11_555 . . 180.0(5) ?
  As1 Fe1 P1 11_555 . 11_555 0.0(5) ?
  As1 Fe1 O2 11_555 . . 157.3(4) ?
  As1 Fe1 O2 11_555 . 11_555 22.7(4) ?
  As1 Fe1 O4a 11_555 . 10_564 68.4(5) ?
  As1 Fe1 O4a 11_555 . 4_566 111.6(5) ?
  As1 Fe1 O4a 11_555 . 6_546 111.6(5) ?
  As1 Fe1 O4a 11_555 . 16_544 68.4(5) ?
  As1 Fe1 O4b 11_555 . 10_564 82.3(5) ?
  As1 Fe1 O4b 11_555 . 4_566 97.7(5) ?
  As1 Fe1 O4b 11_555 . 6_546 97.7(5) ?
  As1 Fe1 O4b 11_555 . 16_544 82.3(5) ?
  As1 Fe1 As2 11_555 . . 78.85(12) ?
  As1 Fe1 As2 11_555 . 10_554 101.58(12) ?
  As1 Fe1 As2 11_555 . 11_555 101.15(12) ?
  As1 Fe1 As2 11_555 . 4_556 78.42(12) ?
  As1 Fe1 As2 11_555 . 13_555 101.15(12) ?
  As1 Fe1 As2 11_555 . 6_556 78.42(12) ?
  As1 Fe1 As2 11_555 . 7_555 78.85(12) ?
  As1 Fe1 As2 11_555 . 16_554 101.58(12) ?
  As1 Fe1 As3 11_555 . 10_564 80.24(12) ?
  As1 Fe1 As3 11_555 . 4_566 99.76(12) ?
  As1 Fe1 As3 11_555 . 6_546 99.76(12) ?
  As1 Fe1 As3 11_555 . 16_544 80.24(12) ?
  As1 Fe1 Ca 11_555 . . 65.3(3) ?
  As1 Fe1 Ca 11_555 . 10_554 114.7(3) ?
  As1 Fe1 Ca 11_555 . 13_555 114.7(3) ?
  As1 Fe1 Ca 11_555 . 6_556 65.3(3) ?
  P1 Fe1 P1 . . 11_555 180.0(5) ?
  P1 Fe1 O2 . . . 22.7(4) ?
  P1 Fe1 O2 . . 11_555 157.3(4) ?
  P1 Fe1 O4a . . 10_564 111.6(5) ?
  P1 Fe1 O4a . . 4_566 68.4(5) ?
  P1 Fe1 O4a . . 6_546 68.4(5) ?
  P1 Fe1 O4a . . 16_544 111.6(5) ?
  P1 Fe1 O4b . . 10_564 97.7(5) ?
  P1 Fe1 O4b . . 4_566 82.3(5) ?
  P1 Fe1 O4b . . 6_546 82.3(5) ?
  P1 Fe1 O4b . . 16_544 97.7(5) ?
  P1 Fe1 As2 . . . 101.15(12) ?
  P1 Fe1 As2 . . 10_554 78.42(12) ?
  P1 Fe1 As2 . . 11_555 78.85(12) ?
  P1 Fe1 As2 . . 4_556 101.58(12) ?
  P1 Fe1 As2 . . 13_555 78.85(12) ?
  P1 Fe1 As2 . . 6_556 101.58(12) ?
  P1 Fe1 As2 . . 7_555 101.15(12) ?
  P1 Fe1 As2 . . 16_554 78.42(12) ?
  P1 Fe1 As3 . . 10_564 99.76(12) ?
  P1 Fe1 As3 . . 4_566 80.24(12) ?
  P1 Fe1 As3 . . 6_546 80.24(12) ?
  P1 Fe1 As3 . . 16_544 99.76(12) ?
  P1 Fe1 Ca . . . 114.7(3) ?
  P1 Fe1 Ca . . 10_554 65.3(3) ?
  P1 Fe1 Ca . . 13_555 65.3(3) ?
  P1 Fe1 Ca . . 6_556 114.7(3) ?
  P1 Fe1 O2 11_555 . . 157.3(4) ?
  P1 Fe1 O2 11_555 . 11_555 22.7(4) ?
  P1 Fe1 O4a 11_555 . 10_564 68.4(5) ?
  P1 Fe1 O4a 11_555 . 4_566 111.6(5) ?
  P1 Fe1 O4a 11_555 . 6_546 111.6(5) ?
  P1 Fe1 O4a 11_555 . 16_544 68.4(5) ?
  P1 Fe1 O4b 11_555 . 10_564 82.3(5) ?
  P1 Fe1 O4b 11_555 . 4_566 97.7(5) ?
  P1 Fe1 O4b 11_555 . 6_546 97.7(5) ?
  P1 Fe1 O4b 11_555 . 16_544 82.3(5) ?
  P1 Fe1 As2 11_555 . . 78.85(12) ?
  P1 Fe1 As2 11_555 . 10_554 101.58(12) ?
  P1 Fe1 As2 11_555 . 11_555 101.15(12) ?
  P1 Fe1 As2 11_555 . 4_556 78.42(12) ?
  P1 Fe1 As2 11_555 . 13_555 101.15(12) ?
  P1 Fe1 As2 11_555 . 6_556 78.42(12) ?
  P1 Fe1 As2 11_555 . 7_555 78.85(12) ?
  P1 Fe1 As2 11_555 . 16_554 101.58(12) ?
  P1 Fe1 As3 11_555 . 10_564 80.24(12) ?
  P1 Fe1 As3 11_555 . 4_566 99.76(12) ?
  P1 Fe1 As3 11_555 . 6_546 99.76(12) ?
  P1 Fe1 As3 11_555 . 16_544 80.24(12) ?
  P1 Fe1 Ca 11_555 . . 65.3(3) ?
  P1 Fe1 Ca 11_555 . 10_554 114.7(3) ?
  P1 Fe1 Ca 11_555 . 13_555 114.7(3) ?
  P1 Fe1 Ca 11_555 . 6_556 65.3(3) ?
  O2 Fe1 O2 . . 11_555 180.0(5) ?
  O2 Fe1 O4a . . 10_564 95.7(6) ?
  O2 Fe1 O4a . . 4_566 84.3(6) ?
  O2 Fe1 O4a . . 6_546 84.3(6) ?
  O2 Fe1 O4a . . 16_544 95.7(6) ?
  O2 Fe1 O4b . . 10_564 81.9(6) ?
  O2 Fe1 O4b . . 4_566 98.1(6) ?
  O2 Fe1 O4b . . 6_546 98.1(6) ?
  O2 Fe1 O4b . . 16_544 81.9(6) ?
  O2 Fe1 As2 . . . 120.3(3) ?
  O2 Fe1 As2 . . 10_554 61.4(3) ?
  O2 Fe1 As2 . . 11_555 59.7(3) ?
  O2 Fe1 As2 . . 4_556 118.6(3) ?
  O2 Fe1 As2 . . 13_555 59.7(3) ?
  O2 Fe1 As2 . . 6_556 118.6(3) ?
  O2 Fe1 As2 . . 7_555 120.3(3) ?
  O2 Fe1 As2 . . 16_554 61.4(3) ?
  O2 Fe1 As3 . . 10_564 95.37(14) ?
  O2 Fe1 As3 . . 4_566 84.63(14) ?
  O2 Fe1 As3 . . 6_546 84.63(14) ?
  O2 Fe1 As3 . . 16_544 95.37(14) ?
  O2 Fe1 Ca . . . 132.5(4) ?
  O2 Fe1 Ca . . 10_554 47.5(4) ?
  O2 Fe1 Ca . . 13_555 47.5(4) ?
  O2 Fe1 Ca . . 6_556 132.5(4) ?
  O2 Fe1 O4a 11_555 . 10_564 84.3(6) ?
  O2 Fe1 O4a 11_555 . 4_566 95.7(6) ?
  O2 Fe1 O4a 11_555 . 6_546 95.7(6) ?
  O2 Fe1 O4a 11_555 . 16_544 84.3(6) ?
  O2 Fe1 O4b 11_555 . 10_564 98.1(6) ?
  O2 Fe1 O4b 11_555 . 4_566 81.9(6) ?
  O2 Fe1 O4b 11_555 . 6_546 81.9(6) ?
  O2 Fe1 O4b 11_555 . 16_544 98.1(6) ?
  O2 Fe1 As2 11_555 . . 59.7(3) ?
  O2 Fe1 As2 11_555 . 10_554 118.6(3) ?
  O2 Fe1 As2 11_555 . 11_555 120.3(3) ?
  O2 Fe1 As2 11_555 . 4_556 61.4(3) ?
  O2 Fe1 As2 11_555 . 13_555 120.3(3) ?
  O2 Fe1 As2 11_555 . 6_556 61.4(3) ?
  O2 Fe1 As2 11_555 . 7_555 59.7(3) ?
  O2 Fe1 As2 11_555 . 16_554 118.6(3) ?
  O2 Fe1 As3 11_555 . 10_564 84.63(14) ?
  O2 Fe1 As3 11_555 . 4_566 95.37(14) ?
  O2 Fe1 As3 11_555 . 6_546 95.37(14) ?
  O2 Fe1 As3 11_555 . 16_544 84.63(14) ?
  O2 Fe1 Ca 11_555 . . 47.5(4) ?
  O2 Fe1 Ca 11_555 . 10_554 132.5(4) ?
  O2 Fe1 Ca 11_555 . 13_555 132.5(4) ?
  O2 Fe1 Ca 11_555 . 6_556 47.5(4) ?
  O4a Fe1 O4a 10_564 . 4_566 92.0(7) ?
  O4a Fe1 O4a 10_564 . 6_546 180.0(5) ?
  O4a Fe1 O4a 10_564 . 16_544 88.0(7) ?
  O4a Fe1 O4b 10_564 . 10_564 14.0(7) ?
  O4a Fe1 O4b 10_564 . 4_566 88.7(7) ?
  O4a Fe1 O4b 10_564 . 6_546 166.0(7) ?
  O4a Fe1 O4b 10_564 . 16_544 91.3(7) ?
  O4a Fe1 As2 10_564 . . 143.0(5) ?
  O4a Fe1 As2 10_564 . 10_554 91.8(5) ?
  O4a Fe1 As2 10_564 . 11_555 84.1(5) ?
  O4a Fe1 As2 10_564 . 4_556 145.6(5) ?
  O4a Fe1 As2 10_564 . 13_555 37.0(5) ?
  O4a Fe1 As2 10_564 . 6_556 88.2(5) ?
  O4a Fe1 As2 10_564 . 7_555 95.9(5) ?
  O4a Fe1 As2 10_564 . 16_554 34.4(5) ?
  O4a Fe1 As3 10_564 . 10_564 33.1(5) ?
  O4a Fe1 As3 10_564 . 4_566 59.2(5) ?
  O4a Fe1 As3 10_564 . 6_546 146.9(5) ?
  O4a Fe1 As3 10_564 . 16_544 120.8(5) ?
  O4a Fe1 Ca 10_564 . . 131.7(6) ?
  O4a Fe1 Ca 10_564 . 10_554 92.4(5) ?
  O4a Fe1 Ca 10_564 . 13_555 48.3(6) ?
  O4a Fe1 Ca 10_564 . 6_556 87.6(5) ?
  O4a Fe1 O4a 4_566 . 6_546 88.0(7) ?
  O4a Fe1 O4a 4_566 . 16_544 180.0(5) ?
  O4a Fe1 O4b 4_566 . 10_564 88.7(7) ?
  O4a Fe1 O4b 4_566 . 4_566 14.0(7) ?
  O4a Fe1 O4b 4_566 . 6_546 91.3(7) ?
  O4a Fe1 O4b 4_566 . 16_544 166.0(7) ?
  O4a Fe1 As2 4_566 . . 84.1(5) ?
  O4a Fe1 As2 4_566 . 10_554 145.6(5) ?
  O4a Fe1 As2 4_566 . 11_555 143.0(5) ?
  O4a Fe1 As2 4_566 . 4_556 91.8(5) ?
  O4a Fe1 As2 4_566 . 13_555 95.9(5) ?
  O4a Fe1 As2 4_566 . 6_556 34.4(5) ?
  O4a Fe1 As2 4_566 . 7_555 37.0(5) ?
  O4a Fe1 As2 4_566 . 16_554 88.2(5) ?
  O4a Fe1 As3 4_566 . 10_564 59.2(5) ?
  O4a Fe1 As3 4_566 . 4_566 33.1(5) ?
  O4a Fe1 As3 4_566 . 6_546 120.8(5) ?
  O4a Fe1 As3 4_566 . 16_544 146.9(5) ?
  O4a Fe1 Ca 4_566 . . 92.4(5) ?
  O4a Fe1 Ca 4_566 . 10_554 131.7(6) ?
  O4a Fe1 Ca 4_566 . 13_555 87.6(5) ?
  O4a Fe1 Ca 4_566 . 6_556 48.3(6) ?
  O4a Fe1 O4a 6_546 . 16_544 92.0(7) ?
  O4a Fe1 O4b 6_546 . 10_564 166.0(7) ?
  O4a Fe1 O4b 6_546 . 4_566 91.3(7) ?
  O4a Fe1 O4b 6_546 . 6_546 14.0(7) ?
  O4a Fe1 O4b 6_546 . 16_544 88.7(7) ?
  O4a Fe1 As2 6_546 . . 37.0(5) ?
  O4a Fe1 As2 6_546 . 10_554 88.2(5) ?
  O4a Fe1 As2 6_546 . 11_555 95.9(5) ?
  O4a Fe1 As2 6_546 . 4_556 34.4(5) ?
  O4a Fe1 As2 6_546 . 13_555 143.0(5) ?
  O4a Fe1 As2 6_546 . 6_556 91.8(5) ?
  O4a Fe1 As2 6_546 . 7_555 84.1(5) ?
  O4a Fe1 As2 6_546 . 16_554 145.6(5) ?
  O4a Fe1 As3 6_546 . 10_564 146.9(5) ?
  O4a Fe1 As3 6_546 . 4_566 120.8(5) ?
  O4a Fe1 As3 6_546 . 6_546 33.1(5) ?
  O4a Fe1 As3 6_546 . 16_544 59.2(5) ?
  O4a Fe1 Ca 6_546 . . 48.3(6) ?
  O4a Fe1 Ca 6_546 . 10_554 87.6(5) ?
  O4a Fe1 Ca 6_546 . 13_555 131.7(6) ?
  O4a Fe1 Ca 6_546 . 6_556 92.4(5) ?
  O4a Fe1 O4b 16_544 . 10_564 91.3(7) ?
  O4a Fe1 O4b 16_544 . 4_566 166.0(7) ?
  O4a Fe1 O4b 16_544 . 6_546 88.7(7) ?
  O4a Fe1 O4b 16_544 . 16_544 14.0(7) ?
  O4a Fe1 As2 16_544 . . 95.9(5) ?
  O4a Fe1 As2 16_544 . 10_554 34.4(5) ?
  O4a Fe1 As2 16_544 . 11_555 37.0(5) ?
  O4a Fe1 As2 16_544 . 4_556 88.2(5) ?
  O4a Fe1 As2 16_544 . 13_555 84.1(5) ?
  O4a Fe1 As2 16_544 . 6_556 145.6(5) ?
  O4a Fe1 As2 16_544 . 7_555 143.0(5) ?
  O4a Fe1 As2 16_544 . 16_554 91.8(5) ?
  O4a Fe1 As3 16_544 . 10_564 120.8(5) ?
  O4a Fe1 As3 16_544 . 4_566 146.9(5) ?
  O4a Fe1 As3 16_544 . 6_546 59.2(5) ?
  O4a Fe1 As3 16_544 . 16_544 33.1(5) ?
  O4a Fe1 Ca 16_544 . . 87.6(5) ?
  O4a Fe1 Ca 16_544 . 10_554 48.3(6) ?
  O4a Fe1 Ca 16_544 . 13_555 92.4(5) ?
  O4a Fe1 Ca 16_544 . 6_556 131.7(6) ?
  O4b Fe1 O4b 10_564 . 4_566 88.8(8) ?
  O4b Fe1 O4b 10_564 . 6_546 180.0(5) ?
  O4b Fe1 O4b 10_564 . 16_544 91.2(8) ?
  O4b Fe1 As2 10_564 . . 155.7(5) ?
  O4b Fe1 As2 10_564 . 10_554 86.9(6) ?
  O4b Fe1 As2 10_564 . 11_555 78.7(6) ?
  O4b Fe1 As2 10_564 . 4_556 159.4(5) ?
  O4b Fe1 As2 10_564 . 13_555 24.3(5) ?
  O4b Fe1 As2 10_564 . 6_556 93.1(6) ?
  O4b Fe1 As2 10_564 . 7_555 101.3(6) ?
  O4b Fe1 As2 10_564 . 16_554 20.6(5) ?
  O4b Fe1 As3 10_564 . 10_564 34.0(6) ?
  O4b Fe1 As3 10_564 . 4_566 55.9(6) ?
  O4b Fe1 As3 10_564 . 6_546 146.0(6) ?
  O4b Fe1 As3 10_564 . 16_544 124.1(6) ?
  O4b Fe1 Ca 10_564 . . 145.5(6) ?
  O4b Fe1 Ca 10_564 . 10_554 84.4(5) ?
  O4b Fe1 Ca 10_564 . 13_555 34.5(6) ?
  O4b Fe1 Ca 10_564 . 6_556 95.6(5) ?
  O4b Fe1 O4b 4_566 . 6_546 91.2(8) ?
  O4b Fe1 O4b 4_566 . 16_544 180.0(5) ?
  O4b Fe1 As2 4_566 . . 78.7(6) ?
  O4b Fe1 As2 4_566 . 10_554 159.4(5) ?
  O4b Fe1 As2 4_566 . 11_555 155.7(5) ?
  O4b Fe1 As2 4_566 . 4_556 86.9(6) ?
  O4b Fe1 As2 4_566 . 13_555 101.3(6) ?
  O4b Fe1 As2 4_566 . 6_556 20.6(5) ?
  O4b Fe1 As2 4_566 . 7_555 24.3(5) ?
  O4b Fe1 As2 4_566 . 16_554 93.1(6) ?
  O4b Fe1 As3 4_566 . 10_564 55.9(6) ?
  O4b Fe1 As3 4_566 . 4_566 34.0(6) ?
  O4b Fe1 As3 4_566 . 6_546 124.1(6) ?
  O4b Fe1 As3 4_566 . 16_544 146.0(6) ?
  O4b Fe1 Ca 4_566 . . 84.4(5) ?
  O4b Fe1 Ca 4_566 . 10_554 145.5(6) ?
  O4b Fe1 Ca 4_566 . 13_555 95.6(5) ?
  O4b Fe1 Ca 4_566 . 6_556 34.5(6) ?
  O4b Fe1 O4b 6_546 . 16_544 88.8(8) ?
  O4b Fe1 As2 6_546 . . 24.3(5) ?
  O4b Fe1 As2 6_546 . 10_554 93.1(6) ?
  O4b Fe1 As2 6_546 . 11_555 101.3(6) ?
  O4b Fe1 As2 6_546 . 4_556 20.6(5) ?
  O4b Fe1 As2 6_546 . 13_555 155.7(5) ?
  O4b Fe1 As2 6_546 . 6_556 86.9(6) ?
  O4b Fe1 As2 6_546 . 7_555 78.7(6) ?
  O4b Fe1 As2 6_546 . 16_554 159.4(5) ?
  O4b Fe1 As3 6_546 . 10_564 146.0(6) ?
  O4b Fe1 As3 6_546 . 4_566 124.1(6) ?
  O4b Fe1 As3 6_546 . 6_546 34.0(6) ?
  O4b Fe1 As3 6_546 . 16_544 55.9(6) ?
  O4b Fe1 Ca 6_546 . . 34.5(6) ?
  O4b Fe1 Ca 6_546 . 10_554 95.6(5) ?
  O4b Fe1 Ca 6_546 . 13_555 145.5(6) ?
  O4b Fe1 Ca 6_546 . 6_556 84.4(5) ?
  O4b Fe1 As2 16_544 . . 101.3(6) ?
  O4b Fe1 As2 16_544 . 10_554 20.6(5) ?
  O4b Fe1 As2 16_544 . 11_555 24.3(5) ?
  O4b Fe1 As2 16_544 . 4_556 93.1(6) ?
  O4b Fe1 As2 16_544 . 13_555 78.7(6) ?
  O4b Fe1 As2 16_544 . 6_556 159.4(5) ?
  O4b Fe1 As2 16_544 . 7_555 155.7(5) ?
  O4b Fe1 As2 16_544 . 16_554 86.9(6) ?
  O4b Fe1 As3 16_544 . 10_564 124.1(6) ?
  O4b Fe1 As3 16_544 . 4_566 146.0(6) ?
  O4b Fe1 As3 16_544 . 6_546 55.9(6) ?
  O4b Fe1 As3 16_544 . 16_544 34.0(6) ?
  O4b Fe1 Ca 16_544 . . 95.6(5) ?
  O4b Fe1 Ca 16_544 . 10_554 34.5(6) ?
  O4b Fe1 Ca 16_544 . 13_555 84.4(5) ?
  O4b Fe1 Ca 16_544 . 6_556 145.5(6) ?
  As2 Fe1 As2 . . 10_554 111.82(17) ?
  As2 Fe1 As2 . . 11_555 119.87(16) ?
  As2 Fe1 As2 . . 4_556 8.17(16) ?
  As2 Fe1 As2 . . 13_555 180.0(5) ?
  As2 Fe1 As2 . . 6_556 68.18(17) ?
  As2 Fe1 As2 . . 7_555 60.13(16) ?
  As2 Fe1 As2 . . 16_554 171.83(16) ?
  As2 Fe1 As3 . . 10_564 126.24(15) ?
  As2 Fe1 As3 . . 4_566 112.51(15) ?
  As2 Fe1 As3 . . 6_546 53.76(15) ?
  As2 Fe1 As3 . . 16_544 67.49(15) ?
  As2 Fe1 Ca . . . 13.9(3) ?
  As2 Fe1 Ca . . 10_554 117.45(12) ?
  As2 Fe1 Ca . . 13_555 166.1(3) ?
  As2 Fe1 Ca . . 6_556 62.55(12) ?
  As2 Fe1 As2 10_554 . 11_555 8.17(16) ?
  As2 Fe1 As2 10_554 . 4_556 103.82(17) ?
  As2 Fe1 As2 10_554 . 13_555 68.18(17) ?
  As2 Fe1 As2 10_554 . 6_556 180.0(5) ?
  As2 Fe1 As2 10_554 . 7_555 171.83(16) ?
  As2 Fe1 As2 10_554 . 16_554 76.18(17) ?
  As2 Fe1 As3 10_554 . 10_564 120.67(15) ?
  As2 Fe1 As3 10_554 . 4_566 133.56(16) ?
  As2 Fe1 As3 10_554 . 6_546 59.33(15) ?
  As2 Fe1 As3 10_554 . 16_544 46.44(16) ?
  As2 Fe1 Ca 10_554 . . 110.06(12) ?
  As2 Fe1 Ca 10_554 . 10_554 13.9(3) ?
  As2 Fe1 Ca 10_554 . 13_555 69.94(12) ?
  As2 Fe1 Ca 10_554 . 6_556 166.1(3) ?
  As2 Fe1 As2 11_555 . 4_556 111.82(17) ?
  As2 Fe1 As2 11_555 . 13_555 60.13(16) ?
  As2 Fe1 As2 11_555 . 6_556 171.83(16) ?
  As2 Fe1 As2 11_555 . 7_555 180.0(5) ?
  As2 Fe1 As2 11_555 . 16_554 68.18(17) ?
  As2 Fe1 As3 11_555 . 10_564 112.51(15) ?
  As2 Fe1 As3 11_555 . 4_566 126.24(15) ?
  As2 Fe1 As3 11_555 . 6_546 67.49(15) ?
  As2 Fe1 As3 11_555 . 16_544 53.76(15) ?
  As2 Fe1 Ca 11_555 . . 117.45(12) ?
  As2 Fe1 Ca 11_555 . 10_554 13.9(3) ?
  As2 Fe1 Ca 11_555 . 13_555 62.55(12) ?
  As2 Fe1 Ca 11_555 . 6_556 166.1(3) ?
  As2 Fe1 As2 4_556 . 13_555 171.83(16) ?
  As2 Fe1 As2 4_556 . 6_556 76.18(17) ?
  As2 Fe1 As2 4_556 . 7_555 68.18(17) ?
  As2 Fe1 As2 4_556 . 16_554 180.0(5) ?
  As2 Fe1 As3 4_556 . 10_564 133.56(16) ?
  As2 Fe1 As3 4_556 . 4_566 120.67(15) ?
  As2 Fe1 As3 4_556 . 6_546 46.44(16) ?
  As2 Fe1 As3 4_556 . 16_544 59.33(15) ?
  As2 Fe1 Ca 4_556 . . 13.9(3) ?
  As2 Fe1 Ca 4_556 . 10_554 110.06(12) ?
  As2 Fe1 Ca 4_556 . 13_555 166.1(3) ?
  As2 Fe1 Ca 4_556 . 6_556 69.94(12) ?
  As2 Fe1 As2 13_555 . 6_556 111.82(17) ?
  As2 Fe1 As2 13_555 . 7_555 119.87(16) ?
  As2 Fe1 As2 13_555 . 16_554 8.17(16) ?
  As2 Fe1 As3 13_555 . 10_564 53.76(15) ?
  As2 Fe1 As3 13_555 . 4_566 67.49(15) ?
  As2 Fe1 As3 13_555 . 6_546 126.24(15) ?
  As2 Fe1 As3 13_555 . 16_544 112.51(15) ?
  As2 Fe1 Ca 13_555 . . 166.1(3) ?
  As2 Fe1 Ca 13_555 . 10_554 62.55(12) ?
  As2 Fe1 Ca 13_555 . 13_555 13.9(3) ?
  As2 Fe1 Ca 13_555 . 6_556 117.45(12) ?
  As2 Fe1 As2 6_556 . 7_555 8.17(16) ?
  As2 Fe1 As2 6_556 . 16_554 103.82(17) ?
  As2 Fe1 As3 6_556 . 10_564 59.33(15) ?
  As2 Fe1 As3 6_556 . 4_566 46.44(16) ?
  As2 Fe1 As3 6_556 . 6_546 120.67(15) ?
  As2 Fe1 As3 6_556 . 16_544 133.56(16) ?
  As2 Fe1 Ca 6_556 . . 69.94(12) ?
  As2 Fe1 Ca 6_556 . 10_554 166.1(3) ?
  As2 Fe1 Ca 6_556 . 13_555 110.06(12) ?
  As2 Fe1 Ca 6_556 . 6_556 13.9(3) ?
  As2 Fe1 As2 7_555 . 16_554 111.82(17) ?
  As2 Fe1 As3 7_555 . 10_564 67.49(15) ?
  As2 Fe1 As3 7_555 . 4_566 53.76(15) ?
  As2 Fe1 As3 7_555 . 6_546 112.51(15) ?
  As2 Fe1 As3 7_555 . 16_544 126.24(15) ?
  As2 Fe1 Ca 7_555 . . 62.55(12) ?
  As2 Fe1 Ca 7_555 . 10_554 166.1(3) ?
  As2 Fe1 Ca 7_555 . 13_555 117.45(12) ?
  As2 Fe1 Ca 7_555 . 6_556 13.9(3) ?
  As2 Fe1 As3 16_554 . 10_564 46.44(16) ?
  As2 Fe1 As3 16_554 . 4_566 59.33(15) ?
  As2 Fe1 As3 16_554 . 6_546 133.56(16) ?
  As2 Fe1 As3 16_554 . 16_544 120.67(15) ?
  As2 Fe1 Ca 16_554 . . 166.1(3) ?
  As2 Fe1 Ca 16_554 . 10_554 69.94(12) ?
  As2 Fe1 Ca 16_554 . 13_555 13.9(3) ?
  As2 Fe1 Ca 16_554 . 6_556 110.06(12) ?
  As3 Fe1 As3 10_564 . 4_566 27.14(15) ?
  As3 Fe1 As3 10_564 . 6_546 180.0(5) ?
  As3 Fe1 As3 10_564 . 16_544 152.86(15) ?
  As3 Fe1 Ca 10_564 . . 123.1(2) ?
  As3 Fe1 Ca 10_564 . 10_554 116.30(11) ?
  As3 Fe1 Ca 10_564 . 13_555 56.9(2) ?
  As3 Fe1 Ca 10_564 . 6_556 63.70(11) ?
  As3 Fe1 As3 4_566 . 6_546 152.86(15) ?
  As3 Fe1 As3 4_566 . 16_544 180.0(5) ?
  As3 Fe1 Ca 4_566 . . 116.30(11) ?
  As3 Fe1 Ca 4_566 . 10_554 123.1(2) ?
  As3 Fe1 Ca 4_566 . 13_555 63.70(11) ?
  As3 Fe1 Ca 4_566 . 6_556 56.9(2) ?
  As3 Fe1 As3 6_546 . 16_544 27.14(15) ?
  As3 Fe1 Ca 6_546 . . 56.9(2) ?
  As3 Fe1 Ca 6_546 . 10_554 63.70(11) ?
  As3 Fe1 Ca 6_546 . 13_555 123.1(2) ?
  As3 Fe1 Ca 6_546 . 6_556 116.30(11) ?
  As3 Fe1 Ca 16_544 . . 63.70(11) ?
  As3 Fe1 Ca 16_544 . 10_554 56.9(2) ?
  As3 Fe1 Ca 16_544 . 13_555 116.30(11) ?
  As3 Fe1 Ca 16_544 . 6_556 123.1(2) ?
  Ca Fe1 Ca . . 10_554 118.83(14) ?
  Ca Fe1 Ca . . 13_555 180.0(5) ?
  Ca Fe1 Ca . . 6_556 61.17(14) ?
  Ca Fe1 Ca 10_554 . 13_555 61.17(14) ?
  Ca Fe1 Ca 10_554 . 6_556 180.0(5) ?
  Ca Fe1 Ca 13_555 . 6_556 118.83(14) ?
  Fe1 Fe2 Fe1 . . 10_565 115.5(4) ?
  Fe1 Fe2 Fe2 . . 6_546 60.49(19) ?
  Fe1 Fe2 Fe2 . . 6_556 119.5(3) ?
  Fe1 Fe2 W2 . . . 64(3) ?
  Fe1 Fe2 W2 . . 4_566 55(3) ?
  Fe1 Fe2 W2 . . 6_546 57.0(4) ?
  Fe1 Fe2 W2 . . 6_556 116.0(4) ?
  Fe1 Fe2 W2 . . 7_555 56.0(3) ?
  Fe1 Fe2 W2 . . 7_565 114.4(5) ?
  Fe1 Fe2 As1 . . . 55.36(8) ?
  Fe1 Fe2 As1 . . 4_566 170.2(5) ?
  Fe1 Fe2 P1 . . . 55.36(8) ?
  Fe1 Fe2 P1 . . 4_566 170.2(5) ?
  Fe1 Fe2 O3 . . . 74.7(3) ?
  Fe1 Fe2 O3 . . 4_566 165.3(4) ?
  Fe1 Fe2 O4a . . . 100.3(8) ?
  Fe1 Fe2 O4a . . 4_566 18.7(5) ?
  Fe1 Fe2 O4b . . . 91.8(7) ?
  Fe1 Fe2 O4b . . 4_566 25.1(5) ?
  Fe1 Fe2 O5 . . . 76.0(4) ?
  Fe1 Fe2 O5 . . 4_566 99.1(4) ?
  Fe1 Fe2 As2 . . 6_556 57.9(3) ?
  Fe1 Fe2 As2 . . 7_555 57.8(3) ?
  Fe1 Fe2 As3 . . . 87.3(3) ?
  Fe1 Fe2 As3 . . 4_566 59.4(2) ?
  Fe1 Fe2 As3 . . 6_556 72.1(2) ?
  Fe1 Fe2 As3 . . 7_555 80.6(3) ?
  Fe1 Fe2 Ca . . 6_556 57.7(2) ?
  Fe1 Fe2 Fe2 10_565 . 6_546 119.5(3) ?
  Fe1 Fe2 Fe2 10_565 . 6_556 60.49(19) ?
  Fe1 Fe2 W2 10_565 . . 55(3) ?
  Fe1 Fe2 W2 10_565 . 4_566 64(3) ?
  Fe1 Fe2 W2 10_565 . 6_546 114.4(5) ?
  Fe1 Fe2 W2 10_565 . 6_556 56.0(3) ?
  Fe1 Fe2 W2 10_565 . 7_555 116.0(4) ?
  Fe1 Fe2 W2 10_565 . 7_565 57.0(4) ?
  Fe1 Fe2 As1 10_565 . . 170.2(5) ?
  Fe1 Fe2 As1 10_565 . 4_566 55.36(8) ?
  Fe1 Fe2 P1 10_565 . . 170.2(5) ?
  Fe1 Fe2 P1 10_565 . 4_566 55.36(8) ?
  Fe1 Fe2 O3 10_565 . . 165.3(4) ?
  Fe1 Fe2 O3 10_565 . 4_566 74.7(3) ?
  Fe1 Fe2 O4a 10_565 . . 18.7(5) ?
  Fe1 Fe2 O4a 10_565 . 4_566 100.3(8) ?
  Fe1 Fe2 O4b 10_565 . . 25.1(5) ?
  Fe1 Fe2 O4b 10_565 . 4_566 91.8(7) ?
  Fe1 Fe2 O5 10_565 . . 99.1(4) ?
  Fe1 Fe2 O5 10_565 . 4_566 76.0(4) ?
  Fe1 Fe2 As2 10_565 . 6_556 57.8(3) ?
  Fe1 Fe2 As2 10_565 . 7_555 57.9(3) ?
  Fe1 Fe2 As3 10_565 . . 59.4(2) ?
  Fe1 Fe2 As3 10_565 . 4_566 87.3(3) ?
  Fe1 Fe2 As3 10_565 . 6_556 80.6(3) ?
  Fe1 Fe2 As3 10_565 . 7_555 72.1(2) ?
  Fe1 Fe2 Ca 10_565 . 6_556 57.7(2) ?
  Fe2 Fe2 Fe2 6_546 . 6_556 180.0(5) ?
  Fe2 Fe2 W2 6_546 . . 108(3) ?
  Fe2 Fe2 W2 6_546 . 4_566 72(2) ?
  Fe2 Fe2 W2 6_546 . 6_546 7.1(4) ?
  Fe2 Fe2 W2 6_546 . 6_556 173.4(7) ?
  Fe2 Fe2 W2 6_546 . 7_555 6.6(4) ?
  Fe2 Fe2 W2 6_546 . 7_565 172.9(7) ?
  Fe2 Fe2 As1 6_546 . . 54.46(14) ?
  Fe2 Fe2 As1 6_546 . 4_566 125.5(3) ?
  Fe2 Fe2 P1 6_546 . . 54.46(14) ?
  Fe2 Fe2 P1 6_546 . 4_566 125.5(3) ?
  Fe2 Fe2 O3 6_546 . . 74.3(3) ?
  Fe2 Fe2 O3 6_546 . 4_566 105.7(4) ?
  Fe2 Fe2 O4a 6_546 . . 103.1(6) ?
  Fe2 Fe2 O4a 6_546 . 4_566 76.9(6) ?
  Fe2 Fe2 O4b 6_546 . . 101.6(6) ?
  Fe2 Fe2 O4b 6_546 . 4_566 78.4(5) ?
  Fe2 Fe2 O5 6_546 . . 22.3(3) ?
  Fe2 Fe2 O5 6_546 . 4_566 157.7(3) ?
  Fe2 Fe2 As2 6_546 . 6_556 93.8(4) ?
  Fe2 Fe2 As2 6_546 . 7_555 86.2(4) ?
  Fe2 Fe2 As3 6_546 . . 60.1(2) ?
  Fe2 Fe2 As3 6_546 . 4_566 119.9(3) ?
  Fe2 Fe2 As3 6_546 . 6_556 132.6(3) ?
  Fe2 Fe2 As3 6_546 . 7_555 47.45(19) ?
  Fe2 Fe2 Ca 6_546 . 6_556 90.0(4) ?
  Fe2 Fe2 W2 6_556 . . 72(2) ?
  Fe2 Fe2 W2 6_556 . 4_566 108(3) ?
  Fe2 Fe2 W2 6_556 . 6_546 172.9(7) ?
  Fe2 Fe2 W2 6_556 . 6_556 6.6(4) ?
  Fe2 Fe2 W2 6_556 . 7_555 173.4(7) ?
  Fe2 Fe2 W2 6_556 . 7_565 7.1(4) ?
  Fe2 Fe2 As1 6_556 . . 125.5(3) ?
  Fe2 Fe2 As1 6_556 . 4_566 54.46(14) ?
  Fe2 Fe2 P1 6_556 . . 125.5(3) ?
  Fe2 Fe2 P1 6_556 . 4_566 54.46(14) ?
  Fe2 Fe2 O3 6_556 . . 105.7(4) ?
  Fe2 Fe2 O3 6_556 . 4_566 74.3(3) ?
  Fe2 Fe2 O4a 6_556 . . 76.9(6) ?
  Fe2 Fe2 O4a 6_556 . 4_566 103.1(6) ?
  Fe2 Fe2 O4b 6_556 . . 78.4(5) ?
  Fe2 Fe2 O4b 6_556 . 4_566 101.6(6) ?
  Fe2 Fe2 O5 6_556 . . 157.7(3) ?
  Fe2 Fe2 O5 6_556 . 4_566 22.3(3) ?
  Fe2 Fe2 As2 6_556 . 6_556 86.2(4) ?
  Fe2 Fe2 As2 6_556 . 7_555 93.8(4) ?
  Fe2 Fe2 As3 6_556 . . 119.9(3) ?
  Fe2 Fe2 As3 6_556 . 4_566 60.1(2) ?
  Fe2 Fe2 As3 6_556 . 6_556 47.45(19) ?
  Fe2 Fe2 As3 6_556 . 7_555 132.6(3) ?
  Fe2 Fe2 Ca 6_556 . 6_556 90.0(4) ?
  W2 Fe2 W2 . . 4_566 39(4) ?
  W2 Fe2 W2 . . 6_546 101(3) ?
  W2 Fe2 W2 . . 6_556 66(2) ?
  W2 Fe2 W2 . . 7_555 101(3) ?
  W2 Fe2 W2 . . 7_565 65(2) ?
  W2 Fe2 As1 . . . 118(3) ?
  W2 Fe2 As1 . . 4_566 106(3) ?
  W2 Fe2 P1 . . . 118(3) ?
  W2 Fe2 P1 . . 4_566 106(3) ?
  W2 Fe2 O3 . . . 129(3) ?
  W2 Fe2 O3 . . 4_566 128(3) ?
  W2 Fe2 O4a . . . 48(3) ?
  W2 Fe2 O4a . . 4_566 47(3) ?
  W2 Fe2 O4b . . . 39(3) ?
  W2 Fe2 O4b . . 4_566 39(3) ?
  W2 Fe2 O5 . . . 105(3) ?
  W2 Fe2 O5 . . 4_566 66(2) ?
  W2 Fe2 As2 . . 6_556 15(2) ?
  W2 Fe2 As2 . . 7_555 24(3) ?
  W2 Fe2 As3 . . . 75(3) ?
  W2 Fe2 As3 . . 4_566 43(3) ?
  W2 Fe2 As3 . . 6_556 46(3) ?
  W2 Fe2 As3 . . 7_555 82(3) ?
  W2 Fe2 Ca . . 6_556 19(3) ?
  W2 Fe2 W2 4_566 . 6_546 65(2) ?
  W2 Fe2 W2 4_566 . 6_556 101(3) ?
  W2 Fe2 W2 4_566 . 7_555 66(2) ?
  W2 Fe2 W2 4_566 . 7_565 101(3) ?
  W2 Fe2 As1 4_566 . . 106(3) ?
  W2 Fe2 As1 4_566 . 4_566 118(3) ?
  W2 Fe2 P1 4_566 . . 106(3) ?
  W2 Fe2 P1 4_566 . 4_566 118(3) ?
  W2 Fe2 O3 4_566 . . 128(3) ?
  W2 Fe2 O3 4_566 . 4_566 129(3) ?
  W2 Fe2 O4a 4_566 . . 47(3) ?
  W2 Fe2 O4a 4_566 . 4_566 48(3) ?
  W2 Fe2 O4b 4_566 . . 39(3) ?
  W2 Fe2 O4b 4_566 . 4_566 39(3) ?
  W2 Fe2 O5 4_566 . . 66(2) ?
  W2 Fe2 O5 4_566 . 4_566 105(3) ?
  W2 Fe2 As2 4_566 . 6_556 24(3) ?
  W2 Fe2 As2 4_566 . 7_555 15(2) ?
  W2 Fe2 As3 4_566 . . 43(3) ?
  W2 Fe2 As3 4_566 . 4_566 75(3) ?
  W2 Fe2 As3 4_566 . 6_556 82(3) ?
  W2 Fe2 As3 4_566 . 7_555 46(3) ?
  W2 Fe2 Ca 4_566 . 6_556 19(3) ?
  W2 Fe2 W2 6_546 . 6_556 166.3(7) ?
  W2 Fe2 W2 6_546 . 7_555 1.7(5) ?
  W2 Fe2 W2 6_546 . 7_565 165.9(7) ?
  W2 Fe2 As1 6_546 . . 58.8(4) ?
  W2 Fe2 As1 6_546 . 4_566 127.9(4) ?
  W2 Fe2 P1 6_546 . . 58.8(4) ?
  W2 Fe2 P1 6_546 . 4_566 127.9(4) ?
  W2 Fe2 O3 6_546 . . 79.8(4) ?
  W2 Fe2 O3 6_546 . 4_566 109.8(5) ?
  W2 Fe2 O4a 6_546 . . 97.3(7) ?
  W2 Fe2 O4a 6_546 . 4_566 72.3(6) ?
  W2 Fe2 O4b 6_546 . . 95.2(7) ?
  W2 Fe2 O4b 6_546 . 4_566 73.0(6) ?
  W2 Fe2 O5 6_546 . . 21.0(5) ?
  W2 Fe2 O5 6_546 . 4_566 156.1(6) ?
  W2 Fe2 As2 6_546 . 6_556 86.8(5) ?
  W2 Fe2 As2 6_546 . 7_555 79.1(4) ?
  W2 Fe2 As3 6_546 . . 55.3(4) ?
  W2 Fe2 As3 6_546 . 4_566 116.2(5) ?
  W2 Fe2 As3 6_546 . 6_556 128.7(5) ?
  W2 Fe2 As3 6_546 . 7_555 42.8(4) ?
  W2 Fe2 Ca 6_546 . 6_556 83.0(4) ?
  W2 Fe2 W2 6_556 . 7_555 167.0(7) ?
  W2 Fe2 W2 6_556 . 7_565 1.7(5) ?
  W2 Fe2 As1 6_556 . . 129.2(4) ?
  W2 Fe2 As1 6_556 . 4_566 57.1(3) ?
  W2 Fe2 P1 6_556 . . 129.2(4) ?
  W2 Fe2 P1 6_556 . 4_566 57.1(3) ?
  W2 Fe2 O3 6_556 . . 110.7(5) ?
  W2 Fe2 O3 6_556 . 4_566 78.3(4) ?
  W2 Fe2 O4a 6_556 . . 71.5(6) ?
  W2 Fe2 O4a 6_556 . 4_566 98.8(7) ?
  W2 Fe2 O4b 6_556 . . 72.5(6) ?
  W2 Fe2 O4b 6_556 . 4_566 96.5(6) ?
  W2 Fe2 O5 6_556 . . 154.8(6) ?
  W2 Fe2 O5 6_556 . 4_566 22.7(5) ?
  W2 Fe2 As2 6_556 . 6_556 79.7(4) ?
  W2 Fe2 As2 6_556 . 7_555 87.2(4) ?
  W2 Fe2 As3 6_556 . . 115.2(5) ?
  W2 Fe2 As3 6_556 . 4_566 57.0(4) ?
  W2 Fe2 As3 6_556 . 6_556 44.5(4) ?
  W2 Fe2 As3 6_556 . 7_555 127.8(5) ?
  W2 Fe2 Ca 6_556 . 6_556 83.5(4) ?
  W2 Fe2 W2 7_555 . 7_565 166.3(7) ?
  W2 Fe2 As1 7_555 . . 57.1(3) ?
  W2 Fe2 As1 7_555 . 4_566 129.2(4) ?
  W2 Fe2 P1 7_555 . . 57.1(3) ?
  W2 Fe2 P1 7_555 . 4_566 129.2(4) ?
  W2 Fe2 O3 7_555 . . 78.3(4) ?
  W2 Fe2 O3 7_555 . 4_566 110.7(5) ?
  W2 Fe2 O4a 7_555 . . 98.8(7) ?
  W2 Fe2 O4a 7_555 . 4_566 71.5(6) ?
  W2 Fe2 O4b 7_555 . . 96.5(6) ?
  W2 Fe2 O4b 7_555 . 4_566 72.5(6) ?
  W2 Fe2 O5 7_555 . . 22.7(5) ?
  W2 Fe2 O5 7_555 . 4_566 154.8(6) ?
  W2 Fe2 As2 7_555 . 6_556 87.2(4) ?
  W2 Fe2 As2 7_555 . 7_555 79.7(4) ?
  W2 Fe2 As3 7_555 . . 57.0(4) ?
  W2 Fe2 As3 7_555 . 4_566 115.2(5) ?
  W2 Fe2 As3 7_555 . 6_556 127.8(5) ?
  W2 Fe2 As3 7_555 . 7_555 44.5(4) ?
  W2 Fe2 Ca 7_555 . 6_556 83.5(4) ?
  W2 Fe2 As1 7_565 . . 127.9(4) ?
  W2 Fe2 As1 7_565 . 4_566 58.8(4) ?
  W2 Fe2 P1 7_565 . . 127.9(4) ?
  W2 Fe2 P1 7_565 . 4_566 58.8(4) ?
  W2 Fe2 O3 7_565 . . 109.8(5) ?
  W2 Fe2 O3 7_565 . 4_566 79.8(4) ?
  W2 Fe2 O4a 7_565 . . 72.3(6) ?
  W2 Fe2 O4a 7_565 . 4_566 97.3(7) ?
  W2 Fe2 O4b 7_565 . . 73.0(6) ?
  W2 Fe2 O4b 7_565 . 4_566 95.2(7) ?
  W2 Fe2 O5 7_565 . . 156.1(6) ?
  W2 Fe2 O5 7_565 . 4_566 21.0(5) ?
  W2 Fe2 As2 7_565 . 6_556 79.1(4) ?
  W2 Fe2 As2 7_565 . 7_555 86.8(5) ?
  W2 Fe2 As3 7_565 . . 116.2(5) ?
  W2 Fe2 As3 7_565 . 4_566 55.3(4) ?
  W2 Fe2 As3 7_565 . 6_556 42.8(4) ?
  W2 Fe2 As3 7_565 . 7_555 128.7(5) ?
  W2 Fe2 Ca 7_565 . 6_556 83.0(4) ?
  As1 Fe2 As1 . . 4_566 134.0(6) ?
  As1 Fe2 P1 . . . 0.0(5) ?
  As1 Fe2 P1 . . 4_566 134.0(6) ?
  As1 Fe2 O3 . . . 23.7(3) ?
  As1 Fe2 O3 . . 4_566 113.6(7) ?
  As1 Fe2 O4a . . . 151.8(7) ?
  As1 Fe2 O4a . . 4_566 71.4(5) ?
  As1 Fe2 O4b . . . 145.1(7) ?
  As1 Fe2 O4b . . 4_566 79.7(5) ?
  As1 Fe2 O5 . . . 76.0(3) ?
  As1 Fe2 O5 . . 4_566 107.7(4) ?
  As1 Fe2 As2 . . 6_556 113.3(3) ?
  As1 Fe2 As2 . . 7_555 112.6(3) ?
  As1 Fe2 As3 . . . 114.14(13) ?
  As1 Fe2 As3 . . 4_566 89.87(13) ?
  As1 Fe2 As3 . . 6_556 98.35(11) ?
  As1 Fe2 As3 . . 7_555 101.55(11) ?
  As1 Fe2 Ca . . 6_556 113.0(3) ?
  As1 Fe2 P1 4_566 . . 134.0(6) ?
  As1 Fe2 P1 4_566 . 4_566 0.0(5) ?
  As1 Fe2 O3 4_566 . . 113.6(7) ?
  As1 Fe2 O3 4_566 . 4_566 23.7(3) ?
  As1 Fe2 O4a 4_566 . . 71.4(5) ?
  As1 Fe2 O4a 4_566 . 4_566 151.8(7) ?
  As1 Fe2 O4b 4_566 . . 79.7(5) ?
  As1 Fe2 O4b 4_566 . 4_566 145.1(7) ?
  As1 Fe2 O5 4_566 . . 107.7(4) ?
  As1 Fe2 O5 4_566 . 4_566 76.0(3) ?
  As1 Fe2 As2 4_566 . 6_556 112.6(3) ?
  As1 Fe2 As2 4_566 . 7_555 113.3(3) ?
  As1 Fe2 As3 4_566 . . 89.87(13) ?
  As1 Fe2 As3 4_566 . 4_566 114.14(13) ?
  As1 Fe2 As3 4_566 . 6_556 101.55(11) ?
  As1 Fe2 As3 4_566 . 7_555 98.35(11) ?
  As1 Fe2 Ca 4_566 . 6_556 113.0(3) ?
  P1 Fe2 P1 . . 4_566 134.0(6) ?
  P1 Fe2 O3 . . . 23.7(3) ?
  P1 Fe2 O3 . . 4_566 113.6(7) ?
  P1 Fe2 O4a . . . 151.8(7) ?
  P1 Fe2 O4a . . 4_566 71.4(5) ?
  P1 Fe2 O4b . . . 145.1(7) ?
  P1 Fe2 O4b . . 4_566 79.7(5) ?
  P1 Fe2 O5 . . . 76.0(3) ?
  P1 Fe2 O5 . . 4_566 107.7(4) ?
  P1 Fe2 As2 . . 6_556 113.3(3) ?
  P1 Fe2 As2 . . 7_555 112.6(3) ?
  P1 Fe2 As3 . . . 114.14(13) ?
  P1 Fe2 As3 . . 4_566 89.87(13) ?
  P1 Fe2 As3 . . 6_556 98.35(11) ?
  P1 Fe2 As3 . . 7_555 101.55(11) ?
  P1 Fe2 Ca . . 6_556 113.0(3) ?
  P1 Fe2 O3 4_566 . . 113.6(7) ?
  P1 Fe2 O3 4_566 . 4_566 23.7(3) ?
  P1 Fe2 O4a 4_566 . . 71.4(5) ?
  P1 Fe2 O4a 4_566 . 4_566 151.8(7) ?
  P1 Fe2 O4b 4_566 . . 79.7(5) ?
  P1 Fe2 O4b 4_566 . 4_566 145.1(7) ?
  P1 Fe2 O5 4_566 . . 107.7(4) ?
  P1 Fe2 O5 4_566 . 4_566 76.0(3) ?
  P1 Fe2 As2 4_566 . 6_556 112.6(3) ?
  P1 Fe2 As2 4_566 . 7_555 113.3(3) ?
  P1 Fe2 As3 4_566 . . 89.87(13) ?
  P1 Fe2 As3 4_566 . 4_566 114.14(13) ?
  P1 Fe2 As3 4_566 . 6_556 101.55(11) ?
  P1 Fe2 As3 4_566 . 7_555 98.35(11) ?
  P1 Fe2 Ca 4_566 . 6_556 113.0(3) ?
  O3 Fe2 O3 . . 4_566 97.4(9) ?
  O3 Fe2 O4a . . . 175.0(9) ?
  O3 Fe2 O4a . . 4_566 87.3(6) ?
  O3 Fe2 O4b . . . 166.2(8) ?
  O3 Fe2 O4b . . 4_566 96.3(6) ?
  O3 Fe2 O5 . . . 93.5(5) ?
  O3 Fe2 O5 . . 4_566 92.4(5) ?
  O3 Fe2 As2 . . 6_556 130.0(5) ?
  O3 Fe2 As2 . . 7_555 132.2(5) ?
  O3 Fe2 As3 . . . 134.0(3) ?
  O3 Fe2 As3 . . 4_566 89.5(3) ?
  O3 Fe2 As3 . . 6_556 93.5(3) ?
  O3 Fe2 As3 . . 7_555 121.5(3) ?
  O3 Fe2 Ca . . 6_556 131.3(5) ?
  O3 Fe2 O4a 4_566 . . 87.3(6) ?
  O3 Fe2 O4a 4_566 . 4_566 175.0(9) ?
  O3 Fe2 O4b 4_566 . . 96.3(6) ?
  O3 Fe2 O4b 4_566 . 4_566 166.2(8) ?
  O3 Fe2 O5 4_566 . . 92.4(5) ?
  O3 Fe2 O5 4_566 . 4_566 93.5(5) ?
  O3 Fe2 As2 4_566 . 6_556 132.2(5) ?
  O3 Fe2 As2 4_566 . 7_555 130.0(5) ?
  O3 Fe2 As3 4_566 . . 89.5(3) ?
  O3 Fe2 As3 4_566 . 4_566 134.0(3) ?
  O3 Fe2 As3 4_566 . 6_556 121.5(3) ?
  O3 Fe2 As3 4_566 . 7_555 93.5(3) ?
  O3 Fe2 Ca 4_566 . 6_556 131.3(5) ?
  O4a Fe2 O4a . . 4_566 87.9(10) ?
  O4a Fe2 O4b . . . 9.0(7) ?
  O4a Fe2 O4b . . 4_566 78.9(9) ?
  O4a Fe2 O5 . . . 84.9(7) ?
  O4a Fe2 O5 . . 4_566 88.7(7) ?
  O4a Fe2 As2 . . 6_556 45.4(7) ?
  O4a Fe2 As2 . . 7_555 42.9(6) ?
  O4a Fe2 As3 . . . 44.2(6) ?
  O4a Fe2 As3 . . 4_566 88.1(7) ?
  O4a Fe2 As3 . . 6_556 85.1(7) ?
  O4a Fe2 As3 . . 7_555 56.6(6) ?
  O4a Fe2 Ca . . 6_556 44.0(6) ?
  O4a Fe2 O4b 4_566 . . 78.9(9) ?
  O4a Fe2 O4b 4_566 . 4_566 9.0(7) ?
  O4a Fe2 O5 4_566 . . 88.7(7) ?
  O4a Fe2 O5 4_566 . 4_566 84.9(7) ?
  O4a Fe2 As2 4_566 . 6_556 42.9(6) ?
  O4a Fe2 As2 4_566 . 7_555 45.4(7) ?
  O4a Fe2 As3 4_566 . . 88.1(7) ?
  O4a Fe2 As3 4_566 . 4_566 44.2(6) ?
  O4a Fe2 As3 4_566 . 6_556 56.6(6) ?
  O4a Fe2 As3 4_566 . 7_555 85.1(7) ?
  O4a Fe2 Ca 4_566 . 6_556 44.0(6) ?
  O4b Fe2 O4b . . 4_566 69.9(8) ?
  O4b Fe2 O5 . . . 85.6(7) ?
  O4b Fe2 O5 . . 4_566 87.1(7) ?
  O4b Fe2 As2 . . 6_556 36.4(5) ?
  O4b Fe2 As2 . . 7_555 34.1(5) ?
  O4b Fe2 As3 . . . 45.7(5) ?
  O4b Fe2 As3 . . 4_566 81.1(7) ?
  O4b Fe2 As3 . . 6_556 79.5(6) ?
  O4b Fe2 As3 . . 7_555 57.1(5) ?
  O4b Fe2 Ca . . 6_556 35.0(5) ?
  O4b Fe2 O5 4_566 . . 87.1(7) ?
  O4b Fe2 O5 4_566 . 4_566 85.6(7) ?
  O4b Fe2 As2 4_566 . 6_556 34.1(5) ?
  O4b Fe2 As2 4_566 . 7_555 36.4(5) ?
  O4b Fe2 As3 4_566 . . 81.1(7) ?
  O4b Fe2 As3 4_566 . 4_566 45.7(5) ?
  O4b Fe2 As3 4_566 . 6_556 57.1(5) ?
  O4b Fe2 As3 4_566 . 7_555 79.5(6) ?
  O4b Fe2 Ca 4_566 . 6_556 35.0(5) ?
  O5 Fe2 O5 . . 4_566 171.1(11) ?
  O5 Fe2 As2 . . 6_556 90.0(6) ?
  O5 Fe2 As2 . . 7_555 81.0(6) ?
  O5 Fe2 As3 . . . 40.6(4) ?
  O5 Fe2 As3 . . 4_566 132.7(7) ?
  O5 Fe2 As3 . . 6_556 144.1(7) ?
  O5 Fe2 As3 . . 7_555 28.5(4) ?
  O5 Fe2 Ca . . 6_556 85.5(6) ?
  O5 Fe2 As2 4_566 . 6_556 81.0(6) ?
  O5 Fe2 As2 4_566 . 7_555 90.0(6) ?
  O5 Fe2 As3 4_566 . . 132.7(7) ?
  O5 Fe2 As3 4_566 . 4_566 40.6(4) ?
  O5 Fe2 As3 4_566 . 6_556 28.5(4) ?
  O5 Fe2 As3 4_566 . 7_555 144.1(7) ?
  O5 Fe2 Ca 4_566 . 6_556 85.5(6) ?
  As2 Fe2 As2 6_556 . 7_555 9.28(19) ?
  As2 Fe2 As3 6_556 . . 63.0(4) ?
  As2 Fe2 As3 6_556 . 4_566 54.3(3) ?
  As2 Fe2 As3 6_556 . 6_556 59.1(3) ?
  As2 Fe2 As3 6_556 . 7_555 68.4(3) ?
  As2 Fe2 Ca 6_556 . 6_556 4.64(13) ?
  As2 Fe2 As3 7_555 . . 54.3(3) ?
  As2 Fe2 As3 7_555 . 4_566 63.0(4) ?
  As2 Fe2 As3 7_555 . 6_556 68.4(3) ?
  As2 Fe2 As3 7_555 . 7_555 59.1(3) ?
  As2 Fe2 Ca 7_555 . 6_556 4.64(13) ?
  As3 Fe2 As3 . . 4_566 117.3(6) ?
  As3 Fe2 As3 . . 6_556 121.0(6) ?
  As3 Fe2 As3 . . 7_555 12.68(15) ?
  As3 Fe2 Ca . . 6_556 58.6(3) ?
  As3 Fe2 As3 4_566 . 6_556 12.68(15) ?
  As3 Fe2 As3 4_566 . 7_555 121.0(6) ?
  As3 Fe2 Ca 4_566 . 6_556 58.6(3) ?
  As3 Fe2 As3 6_556 . 7_555 127.5(6) ?
  As3 Fe2 Ca 6_556 . 6_556 63.8(3) ?
  As3 Fe2 Ca 7_555 . 6_556 63.8(3) ?
  Fe1 W2 Fe1 . . 10_565 127.3(6) ?
  Fe1 W2 Fe2 . . . 109(3) ?
  Fe1 W2 Fe2 . . 6_546 60.4(3) ?
  Fe1 W2 Fe2 . . 6_556 128.1(7) ?
  Fe1 W2 W2 . . 4_566 74(6) ?
  Fe1 W2 W2 . . 6_546 57.6(5) ?
  Fe1 W2 W2 . . 6_556 125.3(7) ?
  Fe1 W2 W2 . . 7_555 56.1(4) ?
  Fe1 W2 W2 . . 7_565 123.9(7) ?
  Fe1 W2 As1 . . . 55.5(3) ?
  Fe1 W2 As1 . . 4_566 175.3(6) ?
  Fe1 W2 P1 . . . 55.5(3) ?
  Fe1 W2 P1 . . 4_566 175.3(6) ?
  Fe1 W2 O3 . . . 76.3(6) ?
  Fe1 W2 O3 . . 4_566 150.0(8) ?
  Fe1 W2 O4a . . . 114.4(11) ?
  Fe1 W2 O4a . . 4_566 14.2(7) ?
  Fe1 W2 O4b . . . 103.5(9) ?
  Fe1 W2 O4b . . 4_566 23.2(6) ?
  Fe1 W2 O5 . . . 78.7(6) ?
  Fe1 W2 O5 . . 4_566 108.4(10) ?
  Fe1 W2 As2 . . 6_556 63.3(5) ?
  Fe1 W2 As2 . . 7_555 63.0(5) ?
  Fe1 W2 As3 . . . 92.2(5) ?
  Fe1 W2 As3 . . 4_566 64.2(5) ?
  Fe1 W2 As3 . . 6_556 78.1(5) ?
  Fe1 W2 As3 . . 7_555 83.7(4) ?
  Fe1 W2 Ca . . 1_565 96.6(5) ?
  Fe1 W2 Ca . . 6_556 63.3(4) ?
  Fe1 W2 Fe2 10_565 . . 119(3) ?
  Fe1 W2 Fe2 10_565 . 6_546 121.6(6) ?
  Fe1 W2 Fe2 10_565 . 6_556 63.9(4) ?
  Fe1 W2 W2 10_565 . 4_566 101(6) ?
  Fe1 W2 W2 10_565 . 6_546 117.7(7) ?
  Fe1 W2 W2 10_565 . 6_556 59.5(5) ?
  Fe1 W2 W2 10_565 . 7_555 119.1(7) ?
  Fe1 W2 W2 10_565 . 7_565 60.9(5) ?
  Fe1 W2 As1 10_565 . . 171.5(7) ?
  Fe1 W2 As1 10_565 . 4_566 56.9(4) ?
  Fe1 W2 P1 10_565 . . 171.5(7) ?
  Fe1 W2 P1 10_565 . 4_566 56.9(4) ?
  Fe1 W2 O3 10_565 . . 156.3(9) ?
  Fe1 W2 O3 10_565 . 4_566 78.0(7) ?
  Fe1 W2 O4a 10_565 . . 19.4(7) ?
  Fe1 W2 O4a 10_565 . 4_566 118.0(11) ?
  Fe1 W2 O4b 10_565 . . 25.7(6) ?
  Fe1 W2 O4b 10_565 . 4_566 106.0(9) ?
  Fe1 W2 O5 10_565 . . 103.3(8) ?
  Fe1 W2 O5 10_565 . 4_566 84.3(8) ?
  Fe1 W2 As2 10_565 . 6_556 64.5(5) ?
  Fe1 W2 As2 10_565 . 7_555 64.4(5) ?
  Fe1 W2 As3 10_565 . . 63.6(5) ?
  Fe1 W2 As3 10_565 . 4_566 98.1(6) ?
  Fe1 W2 As3 10_565 . 6_556 89.0(5) ?
  Fe1 W2 As3 10_565 . 7_555 75.7(5) ?
  Fe1 W2 Ca 10_565 . 1_565 48.1(2) ?
  Fe1 W2 Ca 10_565 . 6_556 64.1(4) ?
  Fe2 W2 Fe2 . . 6_546 65(2) ?
  Fe2 W2 Fe2 . . 6_556 101(3) ?
  Fe2 W2 W2 . . 4_566 71(5) ?
  Fe2 W2 W2 . . 6_546 72(2) ?
  Fe2 W2 W2 . . 6_556 108(3) ?
  Fe2 W2 W2 . . 7_555 72(2) ?
  Fe2 W2 W2 . . 7_565 108(3) ?
  Fe2 W2 As1 . . . 55(3) ?
  Fe2 W2 As1 . . 4_566 67(3) ?
  Fe2 W2 P1 . . . 55(3) ?
  Fe2 W2 P1 . . 4_566 67(3) ?
  Fe2 W2 O3 . . . 42(2) ?
  Fe2 W2 O3 . . 4_566 42(2) ?
  Fe2 W2 O4a . . . 120(3) ?
  Fe2 W2 O4a . . 4_566 121(3) ?
  Fe2 W2 O4b . . . 132(3) ?
  Fe2 W2 O4b . . 4_566 132(3) ?
  Fe2 W2 O5 . . . 63(2) ?
  Fe2 W2 O5 . . 4_566 101(3) ?
  Fe2 W2 As2 . . 6_556 162(3) ?
  Fe2 W2 As2 . . 7_555 152(3) ?
  Fe2 W2 As3 . . . 96(3) ?
  Fe2 W2 As3 . . 4_566 129(3) ?
  Fe2 W2 As3 . . 6_556 128(3) ?
  Fe2 W2 As3 . . 7_555 90(3) ?
  Fe2 W2 Ca . . 1_565 150(3) ?
  Fe2 W2 Ca . . 6_556 158(3) ?
  Fe2 W2 Fe2 6_546 . 6_556 166.3(7) ?
  Fe2 W2 W2 6_546 . 4_566 21(6) ?
  Fe2 W2 W2 6_546 . 6_546 6.6(4) ?
  Fe2 W2 W2 6_546 . 6_556 173.0(7) ?
  Fe2 W2 W2 6_546 . 7_555 6.6(4) ?
  Fe2 W2 W2 6_546 . 7_565 173.4(8) ?
  Fe2 W2 As1 6_546 . . 51.3(3) ?
  Fe2 W2 As1 6_546 . 4_566 116.1(6) ?
  Fe2 W2 P1 6_546 . . 51.3(3) ?
  Fe2 W2 P1 6_546 . 4_566 116.1(6) ?
  Fe2 W2 O3 6_546 . . 68.1(5) ?
  Fe2 W2 O3 6_546 . 4_566 93.9(7) ?
  Fe2 W2 O4a 6_546 . . 103.3(10) ?
  Fe2 W2 O4a 6_546 . 4_566 73.9(9) ?
  Fe2 W2 O4b 6_546 . . 103.6(9) ?
  Fe2 W2 O4b 6_546 . 4_566 77.5(8) ?
  Fe2 W2 O5 6_546 . . 20.8(4) ?
  Fe2 W2 O5 6_546 . 4_566 153.9(11) ?
  Fe2 W2 As2 6_546 . 6_556 97.7(6) ?
  Fe2 W2 As2 6_546 . 7_555 88.7(6) ?
  Fe2 W2 As3 6_546 . . 58.1(4) ?
  Fe2 W2 As3 6_546 . 4_566 123.9(7) ?
  Fe2 W2 As3 6_546 . 6_556 137.7(7) ?
  Fe2 W2 As3 6_546 . 7_555 46.0(3) ?
  Fe2 W2 Ca 6_546 . 1_565 143.3(6) ?
  Fe2 W2 Ca 6_546 . 6_556 94.0(5) ?
  Fe2 W2 W2 6_556 . 4_566 157(6) ?
  Fe2 W2 W2 6_556 . 6_546 172.5(8) ?
  Fe2 W2 W2 6_556 . 6_556 7.1(4) ?
  Fe2 W2 W2 6_556 . 7_555 172.9(7) ?
  Fe2 W2 W2 6_556 . 7_565 7.1(4) ?
  Fe2 W2 As1 6_556 . . 121.8(6) ?
  Fe2 W2 As1 6_556 . 4_566 54.6(3) ?
  Fe2 W2 P1 6_556 . . 121.8(6) ?
  Fe2 W2 P1 6_556 . 4_566 54.6(3) ?
  Fe2 W2 O3 6_556 . . 102.1(7) ?
  Fe2 W2 O3 6_556 . 4_566 74.5(6) ?
  Fe2 W2 O4a 6_556 . . 83.2(10) ?
  Fe2 W2 O4a 6_556 . 4_566 115.7(11) ?
  Fe2 W2 O4b 6_556 . . 85.4(9) ?
  Fe2 W2 O4b 6_556 . 4_566 114.0(10) ?
  Fe2 W2 O5 6_556 . . 153.1(10) ?
  Fe2 W2 O5 6_556 . 4_566 22.7(5) ?
  Fe2 W2 As2 6_556 . 6_556 95.9(6) ?
  Fe2 W2 As2 6_556 . 7_555 104.7(7) ?
  Fe2 W2 As3 6_556 . . 126.6(7) ?
  Fe2 W2 As3 6_556 . 4_566 64.0(4) ?
  Fe2 W2 As3 6_556 . 6_556 50.2(3) ?
  Fe2 W2 As3 6_556 . 7_555 138.6(7) ?
  Fe2 W2 Ca 6_556 . 1_565 50.2(4) ?
  Fe2 W2 Ca 6_556 . 6_556 99.5(6) ?
  W2 W2 W2 4_566 . 6_546 19(6) ?
  W2 W2 W2 4_566 . 6_556 158(6) ?
  W2 W2 W2 4_566 . 7_555 21(6) ?
  W2 W2 W2 4_566 . 7_565 159(6) ?
  W2 W2 As1 4_566 . . 71(6) ?
  W2 W2 As1 4_566 . 4_566 103(6) ?
  W2 W2 P1 4_566 . . 71(6) ?
  W2 W2 P1 4_566 . 4_566 103(6) ?
  W2 W2 O3 4_566 . . 86(6) ?
  W2 W2 O3 4_566 . 4_566 86(6) ?
  W2 W2 O4a 4_566 . . 83(6) ?
  W2 W2 O4a 4_566 . 4_566 86(6) ?
  W2 W2 O4b 4_566 . . 85(6) ?
  W2 W2 O4b 4_566 . 4_566 86(6) ?
  W2 W2 O5 4_566 . . 8(5) ?
  W2 W2 O5 4_566 . 4_566 171(6) ?
  W2 W2 As2 4_566 . 6_556 92(5) ?
  W2 W2 As2 4_566 . 7_555 81(5) ?
  W2 W2 As3 4_566 . . 38(6) ?
  W2 W2 As3 4_566 . 4_566 138(6) ?
  W2 W2 As3 4_566 . 6_556 151(6) ?
  W2 W2 As3 4_566 . 7_555 27(5) ?
  W2 W2 Ca 4_566 . 1_565 133(5) ?
  W2 W2 Ca 4_566 . 6_556 87(5) ?
  W2 W2 W2 6_546 . 6_556 176.6(9) ?
  W2 W2 W2 6_546 . 7_555 1.7(5) ?
  W2 W2 W2 6_546 . 7_565 178.3(9) ?
  W2 W2 As1 6_546 . . 55.7(5) ?
  W2 W2 As1 6_546 . 4_566 119.4(7) ?
  W2 W2 P1 6_546 . . 55.7(5) ?
  W2 W2 P1 6_546 . 4_566 119.4(7) ?
  W2 W2 O3 6_546 . . 73.8(6) ?
  W2 W2 O3 6_546 . 4_566 98.4(8) ?
  W2 W2 O4a 6_546 . . 98.9(11) ?
  W2 W2 O4a 6_546 . 4_566 70.5(9) ?
  W2 W2 O4b 6_546 . . 98.2(9) ?
  W2 W2 O4b 6_546 . 4_566 73.0(8) ?
  W2 W2 O5 6_546 . . 21.4(5) ?
  W2 W2 O5 6_546 . 4_566 158.0(11) ?
  W2 W2 As2 6_546 . 6_556 91.2(6) ?
  W2 W2 As2 6_546 . 7_555 82.1(6) ?
  W2 W2 As3 6_546 . . 54.1(5) ?
  W2 W2 As3 6_546 . 4_566 121.7(8) ?
  W2 W2 As3 6_546 . 6_556 135.6(8) ?
  W2 W2 As3 6_546 . 7_555 41.9(4) ?
  W2 W2 Ca 6_546 . 1_565 136.8(6) ?
  W2 W2 Ca 6_546 . 6_556 87.5(5) ?
  W2 W2 W2 6_556 . 7_555 178.3(9) ?
  W2 W2 W2 6_556 . 7_565 1.7(5) ?
  W2 W2 As1 6_556 . . 126.9(7) ?
  W2 W2 As1 6_556 . 4_566 57.9(5) ?
  W2 W2 P1 6_556 . . 126.9(7) ?
  W2 W2 P1 6_556 . 4_566 57.9(5) ?
  W2 W2 O3 6_556 . . 108.2(8) ?
  W2 W2 O3 6_556 . 4_566 79.4(7) ?
  W2 W2 O4a 6_556 . . 78.4(10) ?
  W2 W2 O4a 6_556 . 4_566 112.1(11) ?
  W2 W2 O4b 6_556 . . 79.6(9) ?
  W2 W2 O4b 6_556 . 4_566 109.1(10) ?
  W2 W2 O5 6_556 . . 155.4(11) ?
  W2 W2 O5 6_556 . 4_566 25.1(6) ?
  W2 W2 As2 6_556 . 6_556 88.9(6) ?
  W2 W2 As2 6_556 . 7_555 97.6(7) ?
  W2 W2 As3 6_556 . . 122.9(8) ?
  W2 W2 As3 6_556 . 4_566 61.2(5) ?
  W2 W2 As3 6_556 . 6_556 47.3(5) ?
  W2 W2 As3 6_556 . 7_555 135.1(8) ?
  W2 W2 Ca 6_556 . 1_565 43.2(4) ?
  W2 W2 Ca 6_556 . 6_556 92.4(5) ?
  W2 W2 W2 7_555 . 7_565 180.0(5) ?
  W2 W2 As1 7_555 . . 54.4(4) ?
  W2 W2 As1 7_555 . 4_566 120.7(7) ?
  W2 W2 P1 7_555 . . 54.4(4) ?
  W2 W2 P1 7_555 . 4_566 120.7(7) ?
  W2 W2 O3 7_555 . . 72.8(6) ?
  W2 W2 O3 7_555 . 4_566 99.5(7) ?
  W2 W2 O4a 7_555 . . 100.2(11) ?
  W2 W2 O4a 7_555 . 4_566 69.2(9) ?
  W2 W2 O4b 7_555 . . 99.3(9) ?
  W2 W2 O4b 7_555 . 4_566 71.9(8) ?
  W2 W2 O5 7_555 . . 23.0(5) ?
  W2 W2 O5 7_555 . 4_566 156.4(11) ?
  W2 W2 As2 7_555 . 6_556 91.1(6) ?
  W2 W2 As2 7_555 . 7_555 82.2(6) ?
  W2 W2 As3 7_555 . . 55.6(5) ?
  W2 W2 As3 7_555 . 4_566 120.2(8) ?
  W2 W2 As3 7_555 . 6_556 134.2(8) ?
  W2 W2 As3 7_555 . 7_555 43.4(4) ?
  W2 W2 Ca 7_555 . 1_565 136.8(6) ?
  W2 W2 Ca 7_555 . 6_556 87.5(5) ?
  W2 W2 As1 7_565 . . 125.6(7) ?
  W2 W2 As1 7_565 . 4_566 59.3(5) ?
  W2 W2 P1 7_565 . . 125.6(7) ?
  W2 W2 P1 7_565 . 4_566 59.3(5) ?
  W2 W2 O3 7_565 . . 107.2(8) ?
  W2 W2 O3 7_565 . 4_566 80.5(7) ?
  W2 W2 O4a 7_565 . . 79.8(10) ?
  W2 W2 O4a 7_565 . 4_566 110.8(12) ?
  W2 W2 O4b 7_565 . . 80.7(9) ?
  W2 W2 O4b 7_565 . 4_566 108.1(10) ?
  W2 W2 O5 7_565 . . 157.0(11) ?
  W2 W2 O5 7_565 . 4_566 23.6(6) ?
  W2 W2 As2 7_565 . 6_556 88.9(7) ?
  W2 W2 As2 7_565 . 7_555 97.8(7) ?
  W2 W2 As3 7_565 . . 124.4(8) ?
  W2 W2 As3 7_565 . 4_566 59.8(6) ?
  W2 W2 As3 7_565 . 6_556 45.8(5) ?
  W2 W2 As3 7_565 . 7_555 136.6(8) ?
  W2 W2 Ca 7_565 . 1_565 43.2(4) ?
  W2 W2 Ca 7_565 . 6_556 92.5(6) ?
  As1 W2 As1 . . 4_566 120.0(6) ?
  As1 W2 P1 . . . 0.0(5) ?
  As1 W2 P1 . . 4_566 120.0(6) ?
  As1 W2 O3 . . . 23.1(3) ?
  As1 W2 O3 . . 4_566 97.2(7) ?
  As1 W2 O4a . . . 154.6(12) ?
  As1 W2 O4a . . 4_566 66.4(9) ?
  As1 W2 O4b . . . 151.8(10) ?
  As1 W2 O4b . . 4_566 78.0(9) ?
  As1 W2 O5 . . . 68.8(6) ?
  As1 W2 O5 . . 4_566 102.7(9) ?
  As1 W2 As2 . . 6_556 118.8(8) ?
  As1 W2 As2 . . 7_555 117.1(7) ?
  As1 W2 As3 . . . 109.4(6) ?
  As1 W2 As3 . . 4_566 90.3(7) ?
  As1 W2 As3 . . 6_556 99.5(7) ?
  As1 W2 As3 . . 7_555 97.3(5) ?
  As1 W2 Ca . . 1_565 140.2(6) ?
  As1 W2 Ca . . 6_556 118.4(6) ?
  As1 W2 P1 4_566 . . 120.0(6) ?
  As1 W2 P1 4_566 . 4_566 0.0(5) ?
  As1 W2 O3 4_566 . . 99.6(7) ?
  As1 W2 O3 4_566 . 4_566 25.3(3) ?
  As1 W2 O4a 4_566 . . 69.0(10) ?
  As1 W2 O4a 4_566 . 4_566 169.9(12) ?
  As1 W2 O4b 4_566 . . 80.2(9) ?
  As1 W2 O4b 4_566 . 4_566 161.5(11) ?
  As1 W2 O5 4_566 . . 98.5(8) ?
  As1 W2 O5 4_566 . 4_566 73.3(7) ?
  As1 W2 As2 4_566 . 6_556 121.1(8) ?
  As1 W2 As2 4_566 . 7_555 120.9(8) ?
  As1 W2 As3 4_566 . . 88.2(6) ?
  As1 W2 As3 4_566 . 4_566 118.6(7) ?
  As1 W2 As3 4_566 . 6_556 104.8(5) ?
  As1 W2 As3 4_566 . 7_555 96.0(6) ?
  As1 W2 Ca 4_566 . 1_565 88.0(4) ?
  As1 W2 Ca 4_566 . 6_556 121.0(7) ?
  P1 W2 P1 . . 4_566 120.0(6) ?
  P1 W2 O3 . . . 23.1(3) ?
  P1 W2 O3 . . 4_566 97.2(7) ?
  P1 W2 O4a . . . 154.6(12) ?
  P1 W2 O4a . . 4_566 66.4(9) ?
  P1 W2 O4b . . . 151.8(10) ?
  P1 W2 O4b . . 4_566 78.0(9) ?
  P1 W2 O5 . . . 68.8(6) ?
  P1 W2 O5 . . 4_566 102.7(9) ?
  P1 W2 As2 . . 6_556 118.8(8) ?
  P1 W2 As2 . . 7_555 117.1(7) ?
  P1 W2 As3 . . . 109.4(6) ?
  P1 W2 As3 . . 4_566 90.3(7) ?
  P1 W2 As3 . . 6_556 99.5(7) ?
  P1 W2 As3 . . 7_555 97.3(5) ?
  P1 W2 Ca . . 1_565 140.2(6) ?
  P1 W2 Ca . . 6_556 118.4(6) ?
  P1 W2 O3 4_566 . . 99.6(7) ?
  P1 W2 O3 4_566 . 4_566 25.3(3) ?
  P1 W2 O4a 4_566 . . 69.0(10) ?
  P1 W2 O4a 4_566 . 4_566 169.9(12) ?
  P1 W2 O4b 4_566 . . 80.2(9) ?
  P1 W2 O4b 4_566 . 4_566 161.5(11) ?
  P1 W2 O5 4_566 . . 98.5(8) ?
  P1 W2 O5 4_566 . 4_566 73.3(7) ?
  P1 W2 As2 4_566 . 6_556 121.1(8) ?
  P1 W2 As2 4_566 . 7_555 120.9(8) ?
  P1 W2 As3 4_566 . . 88.2(6) ?
  P1 W2 As3 4_566 . 4_566 118.6(7) ?
  P1 W2 As3 4_566 . 6_556 104.8(5) ?
  P1 W2 As3 4_566 . 7_555 96.0(6) ?
  P1 W2 Ca 4_566 . 1_565 88.0(4) ?
  P1 W2 Ca 4_566 . 6_556 121.0(7) ?
  O3 W2 O3 . . 4_566 79.9(7) ?
  O3 W2 O4a . . . 161.7(15) ?
  O3 W2 O4a . . 4_566 84.9(12) ?
  O3 W2 O4b . . . 170.8(13) ?
  O3 W2 O4b . . 4_566 97.1(11) ?
  O3 W2 O5 . . . 80.7(7) ?
  O3 W2 O5 . . 4_566 86.7(9) ?
  O3 W2 As2 . . 6_556 138.6(11) ?
  O3 W2 As2 . . 7_555 139.3(10) ?
  O3 W2 As3 . . . 122.8(8) ?
  O3 W2 As3 . . 4_566 91.6(9) ?
  O3 W2 As3 . . 6_556 96.1(8) ?
  O3 W2 As3 . . 7_555 112.1(7) ?
  O3 W2 Ca . . 1_565 138.1(8) ?
  O3 W2 Ca . . 6_556 139.4(9) ?
  O3 W2 O4a 4_566 . . 84.8(12) ?
  O3 W2 O4a 4_566 . 4_566 163.3(14) ?
  O3 W2 O4b 4_566 . . 97.2(11) ?
  O3 W2 O4b 4_566 . 4_566 171.5(12) ?
  O3 W2 O5 4_566 . . 79.8(8) ?
  O3 W2 O5 4_566 . 4_566 87.9(9) ?
  O3 W2 As2 4_566 . 6_556 141.3(11) ?
  O3 W2 As2 4_566 . 7_555 136.9(11) ?
  O3 W2 As3 4_566 . . 85.6(8) ?
  O3 W2 As3 4_566 . 4_566 134.9(9) ?
  O3 W2 As3 4_566 . 6_556 122.7(8) ?
  O3 W2 As3 4_566 . 7_555 88.8(7) ?
  O3 W2 Ca 4_566 . 1_565 113.3(7) ?
  O3 W2 Ca 4_566 . 6_556 139.5(10) ?
  O4a W2 O4a . . 4_566 108.8(14) ?
  O4a W2 O4b . . . 12.4(8) ?
  O4a W2 O4b . . 4_566 96.6(13) ?
  O4a W2 O5 . . . 86.8(12) ?
  O4a W2 O5 . . 4_566 102.7(12) ?
  O4a W2 As2 . . 6_556 56.6(9) ?
  O4a W2 As2 . . 7_555 52.9(8) ?
  O4a W2 As3 . . . 45.3(8) ?
  O4a W2 As3 . . 4_566 106.3(11) ?
  O4a W2 As3 . . 6_556 100.6(10) ?
  O4a W2 As3 . . 7_555 57.3(9) ?
  O4a W2 Ca . . 1_565 58.0(9) ?
  O4a W2 Ca . . 6_556 54.7(8) ?
  O4a W2 O4b 4_566 . . 96.8(13) ?
  O4a W2 O4b 4_566 . 4_566 12.3(8) ?
  O4a W2 O5 4_566 . . 91.1(11) ?
  O4a W2 O5 4_566 . 4_566 98.1(13) ?
  O4a W2 As2 4_566 . 6_556 53.7(9) ?
  O4a W2 As2 4_566 . 7_555 55.9(9) ?
  O4a W2 As3 4_566 . . 97.1(10) ?
  O4a W2 As3 4_566 . 4_566 51.8(9) ?
  O4a W2 As3 4_566 . 6_556 65.5(9) ?
  O4a W2 As3 4_566 . 7_555 90.7(10) ?
  O4a W2 Ca 4_566 . 1_565 82.7(9) ?
  O4a W2 Ca 4_566 . 6_556 54.7(8) ?
  O4b W2 O4b . . 4_566 84.5(11) ?
  O4b W2 O5 . . . 90.2(11) ?
  O4b W2 O5 . . 4_566 102.0(11) ?
  O4b W2 As2 . . 6_556 44.2(7) ?
  O4b W2 As2 . . 7_555 41.0(7) ?
  O4b W2 As3 . . . 48.0(7) ?
  O4b W2 As3 . . 4_566 96.6(10) ?
  O4b W2 As3 . . 6_556 92.9(9) ?
  O4b W2 As3 . . 7_555 58.9(8) ?
  O4b W2 Ca . . 1_565 51.1(7) ?
  O4b W2 Ca . . 6_556 42.4(7) ?
  O4b W2 O5 4_566 . . 91.9(10) ?
  O4b W2 O5 4_566 . 4_566 100.0(12) ?
  O4b W2 As2 4_566 . 6_556 41.5(7) ?
  O4b W2 As2 4_566 . 7_555 43.7(7) ?
  O4b W2 As3 4_566 . . 89.4(9) ?
  O4b W2 As3 4_566 . 4_566 52.8(8) ?
  O4b W2 As3 4_566 . 6_556 65.4(8) ?
  O4b W2 As3 4_566 . 7_555 84.9(9) ?
  O4b W2 Ca 4_566 . 1_565 74.3(8) ?
  O4b W2 Ca 4_566 . 6_556 42.4(7) ?
  O5 W2 O5 . . 4_566 163.7(12) ?
  O5 W2 As2 . . 6_556 99.3(8) ?
  O5 W2 As2 . . 7_555 88.7(8) ?
  O5 W2 As3 . . . 42.2(5) ?
  O5 W2 As3 . . 4_566 142.8(10) ?
  O5 W2 As3 . . 6_556 156.6(10) ?
  O5 W2 As3 . . 7_555 31.6(5) ?
  O5 W2 Ca . . 1_565 139.2(8) ?
  O5 W2 Ca . . 6_556 94.9(7) ?
  O5 W2 As2 4_566 . 6_556 97.0(9) ?
  O5 W2 As2 4_566 . 7_555 107.6(9) ?
  O5 W2 As3 4_566 . . 147.8(11) ?
  O5 W2 As3 4_566 . 4_566 47.2(6) ?
  O5 W2 As3 4_566 . 6_556 35.0(6) ?
  O5 W2 As3 4_566 . 7_555 160.0(11) ?
  O5 W2 Ca 4_566 . 1_565 55.9(6) ?
  O5 W2 Ca 4_566 . 6_556 101.4(8) ?
  As2 W2 As2 6_556 . 7_555 10.9(2) ?
  As2 W2 As3 6_556 . . 70.0(6) ?
  As2 W2 As3 6_556 . 4_566 63.4(5) ?
  As2 W2 As3 6_556 . 6_556 67.9(5) ?
  As2 W2 As3 6_556 . 7_555 73.7(5) ?
  As2 W2 Ca 6_556 . 1_565 45.8(4) ?
  As2 W2 Ca 6_556 . 6_556 4.6(2) ?
  As2 W2 As3 7_555 . . 59.7(5) ?
  As2 W2 As3 7_555 . 4_566 73.6(6) ?
  As2 W2 As3 7_555 . 6_556 78.7(6) ?
  As2 W2 As3 7_555 . 7_555 62.9(5) ?
  As2 W2 Ca 7_555 . 1_565 54.7(4) ?
  As2 W2 Ca 7_555 . 6_556 6.3(2) ?
  As3 W2 As3 . . 4_566 133.3(8) ?
  As3 W2 As3 . . 6_556 136.6(7) ?
  As3 W2 As3 . . 7_555 12.18(18) ?
  As3 W2 Ca . . 1_565 98.4(5) ?
  As3 W2 Ca . . 6_556 65.6(4) ?
  As3 W2 As3 4_566 . 6_556 13.9(2) ?
  As3 W2 As3 4_566 . 7_555 134.4(7) ?
  As3 W2 Ca 4_566 . 1_565 50.1(4) ?
  As3 W2 Ca 4_566 . 6_556 67.8(5) ?
  As3 W2 As3 6_556 . 7_555 141.6(7) ?
  As3 W2 Ca 6_556 . 1_565 42.7(3) ?
  As3 W2 Ca 6_556 . 6_556 72.4(4) ?
  As3 W2 Ca 7_555 . 1_565 107.9(5) ?
  As3 W2 Ca 7_555 . 6_556 69.2(4) ?
  Ca W2 Ca 1_565 . 6_556 49.3(3) ?
  Fe1 As1 Fe2 . . . 71.3(3) ?
  Fe1 As1 Fe2 . . 6_546 71.3(3) ?
  Fe1 As1 W2 . . . 64.7(3) ?
  Fe1 As1 W2 . . 4_566 64.2(4) ?
  Fe1 As1 W2 . . 6_546 64.2(4) ?
  Fe1 As1 W2 . . 7_555 64.7(3) ?
  Fe1 As1 P1 . . . 0 ?
  Fe1 As1 O1 . . . 138.9(6) ?
  Fe1 As1 O2 . . . 27.2(4) ?
  Fe1 As1 O3 . . . 92.9(4) ?
  Fe1 As1 O3 . . 7_555 92.9(4) ?
  Fe1 As1 Ca . . 10_554 62.2(3) ?
  Fe1 As1 Ca . . 13_555 62.2(3) ?
  Fe1 As1 Fe3 . . . 139.37(15) ?
  Fe1 As1 Fe3 . . 2_655 139.37(15) ?
  Fe2 As1 Fe2 . . 6_546 71.07(13) ?
  Fe2 As1 W2 . . . 6.9(4) ?
  Fe2 As1 W2 . . 4_566 7.7(4) ?
  Fe2 As1 W2 . . 6_546 66.6(4) ?
  Fe2 As1 W2 . . 7_555 71.6(4) ?
  Fe2 As1 P1 . . . 0 ?
  Fe2 As1 O1 . . . 137.2(4) ?
  Fe2 As1 O2 . . . 93.2(5) ?
  Fe2 As1 O3 . . . 27.2(4) ?
  Fe2 As1 O3 . . 7_555 93.3(3) ?
  Fe2 As1 Ca . . 10_554 133.3(4) ?
  Fe2 As1 Ca . . 13_555 96.3(2) ?
  Fe2 As1 Fe3 . . . 123.6(3) ?
  Fe2 As1 Fe3 . . 2_655 146.8(3) ?
  Fe2 As1 W2 6_546 . . 71.6(4) ?
  Fe2 As1 W2 6_546 . 4_566 66.6(4) ?
  Fe2 As1 W2 6_546 . 6_546 7.7(4) ?
  Fe2 As1 W2 6_546 . 7_555 6.9(4) ?
  Fe2 As1 P1 6_546 . . 0 ?
  Fe2 As1 O1 6_546 . . 137.2(4) ?
  Fe2 As1 O2 6_546 . . 93.2(5) ?
  Fe2 As1 O3 6_546 . . 93.3(3) ?
  Fe2 As1 O3 6_546 . 7_555 27.2(4) ?
  Fe2 As1 Ca 6_546 . 10_554 96.3(2) ?
  Fe2 As1 Ca 6_546 . 13_555 133.3(4) ?
  Fe2 As1 Fe3 6_546 . . 146.8(3) ?
  Fe2 As1 Fe3 6_546 . 2_655 123.6(3) ?
  W2 As1 W2 . . 4_566 5.0(5) ?
  W2 As1 W2 . . 6_546 66.3(5) ?
  W2 As1 W2 . . 7_555 71.2(5) ?
  W2 As1 P1 . . . 0 ?
  W2 As1 O1 . . . 141.0(4) ?
  W2 As1 O2 . . . 86.3(5) ?
  W2 As1 O3 . . . 31.6(5) ?
  W2 As1 O3 . . 7_555 95.5(5) ?
  W2 As1 Ca . . 10_554 126.5(5) ?
  W2 As1 Ca . . 13_555 91.0(4) ?
  W2 As1 Fe3 . . . 126.8(4) ?
  W2 As1 Fe3 . . 2_655 152.2(4) ?
  W2 As1 W2 4_566 . 6_546 61.4(5) ?
  W2 As1 W2 4_566 . 7_555 66.3(5) ?
  W2 As1 P1 4_566 . . 0 ?
  W2 As1 O1 4_566 . . 144.6(4) ?
  W2 As1 O2 4_566 . . 87.2(5) ?
  W2 As1 O3 4_566 . . 34.7(5) ?
  W2 As1 O3 4_566 . 7_555 90.5(5) ?
  W2 As1 Ca 4_566 . 10_554 126.3(5) ?
  W2 As1 Ca 4_566 . 13_555 95.0(4) ?
  W2 As1 Fe3 4_566 . . 130.8(4) ?
  W2 As1 Fe3 4_566 . 2_655 154.5(4) ?
  W2 As1 W2 6_546 . 7_555 5.0(5) ?
  W2 As1 P1 6_546 . . 0 ?
  W2 As1 O1 6_546 . . 144.6(4) ?
  W2 As1 O2 6_546 . . 87.2(5) ?
  W2 As1 O3 6_546 . . 90.5(5) ?
  W2 As1 O3 6_546 . 7_555 34.7(5) ?
  W2 As1 Ca 6_546 . 10_554 95.0(4) ?
  W2 As1 Ca 6_546 . 13_555 126.3(5) ?
  W2 As1 Fe3 6_546 . . 154.5(4) ?
  W2 As1 Fe3 6_546 . 2_655 130.8(4) ?
  W2 As1 P1 7_555 . . 0 ?
  W2 As1 O1 7_555 . . 141.0(4) ?
  W2 As1 O2 7_555 . . 86.3(5) ?
  W2 As1 O3 7_555 . . 95.5(5) ?
  W2 As1 O3 7_555 . 7_555 31.6(5) ?
  W2 As1 Ca 7_555 . 10_554 91.0(4) ?
  W2 As1 Ca 7_555 . 13_555 126.5(5) ?
  W2 As1 Fe3 7_555 . . 152.2(4) ?
  W2 As1 Fe3 7_555 . 2_655 126.8(4) ?
  P1 As1 O1 . . . 0 ?
  P1 As1 O2 . . . 0 ?
  P1 As1 O3 . . . 0 ?
  P1 As1 O3 . . 7_555 0 ?
  P1 As1 Ca . . 10_554 0 ?
  P1 As1 Ca . . 13_555 0 ?
  P1 As1 Fe3 . . . 0 ?
  P1 As1 Fe3 . . 2_655 0 ?
  O1 As1 O2 . . . 111.7(7) ?
  O1 As1 O3 . . . 110.0(5) ?
  O1 As1 O3 . . 7_555 110.0(5) ?
  O1 As1 Ca . . 10_554 82.6(6) ?
  O1 As1 Ca . . 13_555 82.6(6) ?
  O1 As1 Fe3 . . . 14.4(2) ?
  O1 As1 Fe3 . . 2_655 14.4(2) ?
  O2 As1 O3 . . . 108.0(4) ?
  O2 As1 O3 . . 7_555 108.0(4) ?
  O2 As1 Ca . . 10_554 41.4(4) ?
  O2 As1 Ca . . 13_555 41.4(4) ?
  O2 As1 Fe3 . . . 113.5(5) ?
  O2 As1 Fe3 . . 2_655 113.5(5) ?
  O3 As1 O3 . . 7_555 109.0(4) ?
  O3 As1 Ca . . 10_554 148.3(4) ?
  O3 As1 Ca . . 13_555 92.5(3) ?
  O3 As1 Fe3 . . . 96.4(4) ?
  O3 As1 Fe3 . . 2_655 120.6(4) ?
  O3 As1 Ca 7_555 . 10_554 92.5(3) ?
  O3 As1 Ca 7_555 . 13_555 148.3(4) ?
  O3 As1 Fe3 7_555 . . 120.6(4) ?
  O3 As1 Fe3 7_555 . 2_655 96.4(4) ?
  Ca As1 Ca 10_554 . 13_555 59.35(12) ?
  Ca As1 Fe3 10_554 . . 91.9(3) ?
  Ca As1 Fe3 10_554 . 2_655 78.0(3) ?
  Ca As1 Fe3 13_555 . . 78.0(3) ?
  Ca As1 Fe3 13_555 . 2_655 91.9(3) ?
  Fe3 As1 Fe3 . . 2_655 28.3(2) ?
  Fe1 P1 Fe2 . . . 71.3(3) ?
  Fe1 P1 Fe2 . . 6_546 71.3(3) ?
  Fe1 P1 W2 . . . 64.7(3) ?
  Fe1 P1 W2 . . 4_566 64.2(4) ?
  Fe1 P1 W2 . . 6_546 64.2(4) ?
  Fe1 P1 W2 . . 7_555 64.7(3) ?
  Fe1 P1 As1 . . . 0 ?
  Fe1 P1 O1 . . . 138.9(6) ?
  Fe1 P1 O2 . . . 27.2(4) ?
  Fe1 P1 O3 . . . 92.9(4) ?
  Fe1 P1 O3 . . 7_555 92.9(4) ?
  Fe1 P1 Ca . . 10_554 62.2(3) ?
  Fe1 P1 Ca . . 13_555 62.2(3) ?
  Fe1 P1 Fe3 . . . 139.37(15) ?
  Fe1 P1 Fe3 . . 2_655 139.37(15) ?
  Fe2 P1 Fe2 . . 6_546 71.07(13) ?
  Fe2 P1 W2 . . . 6.9(4) ?
  Fe2 P1 W2 . . 4_566 7.7(4) ?
  Fe2 P1 W2 . . 6_546 66.6(4) ?
  Fe2 P1 W2 . . 7_555 71.6(4) ?
  Fe2 P1 As1 . . . 0 ?
  Fe2 P1 O1 . . . 137.2(4) ?
  Fe2 P1 O2 . . . 93.2(5) ?
  Fe2 P1 O3 . . . 27.2(4) ?
  Fe2 P1 O3 . . 7_555 93.3(3) ?
  Fe2 P1 Ca . . 10_554 133.3(4) ?
  Fe2 P1 Ca . . 13_555 96.3(2) ?
  Fe2 P1 Fe3 . . . 123.6(3) ?
  Fe2 P1 Fe3 . . 2_655 146.8(3) ?
  Fe2 P1 W2 6_546 . . 71.6(4) ?
  Fe2 P1 W2 6_546 . 4_566 66.6(4) ?
  Fe2 P1 W2 6_546 . 6_546 7.7(4) ?
  Fe2 P1 W2 6_546 . 7_555 6.9(4) ?
  Fe2 P1 As1 6_546 . . 0 ?
  Fe2 P1 O1 6_546 . . 137.2(4) ?
  Fe2 P1 O2 6_546 . . 93.2(5) ?
  Fe2 P1 O3 6_546 . . 93.3(3) ?
  Fe2 P1 O3 6_546 . 7_555 27.2(4) ?
  Fe2 P1 Ca 6_546 . 10_554 96.3(2) ?
  Fe2 P1 Ca 6_546 . 13_555 133.3(4) ?
  Fe2 P1 Fe3 6_546 . . 146.8(3) ?
  Fe2 P1 Fe3 6_546 . 2_655 123.6(3) ?
  W2 P1 W2 . . 4_566 5.0(5) ?
  W2 P1 W2 . . 6_546 66.3(5) ?
  W2 P1 W2 . . 7_555 71.2(5) ?
  W2 P1 As1 . . . 0 ?
  W2 P1 O1 . . . 141.0(4) ?
  W2 P1 O2 . . . 86.3(5) ?
  W2 P1 O3 . . . 31.6(5) ?
  W2 P1 O3 . . 7_555 95.5(5) ?
  W2 P1 Ca . . 10_554 126.5(5) ?
  W2 P1 Ca . . 13_555 91.0(4) ?
  W2 P1 Fe3 . . . 126.8(4) ?
  W2 P1 Fe3 . . 2_655 152.2(4) ?
  W2 P1 W2 4_566 . 6_546 61.4(5) ?
  W2 P1 W2 4_566 . 7_555 66.3(5) ?
  W2 P1 As1 4_566 . . 0 ?
  W2 P1 O1 4_566 . . 144.6(4) ?
  W2 P1 O2 4_566 . . 87.2(5) ?
  W2 P1 O3 4_566 . . 34.7(5) ?
  W2 P1 O3 4_566 . 7_555 90.5(5) ?
  W2 P1 Ca 4_566 . 10_554 126.3(5) ?
  W2 P1 Ca 4_566 . 13_555 95.0(4) ?
  W2 P1 Fe3 4_566 . . 130.8(4) ?
  W2 P1 Fe3 4_566 . 2_655 154.5(4) ?
  W2 P1 W2 6_546 . 7_555 5.0(5) ?
  W2 P1 As1 6_546 . . 0 ?
  W2 P1 O1 6_546 . . 144.6(4) ?
  W2 P1 O2 6_546 . . 87.2(5) ?
  W2 P1 O3 6_546 . . 90.5(5) ?
  W2 P1 O3 6_546 . 7_555 34.7(5) ?
  W2 P1 Ca 6_546 . 10_554 95.0(4) ?
  W2 P1 Ca 6_546 . 13_555 126.3(5) ?
  W2 P1 Fe3 6_546 . . 154.5(4) ?
  W2 P1 Fe3 6_546 . 2_655 130.8(4) ?
  W2 P1 As1 7_555 . . 0 ?
  W2 P1 O1 7_555 . . 141.0(4) ?
  W2 P1 O2 7_555 . . 86.3(5) ?
  W2 P1 O3 7_555 . . 95.5(5) ?
  W2 P1 O3 7_555 . 7_555 31.6(5) ?
  W2 P1 Ca 7_555 . 10_554 91.0(4) ?
  W2 P1 Ca 7_555 . 13_555 126.5(5) ?
  W2 P1 Fe3 7_555 . . 152.2(4) ?
  W2 P1 Fe3 7_555 . 2_655 126.8(4) ?
  As1 P1 O1 . . . 0 ?
  As1 P1 O2 . . . 0 ?
  As1 P1 O3 . . . 0 ?
  As1 P1 O3 . . 7_555 0 ?
  As1 P1 Ca . . 10_554 0 ?
  As1 P1 Ca . . 13_555 0 ?
  As1 P1 Fe3 . . . 0 ?
  As1 P1 Fe3 . . 2_655 0 ?
  O1 P1 O2 . . . 111.7(7) ?
  O1 P1 O3 . . . 110.0(5) ?
  O1 P1 O3 . . 7_555 110.0(5) ?
  O1 P1 Ca . . 10_554 82.6(6) ?
  O1 P1 Ca . . 13_555 82.6(6) ?
  O1 P1 Fe3 . . . 14.4(2) ?
  O1 P1 Fe3 . . 2_655 14.4(2) ?
  O2 P1 O3 . . . 108.0(4) ?
  O2 P1 O3 . . 7_555 108.0(4) ?
  O2 P1 Ca . . 10_554 41.4(4) ?
  O2 P1 Ca . . 13_555 41.4(4) ?
  O2 P1 Fe3 . . . 113.5(5) ?
  O2 P1 Fe3 . . 2_655 113.5(5) ?
  O3 P1 O3 . . 7_555 109.0(4) ?
  O3 P1 Ca . . 10_554 148.3(4) ?
  O3 P1 Ca . . 13_555 92.5(3) ?
  O3 P1 Fe3 . . . 96.4(4) ?
  O3 P1 Fe3 . . 2_655 120.6(4) ?
  O3 P1 Ca 7_555 . 10_554 92.5(3) ?
  O3 P1 Ca 7_555 . 13_555 148.3(4) ?
  O3 P1 Fe3 7_555 . . 120.6(4) ?
  O3 P1 Fe3 7_555 . 2_655 96.4(4) ?
  Ca P1 Ca 10_554 . 13_555 59.35(12) ?
  Ca P1 Fe3 10_554 . . 91.9(3) ?
  Ca P1 Fe3 10_554 . 2_655 78.0(3) ?
  Ca P1 Fe3 13_555 . . 78.0(3) ?
  Ca P1 Fe3 13_555 . 2_655 91.9(3) ?
  Fe3 P1 Fe3 . . 2_655 28.3(2) ?
  As1 O1 P1 . . . 0.0(5) ?
  As1 O1 Fe3 . . . 152.6(4) ?
  As1 O1 Fe3 . . 2_655 152.6(4) ?
  P1 O1 Fe3 . . . 152.6(4) ?
  P1 O1 Fe3 . . 2_655 152.6(4) ?
  Fe3 O1 Fe3 . . 2_655 54.0(6) ?
  Fe1 O2 As1 . . . 130.1(7) ?
  Fe1 O2 P1 . . . 130.1(7) ?
  Fe1 O2 Ca . . 10_554 100.7(6) ?
  Fe1 O2 Ca . . 13_555 100.7(6) ?
  As1 O2 P1 . . . 0.0(5) ?
  As1 O2 Ca . . 10_554 115.1(6) ?
  As1 O2 Ca . . 13_555 115.1(6) ?
  P1 O2 Ca . . 10_554 115.1(6) ?
  P1 O2 Ca . . 13_555 115.1(6) ?
  Ca O2 Ca 10_554 . 13_555 85.4(3) ?
  Fe2 O3 W2 . . . 9.5(7) ?
  Fe2 O3 W2 . . 4_566 9.6(6) ?
  Fe2 O3 As1 . . . 129.0(6) ?
  Fe2 O3 P1 . . . 129.0(6) ?
  W2 O3 W2 . . 4_566 8.0(7) ?
  W2 O3 As1 . . . 125.3(7) ?
  W2 O3 P1 . . . 125.3(7) ?
  W2 O3 As1 4_566 . . 120.0(7) ?
  W2 O3 P1 4_566 . . 120.0(7) ?
  As1 O3 P1 . . . 0.0(5) ?
  Fe1 O4a Fe2 10_565 . . 143.7(10) ?
  Fe1 O4a W2 10_565 . . 145.0(13) ?
  Fe1 O4a W2 10_565 . 4_566 154.5(13) ?
  Fe1 O4a O4b 10_565 . . 73(3) ?
  Fe1 O4a As2 10_565 . 6_556 106.9(8) ?
  Fe1 O4a As2 10_565 . 7_555 110.5(9) ?
  Fe1 O4a As3 10_565 . . 113.2(8) ?
  Fe1 O4a Ca 10_565 . 6_556 98.1(7) ?
  Fe2 O4a W2 . . . 12.1(8) ?
  Fe2 O4a W2 . . 4_566 12.0(8) ?
  Fe2 O4a O4b . . . 133(3) ?
  Fe2 O4a As2 . . 6_556 93.6(8) ?
  Fe2 O4a As2 . . 7_555 96.3(9) ?
  Fe2 O4a As3 . . . 93.8(8) ?
  Fe2 O4a Ca . . 6_556 107.0(8) ?
  W2 O4a W2 . . 4_566 10.8(10) ?
  W2 O4a O4b . . . 122(3) ?
  W2 O4a As2 . . 6_556 82.2(10) ?
  W2 O4a As2 . . 7_555 86.1(11) ?
  W2 O4a As3 . . . 99.0(11) ?
  W2 O4a Ca . . 6_556 96.1(11) ?
  W2 O4a O4b 4_566 . . 123(3) ?
  W2 O4a As2 4_566 . 6_556 83.6(11) ?
  W2 O4a As2 4_566 . 7_555 85.1(11) ?
  W2 O4a As3 4_566 . . 88.2(11) ?
  W2 O4a Ca 4_566 . 6_556 96.2(11) ?
  O4b O4a As2 . . 6_556 40(3) ?
  O4b O4a As2 . . 7_555 38(3) ?
  O4b O4a As3 . . . 91(3) ?
  O4b O4a Ca . . 6_556 27(3) ?
  As2 O4a As2 6_556 . 7_555 13.1(3) ?
  As2 O4a As3 6_556 . . 95.4(8) ?
  As2 O4a Ca 6_556 . 6_556 14.7(3) ?
  As2 O4a As3 7_555 . . 82.5(7) ?
  As2 O4a Ca 7_555 . 6_556 12.4(3) ?
  As3 O4a Ca . . 6_556 88.4(7) ?
  Fe1 O4b Fe2 10_565 . . 125.0(9) ?
  Fe1 O4b W2 10_565 . . 128.6(11) ?
  Fe1 O4b W2 10_565 . 4_566 133.7(11) ?
  Fe1 O4b O4a 10_565 . . 93(3) ?
  Fe1 O4b As2 10_565 . 6_556 128.0(10) ?
  Fe1 O4b As2 10_565 . 7_555 134.7(10) ?
  Fe1 O4b As3 10_565 . . 114.1(9) ?
  Fe1 O4b Ca 10_565 . 6_556 117.0(8) ?
  Fe2 O4b W2 . . . 8.7(7) ?
  Fe2 O4b W2 . . 4_566 8.7(6) ?
  Fe2 O4b O4a . . . 38(3) ?
  Fe2 O4b As2 . . 6_556 92.2(9) ?
  Fe2 O4b As2 . . 7_555 94.6(9) ?
  Fe2 O4b As3 . . . 82.1(6) ?
  Fe2 O4b Ca . . 6_556 110.6(9) ?
  W2 O4b W2 . . 4_566 9.1(8) ?
  W2 O4b O4a . . . 46(3) ?
  W2 O4b As2 . . 6_556 84.2(11) ?
  W2 O4b As2 . . 7_555 87.9(11) ?
  W2 O4b As3 . . . 87.6(9) ?
  W2 O4b Ca . . 6_556 103.0(11) ?
  W2 O4b O4a 4_566 . . 45(3) ?
  W2 O4b As2 4_566 . 6_556 85.4(11) ?
  W2 O4b As2 4_566 . 7_555 86.6(11) ?
  W2 O4b As3 4_566 . . 78.6(9) ?
  W2 O4b Ca 4_566 . 6_556 103.0(11) ?
  O4a O4b As2 . . 6_556 130(3) ?
  O4a O4b As2 . . 7_555 131(3) ?
  O4a O4b As3 . . . 75(3) ?
  O4a O4b Ca . . 6_556 148(3) ?
  As2 O4b As2 6_556 . 7_555 15.8(4) ?
  As2 O4b As3 6_556 . . 105.0(9) ?
  As2 O4b Ca 6_556 . 6_556 19.8(4) ?
  As2 O4b As3 7_555 . . 89.9(9) ?
  As2 O4b Ca 7_555 . 6_556 17.7(4) ?
  As3 O4b Ca . . 6_556 99.6(8) ?
  Fe2 O5 Fe2 . . 6_546 135.4(6) ?
  Fe2 O5 W2 . . . 12.0(7) ?
  Fe2 O5 W2 . . 4_566 13.2(8) ?
  Fe2 O5 W2 . . 6_546 136.3(9) ?
  Fe2 O5 W2 . . 7_555 136.5(8) ?
  Fe2 O5 As3 . . . 95.2(5) ?
  Fe2 O5 As3 . . 7_555 120.8(6) ?
  Fe2 O5 W2 6_546 . . 136.5(8) ?
  Fe2 O5 W2 6_546 . 4_566 136.3(9) ?
  Fe2 O5 W2 6_546 . 6_546 13.2(8) ?
  Fe2 O5 W2 6_546 . 7_555 12.0(7) ?
  Fe2 O5 As3 6_546 . . 120.8(6) ?
  Fe2 O5 As3 6_546 . 7_555 95.2(5) ?
  W2 O5 W2 . . 4_566 1.3(8) ?
  W2 O5 W2 . . 6_546 133.5(11) ?
  W2 O5 W2 . . 7_555 134.0(10) ?
  W2 O5 As3 . . . 86.6(7) ?
  W2 O5 As3 . . 7_555 111.1(7) ?
  W2 O5 W2 4_566 . 6_546 132.8(12) ?
  W2 O5 W2 4_566 . 7_555 133.5(11) ?
  W2 O5 As3 4_566 . . 85.9(8) ?
  W2 O5 As3 4_566 . 7_555 110.2(8) ?
  W2 O5 W2 6_546 . 7_555 1.3(8) ?
  W2 O5 As3 6_546 . . 110.2(8) ?
  W2 O5 As3 6_546 . 7_555 85.9(8) ?
  W2 O5 As3 7_555 . . 111.1(7) ?
  W2 O5 As3 7_555 . 7_555 86.6(7) ?
  As3 O5 As3 . . 7_555 26.3(3) ?
  Fe1 As2 Fe1 . . 10_555 147.3(2) ?
  Fe1 As2 Fe2 . . 6_546 73.95(15) ?
  Fe1 As2 W2 . . 6_546 73.2(5) ?
  Fe1 As2 W2 . . 7_555 74.7(5) ?
  Fe1 As2 O4a . . 6_546 36.1(5) ?
  Fe1 As2 O4a . . 7_555 114.3(6) ?
  Fe1 As2 O4b . . 6_546 27.6(6) ?
  Fe1 As2 O4b . . 7_555 125.0(7) ?
  Fe1 As2 As2 . . 4_556 86.5(12) ?
  Fe1 As2 As2 . . 7_555 59.93(17) ?
  Fe1 As2 As3 . . . 91.6(2) ?
  Fe1 As2 As3 . . 4_556 75.49(17) ?
  Fe1 As2 As3 . . 13_556 122.6(2) ?
  Fe1 As2 As3 . . 6_546 64.15(17) ?
  Fe1 As2 As3 . . 7_555 101.3(2) ?
  Fe1 As2 Ca . . . 104.3(5) ?
  Fe1 As2 Ca . . 6_546 121.3(2) ?
  Fe1 As2 Ca . . 6_556 63.18(19) ?
  Fe1 As2 O6 . . . 90.1(5) ?
  Fe1 As2 O6 . . 4_556 91.3(4) ?
  Fe1 As2 Fe2 10_555 . 6_546 73.87(15) ?
  Fe1 As2 W2 10_555 . 6_546 74.9(5) ?
  Fe1 As2 W2 10_555 . 7_555 72.8(5) ?
  Fe1 As2 O4a 10_555 . 6_546 111.5(5) ?
  Fe1 As2 O4a 10_555 . 7_555 35.2(5) ?
  Fe1 As2 O4b 10_555 . 6_546 120.8(7) ?
  Fe1 As2 O4b 10_555 . 7_555 24.7(6) ?
  Fe1 As2 As2 10_555 . 4_556 85.3(12) ?
  Fe1 As2 As2 10_555 . 7_555 128.1(2) ?
  Fe1 As2 As3 10_555 . . 81.44(19) ?
  Fe1 As2 As3 10_555 . 4_556 84.43(18) ?
  Fe1 As2 As3 10_555 . 13_556 61.18(16) ?
  Fe1 As2 As3 10_555 . 6_546 93.4(2) ?
  Fe1 As2 As3 10_555 . 7_555 67.9(2) ?
  Fe1 As2 Ca 10_555 . . 104.0(5) ?
  Fe1 As2 Ca 10_555 . 6_546 58.84(18) ?
  Fe1 As2 Ca 10_555 . 6_556 133.7(2) ?
  Fe1 As2 O6 10_555 . . 100.6(5) ?
  Fe1 As2 O6 10_555 . 4_556 82.6(4) ?
  Fe2 As2 W2 6_546 . 6_546 2.8(4) ?
  Fe2 As2 W2 6_546 . 7_555 4.3(5) ?
  Fe2 As2 O4a 6_546 . 6_546 41.0(5) ?
  Fe2 As2 O4a 6_546 . 7_555 40.8(5) ?
  Fe2 As2 O4b 6_546 . 6_546 51.5(6) ?
  Fe2 As2 O4b 6_546 . 7_555 51.3(6) ?
  Fe2 As2 As2 6_546 . 4_556 85.4(11) ?
  Fe2 As2 As2 6_546 . 7_555 93.8(2) ?
  Fe2 As2 As3 6_546 . . 67.63(19) ?
  Fe2 As2 As3 6_546 . 4_556 61.84(17) ?
  Fe2 As2 As3 6_546 . 13_556 87.2(2) ?
  Fe2 As2 As3 6_546 . 6_546 57.58(18) ?
  Fe2 As2 As3 6_546 . 7_555 61.8(2) ?
  Fe2 As2 Ca 6_546 . . 160.2(7) ?
  Fe2 As2 Ca 6_546 . 6_546 98.7(4) ?
  Fe2 As2 Ca 6_546 . 6_556 107.6(4) ?
  Fe2 As2 O6 6_546 . . 99.4(6) ?
  Fe2 As2 O6 6_546 . 4_556 89.2(5) ?
  W2 As2 W2 6_546 . 7_555 7.1(6) ?
  W2 As2 O4a 6_546 . 6_546 41.2(7) ?
  W2 As2 O4a 6_546 . 7_555 41.2(7) ?
  W2 As2 O4b 6_546 . 6_546 51.6(8) ?
  W2 As2 O4b 6_546 . 7_555 51.9(8) ?
  W2 As2 As2 6_546 . 4_556 88.0(12) ?
  W2 As2 As2 6_546 . 7_555 91.1(5) ?
  W2 As2 As3 6_546 . . 65.1(5) ?
  W2 As2 As3 6_546 . 4_556 64.4(5) ?
  W2 As2 As3 6_546 . 13_556 85.5(6) ?
  W2 As2 As3 6_546 . 6_546 59.8(5) ?
  W2 As2 As3 6_546 . 7_555 59.6(6) ?
  W2 As2 Ca 6_546 . . 162.8(8) ?
  W2 As2 Ca 6_546 . 6_546 101.4(6) ?
  W2 As2 Ca 6_546 . 6_556 105.0(6) ?
  W2 As2 O6 6_546 . . 96.7(8) ?
  W2 As2 O6 6_546 . 4_556 91.9(7) ?
  W2 As2 O4a 7_555 . 6_546 40.5(7) ?
  W2 As2 O4a 7_555 . 7_555 40.9(7) ?
  W2 As2 O4b 7_555 . 6_546 50.9(8) ?
  W2 As2 O4b 7_555 . 7_555 51.1(8) ?
  W2 As2 As2 7_555 . 4_556 81.1(12) ?
  W2 As2 As2 7_555 . 7_555 97.8(5) ?
  W2 As2 As3 7_555 . . 71.7(5) ?
  W2 As2 As3 7_555 . 4_556 57.7(5) ?
  W2 As2 As3 7_555 . 13_556 90.3(6) ?
  W2 As2 As3 7_555 . 6_546 53.9(5) ?
  W2 As2 As3 7_555 . 7_555 65.5(6) ?
  W2 As2 Ca 7_555 . . 155.9(8) ?
  W2 As2 Ca 7_555 . 6_546 94.6(6) ?
  W2 As2 Ca 7_555 . 6_556 111.5(6) ?
  W2 As2 O6 7_555 . . 103.7(8) ?
  W2 As2 O6 7_555 . 4_556 84.9(7) ?
  O4a As2 O4a 6_546 . 7_555 81.5(7) ?
  O4a As2 O4b 6_546 . 6_546 10.5(8) ?
  O4a As2 O4b 6_546 . 7_555 91.6(8) ?
  O4a As2 As2 6_546 . 4_556 73.2(12) ?
  O4a As2 As2 6_546 . 7_555 83.3(5) ?
  O4a As2 As3 6_546 . . 89.2(5) ?
  O4a As2 As3 6_546 . 4_556 52.3(5) ?
  O4a As2 As3 6_546 . 13_556 119.2(6) ?
  O4a As2 As3 6_546 . 6_546 41.2(5) ?
  O4a As2 As3 6_546 . 7_555 91.2(6) ?
  O4a As2 Ca 6_546 . . 129.2(8) ?
  O4a As2 Ca 6_546 . 6_546 104.5(6) ?
  O4a As2 Ca 6_546 . 6_556 92.2(6) ?
  O4a As2 O6 6_546 . . 107.2(8) ?
  O4a As2 O6 6_546 . 4_556 78.7(7) ?
  O4a As2 O4b 7_555 . 6_546 91.9(8) ?
  O4a As2 O4b 7_555 . 7_555 10.8(8) ?
  O4a As2 As2 7_555 . 4_556 93.7(13) ?
  O4a As2 As2 7_555 . 7_555 108.4(6) ?
  O4a As2 As3 7_555 . . 62.0(5) ?
  O4a As2 As3 7_555 . 4_556 79.1(5) ?
  O4a As2 As3 7_555 . 13_556 60.7(5) ?
  O4a As2 As3 7_555 . 6_546 82.3(6) ?
  O4a As2 As3 7_555 . 7_555 48.8(5) ?
  O4a As2 Ca 7_555 . . 139.0(8) ?
  O4a As2 Ca 7_555 . 6_546 83.0(6) ?
  O4a As2 Ca 7_555 . 6_556 120.7(6) ?
  O4a As2 O6 7_555 . . 93.1(8) ?
  O4a As2 O6 7_555 . 4_556 94.1(7) ?
  O4b As2 O4b 6_546 . 7_555 101.9(9) ?
  O4b As2 As2 6_546 . 4_556 71.0(13) ?
  O4b As2 As2 6_546 . 7_555 81.2(7) ?
  O4b As2 As3 6_546 . . 95.2(7) ?
  O4b As2 As3 6_546 . 4_556 53.0(7) ?
  O4b As2 As3 6_546 . 13_556 126.7(7) ?
  O4b As2 As3 6_546 . 6_546 41.4(6) ?
  O4b As2 As3 6_546 . 7_555 99.1(7) ?
  O4b As2 Ca 6_546 . . 119.5(9) ?
  O4b As2 Ca 6_546 . 6_546 104.7(7) ?
  O4b As2 Ca 6_546 . 6_556 88.0(7) ?
  O4b As2 O6 6_546 . . 108.1(9) ?
  O4b As2 O6 6_546 . 4_556 76.5(8) ?
  O4b As2 As2 7_555 . 4_556 93.2(14) ?
  O4b As2 As2 7_555 . 7_555 113.4(7) ?
  O4b As2 As3 7_555 . . 65.5(7) ?
  O4b As2 As3 7_555 . 4_556 82.4(7) ?
  O4b As2 As3 7_555 . 13_556 57.5(7) ?
  O4b As2 As3 7_555 . 6_546 87.5(7) ?
  O4b As2 As3 7_555 . 7_555 51.6(7) ?
  O4b As2 Ca 7_555 . . 128.7(9) ?
  O4b As2 Ca 7_555 . 6_546 76.8(7) ?
  O4b As2 Ca 7_555 . 6_556 124.2(8) ?
  O4b As2 O6 7_555 . . 93.6(9) ?
  O4b As2 O6 7_555 . 4_556 92.6(8) ?
  As2 As2 As2 4_556 . 7_555 145.0(13) ?
  As2 As2 As3 4_556 . . 152.3(12) ?
  As2 As2 As3 4_556 . 4_556 24.2(11) ?
  As2 As2 As3 4_556 . 13_556 146.4(13) ?
  As2 As2 As3 4_556 . 6_546 32.7(11) ?
  As2 As2 As3 4_556 . 7_555 141.7(12) ?
  As2 As2 Ca 4_556 . . 74.8(12) ?
  As2 As2 Ca 4_556 . 6_546 35.1(11) ?
  As2 As2 Ca 4_556 . 6_556 140.6(13) ?
  As2 As2 O6 4_556 . . 173.2(14) ?
  As2 As2 O6 4_556 . 4_556 5.5(11) ?
  As2 As2 As3 7_555 . . 48.19(19) ?
  As2 As2 As3 7_555 . 4_556 134.1(3) ?
  As2 As2 As3 7_555 . 13_556 68.1(2) ?
  As2 As2 As3 7_555 . 6_546 122.4(3) ?
  As2 As2 As3 7_555 . 7_555 62.1(2) ?
  As2 As2 Ca 7_555 . . 102.4(6) ?
  As2 As2 Ca 7_555 . 6_546 167.3(4) ?
  As2 As2 Ca 7_555 . 6_556 14.1(4) ?
  As2 As2 O6 7_555 . . 30.5(5) ?
  As2 As2 O6 7_555 . 4_556 148.7(5) ?
  As3 As2 As3 . . 4_556 129.5(3) ?
  As3 As2 As3 . . 13_556 32.27(17) ?
  As3 As2 As3 . . 6_546 124.0(3) ?
  As3 As2 As3 . . 7_555 13.95(16) ?
  As3 As2 Ca . . . 132.0(6) ?
  As3 As2 Ca . . 6_546 140.3(3) ?
  As3 As2 Ca . . 6_556 59.0(3) ?
  As3 As2 O6 . . . 33.6(6) ?
  As3 As2 O6 . . 4_556 154.8(5) ?
  As3 As2 As3 4_556 . 13_556 139.7(3) ?
  As3 As2 As3 4_556 . 6_546 11.70(14) ?
  As3 As2 As3 4_556 . 7_555 121.9(3) ?
  As3 As2 Ca 4_556 . . 98.4(6) ?
  As3 As2 Ca 4_556 . 6_546 52.3(3) ?
  As3 As2 Ca 4_556 . 6_556 138.5(3) ?
  As3 As2 O6 4_556 . . 158.7(6) ?
  As3 As2 O6 4_556 . 4_556 28.9(5) ?
  As3 As2 As3 13_556 . 6_546 142.3(3) ?
  As3 As2 As3 13_556 . 7_555 28.1(2) ?
  As3 As2 Ca 13_556 . . 109.3(6) ?
  As3 As2 Ca 13_556 . 6_546 114.8(2) ?
  As3 As2 Ca 13_556 . 6_556 72.62(18) ?
  As3 As2 O6 13_556 . . 39.5(5) ?
  As3 As2 O6 13_556 . 4_556 143.2(5) ?
  As3 As2 As3 6_546 . 7_555 119.3(3) ?
  As3 As2 Ca 6_546 . . 103.5(6) ?
  As3 As2 Ca 6_546 . 6_546 63.6(3) ?
  As3 As2 Ca 6_546 . 6_556 127.3(3) ?
  As3 As2 O6 6_546 . . 148.4(6) ?
  As3 As2 O6 6_546 . 4_556 38.0(5) ?
  As3 As2 Ca 7_555 . . 136.5(7) ?
  As3 As2 Ca 7_555 . 6_546 126.6(3) ?
  As3 As2 Ca 7_555 . 6_556 72.7(3) ?
  As3 As2 O6 7_555 . . 44.9(6) ?
  As3 As2 O6 7_555 . 4_556 142.8(5) ?
  Ca As2 Ca . . 6_546 64.9(6) ?
  Ca As2 Ca . . 6_556 88.3(6) ?
  Ca As2 O6 . . . 100.3(8) ?
  Ca As2 O6 . . 4_556 71.0(7) ?
  Ca As2 Ca 6_546 . 6_556 153.2(5) ?
  Ca As2 O6 6_546 . . 147.1(6) ?
  Ca As2 O6 6_546 . 4_556 30.1(4) ?
  Ca As2 O6 6_556 . . 33.2(5) ?
  Ca As2 O6 6_556 . 4_556 142.5(5) ?
  O6 As2 O6 . . 4_556 171.3(8) ?
  Fe1 As3 Fe2 10_565 . . 73.67(16) ?
  Fe1 As3 Fe2 10_565 . 6_546 146.1(2) ?
  Fe1 As3 W2 10_565 . . 68.9(4) ?
  Fe1 As3 W2 10_565 . 4_566 73.1(5) ?
  Fe1 As3 W2 10_565 . 6_546 147.3(4) ?
  Fe1 As3 W2 10_565 . 7_555 149.6(4) ?
  Fe1 As3 O4a 10_565 . . 33.8(5) ?
  Fe1 As3 O4b 10_565 . . 31.9(5) ?
  Fe1 As3 O5 10_565 . . 116.7(2) ?
  Fe1 As3 As2 10_565 . . 133.1(2) ?
  Fe1 As3 As2 10_565 . 4_556 136.2(2) ?
  Fe1 As3 As2 10_565 . 13_556 59.49(15) ?
  Fe1 As3 As2 10_565 . 6_556 62.09(16) ?
  Fe1 As3 As2 10_565 . 7_555 65.66(19) ?
  Fe1 As3 As3 10_565 . 11_556 76.4(3) ?
  Fe1 As3 As3 10_565 . 13_556 104.8(3) ?
  Fe1 As3 As3 10_565 . 7_555 166.4(7) ?
  Fe1 As3 Ca 10_565 . . 125.8(3) ?
  Fe1 As3 Ca 10_565 . 10_555 116.62(15) ?
  Fe1 As3 Ca 10_565 . 13_556 61.67(15) ?
  Fe1 As3 Ca 10_565 . 6_556 65.59(12) ?
  Fe1 As3 O6 10_565 . . 100.2(3) ?
  Fe1 As3 O6 10_565 . 11_556 93.3(2) ?
  Fe2 As3 Fe2 . . 6_546 72.4(2) ?
  Fe2 As3 W2 . . . 9.3(5) ?
  Fe2 As3 W2 . . 4_566 7.2(5) ?
  Fe2 As3 W2 . . 6_546 74.4(4) ?
  Fe2 As3 W2 . . 7_555 76.9(4) ?
  Fe2 As3 O4a . . . 42.0(5) ?
  Fe2 As3 O4b . . . 52.2(6) ?
  Fe2 As3 O5 . . . 44.1(2) ?
  Fe2 As3 As2 . . . 99.1(2) ?
  Fe2 As3 As2 . . 4_556 98.1(2) ?
  Fe2 As3 As2 . . 13_556 113.1(2) ?
  Fe2 As3 As2 . . 6_556 59.4(3) ?
  Fe2 As3 As2 . . 7_555 63.9(4) ?
  Fe2 As3 As3 . . 11_556 149.9(4) ?
  Fe2 As3 As3 . . 13_556 176.3(5) ?
  Fe2 As3 As3 . . 7_555 119.9(7) ?
  Fe2 As3 Ca . . . 104.5(3) ?
  Fe2 As3 Ca . . 10_555 130.9(5) ?
  Fe2 As3 Ca . . 13_556 103.2(3) ?
  Fe2 As3 Ca . . 6_556 74.5(4) ?
  Fe2 As3 O6 . . . 103.0(6) ?
  Fe2 As3 O6 . . 11_556 128.7(6) ?
  Fe2 As3 W2 6_546 . . 77.4(4) ?
  Fe2 As3 W2 6_546 . 4_566 73.2(5) ?
  Fe2 As3 W2 6_546 . 6_546 6.3(5) ?
  Fe2 As3 W2 6_546 . 7_555 8.0(4) ?
  Fe2 As3 O4a 6_546 . . 113.0(6) ?
  Fe2 As3 O4b 6_546 . . 118.8(6) ?
  Fe2 As3 O5 6_546 . . 30.7(2) ?
  Fe2 As3 As2 6_546 . . 53.2(3) ?
  Fe2 As3 As2 6_546 . 4_556 49.8(3) ?
  Fe2 As3 As2 6_546 . 13_556 138.0(3) ?
  Fe2 As3 As2 6_546 . 6_556 99.0(2) ?
  Fe2 As3 As2 6_546 . 7_555 98.1(3) ?
  Fe2 As3 As3 6_546 . 11_556 137.3(4) ?
  Fe2 As3 As3 6_546 . 13_556 109.0(3) ?
  Fe2 As3 As3 6_546 . 7_555 47.4(6) ?
  Fe2 As3 Ca 6_546 . . 63.4(4) ?
  Fe2 As3 Ca 6_546 . 10_555 86.9(2) ?
  Fe2 As3 Ca 6_546 . 13_556 128.0(4) ?
  Fe2 As3 Ca 6_546 . 6_556 103.9(3) ?
  Fe2 As3 O6 6_546 . . 86.5(5) ?
  Fe2 As3 O6 6_546 . 11_556 108.5(4) ?
  W2 As3 W2 . . 4_566 4.3(6) ?
  W2 As3 W2 . . 6_546 78.6(6) ?
  W2 As3 W2 . . 7_555 81.0(6) ?
  W2 As3 O4a . . . 35.7(7) ?
  W2 As3 O4b . . . 44.4(6) ?
  W2 As3 O5 . . . 51.2(5) ?
  W2 As3 As2 . . . 96.5(5) ?
  W2 As3 As2 . . 4_556 96.1(5) ?
  W2 As3 As2 . . 13_556 114.9(5) ?
  W2 As3 As2 . . 6_556 50.2(4) ?
  W2 As3 As2 . . 7_555 54.9(5) ?
  W2 As3 As3 . . 11_556 143.3(5) ?
  W2 As3 As3 . . 13_556 167.0(6) ?
  W2 As3 As3 . . 7_555 124.4(8) ?
  W2 As3 Ca . . . 100.6(5) ?
  W2 As3 Ca . . 10_555 140.0(6) ?
  W2 As3 Ca . . 13_556 106.6(5) ?
  W2 As3 Ca . . 6_556 65.3(5) ?
  W2 As3 O6 . . . 95.8(7) ?
  W2 As3 O6 . . 11_556 135.4(7) ?
  W2 As3 W2 4_566 . 6_546 74.4(6) ?
  W2 As3 W2 4_566 . 7_555 76.8(6) ?
  W2 As3 O4a 4_566 . . 40.0(7) ?
  W2 As3 O4b 4_566 . . 48.6(7) ?
  W2 As3 O5 4_566 . . 46.9(5) ?
  W2 As3 As2 4_566 . . 94.2(5) ?
  W2 As3 As2 4_566 . 4_556 93.6(5) ?
  W2 As3 As2 4_566 . 13_556 117.6(5) ?
  W2 As3 As2 4_566 . 6_556 52.5(5) ?
  W2 As3 As2 4_566 . 7_555 56.9(5) ?
  W2 As3 As3 4_566 . 11_556 147.6(6) ?
  W2 As3 As3 4_566 . 13_556 169.1(6) ?
  W2 As3 As3 4_566 . 7_555 120.2(8) ?
  W2 As3 Ca 4_566 . . 98.9(5) ?
  W2 As3 Ca 4_566 . 10_555 137.8(6) ?
  W2 As3 Ca 4_566 . 13_556 108.6(5) ?
  W2 As3 Ca 4_566 . 6_556 67.5(5) ?
  W2 As3 O6 4_566 . . 96.0(7) ?
  W2 As3 O6 4_566 . 11_556 135.7(7) ?
  W2 As3 W2 6_546 . 7_555 2.6(5) ?
  W2 As3 O4a 6_546 . . 113.6(7) ?
  W2 As3 O4b 6_546 . . 117.8(7) ?
  W2 As3 O5 6_546 . . 34.8(4) ?
  W2 As3 As2 6_546 . . 47.0(4) ?
  W2 As3 As2 6_546 . 4_556 43.6(4) ?
  W2 As3 As2 6_546 . 13_556 143.1(5) ?
  W2 As3 As2 6_546 . 6_556 95.3(5) ?
  W2 As3 As2 6_546 . 7_555 93.9(5) ?
  W2 As3 As3 6_546 . 11_556 134.5(5) ?
  W2 As3 As3 6_546 . 13_556 106.6(5) ?
  W2 As3 As3 6_546 . 7_555 45.8(7) ?
  W2 As3 Ca 6_546 . . 57.2(5) ?
  W2 As3 Ca 6_546 . 10_555 89.8(4) ?
  W2 As3 Ca 6_546 . 13_556 133.9(5) ?
  W2 As3 Ca 6_546 . 6_556 99.0(4) ?
  W2 As3 O6 6_546 . . 80.3(6) ?
  W2 As3 O6 6_546 . 11_556 112.2(5) ?
  W2 As3 O4a 7_555 . . 115.9(7) ?
  W2 As3 O4b 7_555 . . 119.7(7) ?
  W2 As3 O5 7_555 . . 37.3(4) ?
  W2 As3 As2 7_555 . . 45.3(4) ?
  W2 As3 As2 7_555 . 4_556 41.9(4) ?
  W2 As3 As2 7_555 . 13_556 142.8(4) ?
  W2 As3 As2 7_555 . 6_556 96.2(4) ?
  W2 As3 As2 7_555 . 7_555 94.6(4) ?
  W2 As3 As3 7_555 . 11_556 131.9(5) ?
  W2 As3 As3 7_555 . 13_556 104.1(4) ?
  W2 As3 As3 7_555 . 7_555 43.4(6) ?
  W2 As3 Ca 7_555 . . 55.5(4) ?
  W2 As3 Ca 7_555 . 10_555 88.6(4) ?
  W2 As3 Ca 7_555 . 13_556 134.2(5) ?
  W2 As3 Ca 7_555 . 6_556 99.3(4) ?
  W2 As3 O6 7_555 . . 79.0(6) ?
  W2 As3 O6 7_555 . 11_556 111.2(5) ?
  O4a As3 O4b . . . 13.8(7) ?
  O4a As3 O5 . . . 86.1(6) ?
  O4a As3 As2 . . . 115.5(6) ?
  O4a As3 As2 . . 4_556 116.9(6) ?
  O4a As3 As2 . . 13_556 89.0(5) ?
  O4a As3 As2 . . 6_556 43.3(5) ?
  O4a As3 As2 . . 7_555 48.7(5) ?
  O4a As3 As3 . . 11_556 108.1(6) ?
  O4a As3 As3 . . 13_556 135.6(6) ?
  O4a As3 As3 . . 7_555 158.5(8) ?
  O4a As3 Ca . . . 113.7(6) ?
  O4a As3 Ca . . 10_555 141.3(6) ?
  O4a As3 Ca . . 13_556 86.3(5) ?
  O4a As3 Ca . . 6_556 55.0(6) ?
  O4a As3 O6 . . . 95.0(6) ?
  O4a As3 O6 . . 11_556 120.8(6) ?
  O4b As3 O5 . . . 95.5(6) ?
  O4b As3 As2 . . . 107.9(6) ?
  O4b As3 As2 . . 4_556 110.0(6) ?
  O4b As3 As2 . . 13_556 91.2(6) ?
  O4b As3 As2 . . 6_556 33.6(5) ?
  O4b As3 As2 . . 7_555 38.5(5) ?
  O4b As3 As3 . . 11_556 99.0(6) ?
  O4b As3 As3 . . 13_556 124.8(6) ?
  O4b As3 As3 . . 7_555 155.7(9) ?
  O4b As3 Ca . . . 104.1(6) ?
  O4b As3 Ca . . 10_555 147.8(6) ?
  O4b As3 Ca . . 13_556 91.6(6) ?
  O4b As3 Ca . . 6_556 42.9(5) ?
  O4b As3 O6 . . . 82.9(6) ?
  O4b As3 O6 . . 11_556 124.8(6) ?
  O5 As3 As2 . . . 77.2(4) ?
  O5 As3 As2 . . 4_556 74.3(3) ?
  O5 As3 As2 . . 13_556 127.8(5) ?
  O5 As3 As2 . . 6_556 89.5(4) ?
  O5 As3 As2 . . 7_555 91.4(4) ?
  O5 As3 As3 . . 11_556 165.4(4) ?
  O5 As3 As3 . . 13_556 138.1(4) ?
  O5 As3 As3 . . 7_555 76.8(6) ?
  O5 As3 Ca . . . 86.9(4) ?
  O5 As3 Ca . . 10_555 99.8(4) ?
  O5 As3 Ca . . 13_556 114.6(5) ?
  O5 As3 Ca . . 6_556 101.0(5) ?
  O5 As3 O6 . . . 103.7(7) ?
  O5 As3 O6 . . 11_556 114.1(7) ?
  As2 As3 As2 . . 4_556 3.54(16) ?
  As2 As3 As2 . . 13_556 147.7(3) ?
  As2 As3 As2 . . 6_556 74.3(2) ?
  As2 As3 As2 . . 7_555 69.7(2) ?
  As2 As3 As3 . . 11_556 98.7(4) ?
  As2 As3 As3 . . 13_556 79.5(3) ?
  As2 As3 As3 . . 7_555 48.2(6) ?
  As2 As3 Ca . . . 10.2(3) ?
  As2 As3 Ca . . 10_555 103.1(2) ?
  As2 As3 Ca . . 13_556 156.6(3) ?
  As2 As3 Ca . . 6_556 67.86(19) ?
  As2 As3 O6 . . . 35.0(4) ?
  As2 As3 O6 . . 11_556 123.0(3) ?
  As2 As3 As2 4_556 . 13_556 148.8(3) ?
  As2 As3 As2 4_556 . 6_556 76.5(2) ?
  As2 As3 As2 4_556 . 7_555 72.0(2) ?
  As2 As3 As3 4_556 . 11_556 101.0(4) ?
  As2 As3 As3 4_556 . 13_556 80.7(3) ?
  As2 As3 As3 4_556 . 7_555 45.9(6) ?
  As2 As3 Ca 4_556 . . 13.6(3) ?
  As2 As3 Ca 4_556 . 10_555 101.5(2) ?
  As2 As3 Ca 4_556 . 13_556 156.3(2) ?
  As2 As3 Ca 4_556 . 6_556 70.69(18) ?
  As2 As3 O6 4_556 . . 38.5(4) ?
  As2 As3 O6 4_556 . 11_556 122.0(3) ?
  As2 As3 As2 13_556 . 6_556 120.1(2) ?
  As2 As3 As2 13_556 . 7_555 122.3(3) ?
  As2 As3 As3 13_556 . 11_556 51.6(3) ?
  As2 As3 As3 13_556 . 13_556 68.3(3) ?
  As2 As3 As3 13_556 . 7_555 111.9(6) ?
  As2 As3 Ca 13_556 . . 140.9(3) ?
  As2 As3 Ca 13_556 . 10_555 57.17(15) ?
  As2 As3 Ca 13_556 . 13_556 13.3(3) ?
  As2 As3 Ca 13_556 . 6_556 117.8(2) ?
  As2 As3 O6 13_556 . . 128.5(6) ?
  As2 As3 O6 13_556 . 11_556 33.9(2) ?
  As2 As3 As2 6_556 . 7_555 5.55(19) ?
  As2 As3 As3 6_556 . 11_556 103.0(4) ?
  As2 As3 As3 6_556 . 13_556 116.9(4) ?
  As2 As3 As3 6_556 . 7_555 122.4(7) ?
  As2 As3 Ca 6_556 . . 70.8(2) ?
  As2 As3 Ca 6_556 . 10_555 169.6(4) ?
  As2 As3 Ca 6_556 . 13_556 123.8(2) ?
  As2 As3 Ca 6_556 . 6_556 15.2(3) ?
  As2 As3 O6 6_556 . . 52.4(4) ?
  As2 As3 O6 6_556 . 11_556 152.5(4) ?
  As2 As3 As3 7_555 . 11_556 100.3(4) ?
  As2 As3 As3 7_555 . 13_556 112.3(4) ?
  As2 As3 As3 7_555 . 7_555 117.9(7) ?
  As2 As3 Ca 7_555 . . 65.7(2) ?
  As2 As3 Ca 7_555 . 10_555 165.1(4) ?
  As2 As3 Ca 7_555 . 13_556 127.2(3) ?
  As2 As3 Ca 7_555 . 6_556 10.7(3) ?
  As2 As3 O6 7_555 . . 46.9(4) ?
  As2 As3 O6 7_555 . 11_556 152.9(5) ?
  As3 As3 As3 11_556 . 13_556 28.3(3) ?
  As3 As3 As3 11_556 . 7_555 90.0(7) ?
  As3 As3 Ca 11_556 . . 90.1(4) ?
  As3 As3 Ca 11_556 . 10_555 67.2(4) ?
  As3 As3 Ca 11_556 . 13_556 64.6(4) ?
  As3 As3 Ca 11_556 . 6_556 90.1(4) ?
  As3 As3 O6 11_556 . . 78.8(7) ?
  As3 As3 O6 11_556 . 11_556 56.2(6) ?
  As3 As3 As3 13_556 . 7_555 61.7(6) ?
  As3 As3 Ca 13_556 . . 73.5(3) ?
  As3 As3 Ca 13_556 . 10_555 52.9(4) ?
  As3 As3 Ca 13_556 . 13_556 78.7(4) ?
  As3 As3 Ca 13_556 . 6_556 101.8(4) ?
  As3 As3 O6 13_556 . . 73.8(6) ?
  As3 As3 O6 13_556 . 11_556 54.4(5) ?
  As3 As3 Ca 7_555 . . 53.1(6) ?
  As3 As3 Ca 7_555 . 10_555 56.3(5) ?
  As3 As3 Ca 7_555 . 13_556 112.6(6) ?
  As3 As3 Ca 7_555 . 6_556 115.2(7) ?
  As3 As3 O6 7_555 . . 76.7(6) ?
  As3 As3 O6 7_555 . 11_556 78.8(6) ?
  Ca As3 Ca . . 10_555 104.9(2) ?
  Ca As3 Ca . . 13_556 152.3(3) ?
  Ca As3 Ca . . 6_556 62.1(2) ?
  Ca As3 O6 . . . 25.9(4) ?
  Ca As3 O6 . . 11_556 122.0(3) ?
  Ca As3 Ca 10_555 . 13_556 56.28(12) ?
  Ca As3 Ca 10_555 . 6_556 154.7(5) ?
  Ca As3 O6 10_555 . . 120.1(5) ?
  Ca As3 O6 10_555 . 11_556 23.32(17) ?
  Ca As3 Ca 13_556 . 6_556 125.2(3) ?
  Ca As3 O6 13_556 . . 141.7(7) ?
  Ca As3 O6 13_556 . 11_556 34.47(16) ?
  Ca As3 O6 6_556 . . 40.1(3) ?
  Ca As3 O6 6_556 . 11_556 144.6(6) ?
  O6 As3 O6 . . 11_556 128.2(8) ?
  Fe1 Ca Fe1 . . 10_555 121.7(6) ?
  Fe1 Ca Fe2 . . 6_546 60.9(3) ?
  Fe1 Ca W2 . . 1_545 91.7(5) ?
  Fe1 Ca W2 . . 4_566 45.9(3) ?
  Fe1 Ca W2 . . 6_546 60.2(5) ?
  Fe1 Ca W2 . . 7_555 61.6(5) ?
  Fe1 Ca As1 . . 10_555 173.6(6) ?
  Fe1 Ca As1 . . 11_555 52.51(4) ?
  Fe1 Ca P1 . . 10_555 173.6(6) ?
  Fe1 Ca P1 . . 11_555 52.51(4) ?
  Fe1 Ca O2 . . 10_555 152.0(8) ?
  Fe1 Ca O2 . . 11_555 31.8(3) ?
  Fe1 Ca O4a . . 6_546 33.7(4) ?
  Fe1 Ca O4a . . 7_555 88.9(6) ?
  Fe1 Ca O4b . . 6_546 28.5(5) ?
  Fe1 Ca O4b . . 7_555 94.4(8) ?
  Fe1 Ca As2 . . . 61.8(6) ?
  Fe1 Ca As2 . . 4_556 62.1(6) ?
  Fe1 Ca As2 . . 6_546 110.5(4) ?
  Fe1 Ca As2 . . 6_556 51.22(14) ?
  Fe1 Ca As2 . . 7_545 114.5(4) ?
  Fe1 Ca As2 . . 7_555 54.27(17) ?
  Fe1 Ca As3 . . . 76.8(3) ?
  Fe1 Ca As3 . . 10_554 65.39(18) ?
  Fe1 Ca As3 . . 11_556 96.8(3) ?
  Fe1 Ca As3 . . 4_556 68.9(3) ?
  Fe1 Ca As3 . . 13_556 104.4(4) ?
  Fe1 Ca As3 . . 6_546 57.5(2) ?
  Fe1 Ca As3 . . 7_555 82.6(4) ?
  Fe1 Ca As3 . . 16_544 54.63(17) ?
  Fe1 Ca Ca . . 6_546 120.6(4) ?
  Fe1 Ca Ca . . 6_556 59.4(2) ?
  Fe1 Ca Fe3 . . 9_445 138.8(4) ?
  Fe1 Ca Fe3 . . 12_455 99.4(2) ?
  Fe1 Ca O6 . . . 77.1(5) ?
  Fe1 Ca O6 . . 4_556 85.4(5) ?
  Fe1 Ca Ow2 . . 9_445 119.1(3) ?
  Fe1 Ca Fe2 10_555 . 6_546 60.9(3) ?
  Fe1 Ca W2 10_555 . 1_545 45.9(3) ?
  Fe1 Ca W2 10_555 . 4_566 91.7(5) ?
  Fe1 Ca W2 10_555 . 6_546 61.6(5) ?
  Fe1 Ca W2 10_555 . 7_555 60.2(5) ?
  Fe1 Ca As1 10_555 . 10_555 52.51(4) ?
  Fe1 Ca As1 10_555 . 11_555 173.6(6) ?
  Fe1 Ca P1 10_555 . 10_555 52.51(4) ?
  Fe1 Ca P1 10_555 . 11_555 173.6(6) ?
  Fe1 Ca O2 10_555 . 10_555 31.8(3) ?
  Fe1 Ca O2 10_555 . 11_555 152.0(8) ?
  Fe1 Ca O4a 10_555 . 6_546 88.9(6) ?
  Fe1 Ca O4a 10_555 . 7_555 33.7(4) ?
  Fe1 Ca O4b 10_555 . 6_546 94.4(8) ?
  Fe1 Ca O4b 10_555 . 7_555 28.5(5) ?
  Fe1 Ca As2 10_555 . . 62.1(6) ?
  Fe1 Ca As2 10_555 . 4_556 61.8(6) ?
  Fe1 Ca As2 10_555 . 6_546 54.27(17) ?
  Fe1 Ca As2 10_555 . 6_556 114.5(4) ?
  Fe1 Ca As2 10_555 . 7_545 51.22(14) ?
  Fe1 Ca As2 10_555 . 7_555 110.5(4) ?
  Fe1 Ca As3 10_555 . . 68.9(3) ?
  Fe1 Ca As3 10_555 . 10_554 96.8(3) ?
  Fe1 Ca As3 10_555 . 11_556 65.39(18) ?
  Fe1 Ca As3 10_555 . 4_556 76.8(3) ?
  Fe1 Ca As3 10_555 . 13_556 54.63(17) ?
  Fe1 Ca As3 10_555 . 6_546 82.6(4) ?
  Fe1 Ca As3 10_555 . 7_555 57.5(2) ?
  Fe1 Ca As3 10_555 . 16_544 104.4(4) ?
  Fe1 Ca Ca 10_555 . 6_546 59.4(2) ?
  Fe1 Ca Ca 10_555 . 6_556 120.6(4) ?
  Fe1 Ca Fe3 10_555 . 9_445 99.4(2) ?
  Fe1 Ca Fe3 10_555 . 12_455 138.8(4) ?
  Fe1 Ca O6 10_555 . . 85.4(5) ?
  Fe1 Ca O6 10_555 . 4_556 77.1(5) ?
  Fe1 Ca Ow2 10_555 . 9_445 119.1(3) ?
  Fe2 Ca W2 6_546 . 1_545 46.8(3) ?
  Fe2 Ca W2 6_546 . 4_566 46.8(3) ?
  Fe2 Ca W2 6_546 . 6_546 2.6(3) ?
  Fe2 Ca W2 6_546 . 7_555 2.6(3) ?
  Fe2 Ca As1 6_546 . 10_555 113.3(3) ?
  Fe2 Ca As1 6_546 . 11_555 113.3(3) ?
  Fe2 Ca P1 6_546 . 10_555 113.3(3) ?
  Fe2 Ca P1 6_546 . 11_555 113.3(3) ?
  Fe2 Ca O2 6_546 . 10_555 91.9(5) ?
  Fe2 Ca O2 6_546 . 11_555 91.9(5) ?
  Fe2 Ca O4a 6_546 . 6_546 29.0(4) ?
  Fe2 Ca O4a 6_546 . 7_555 29.0(4) ?
  Fe2 Ca O4b 6_546 . 6_546 34.5(6) ?
  Fe2 Ca O4b 6_546 . 7_555 34.5(6) ?
  Fe2 Ca As2 6_546 . . 15.2(6) ?
  Fe2 Ca As2 6_546 . 4_556 15.2(6) ?
  Fe2 Ca As2 6_546 . 6_546 76.1(4) ?
  Fe2 Ca As2 6_546 . 6_556 77.4(3) ?
  Fe2 Ca As2 6_546 . 7_545 77.4(3) ?
  Fe2 Ca As2 6_546 . 7_555 76.1(4) ?
  Fe2 Ca As3 6_546 . . 52.9(3) ?
  Fe2 Ca As3 6_546 . 10_554 72.2(3) ?
  Fe2 Ca As3 6_546 . 11_556 72.2(3) ?
  Fe2 Ca As3 6_546 . 4_556 52.9(3) ?
  Fe2 Ca As3 6_546 . 13_556 70.2(3) ?
  Fe2 Ca As3 6_546 . 6_546 46.9(3) ?
  Fe2 Ca As3 6_546 . 7_555 46.9(3) ?
  Fe2 Ca As3 6_546 . 16_544 70.2(3) ?
  Fe2 Ca Ca 6_546 . 6_546 90.0(5) ?
  Fe2 Ca Ca 6_546 . 6_556 90.0(5) ?
  Fe2 Ca Fe3 6_546 . 9_445 160.13(15) ?
  Fe2 Ca Fe3 6_546 . 12_455 160.13(15) ?
  Fe2 Ca O6 6_546 . . 71.8(7) ?
  Fe2 Ca O6 6_546 . 4_556 71.8(7) ?
  Fe2 Ca Ow2 6_546 . 9_445 180.0(5) ?
  W2 Ca W2 1_545 . 4_566 93.7(5) ?
  W2 Ca W2 1_545 . 6_546 49.3(4) ?
  W2 Ca W2 1_545 . 7_555 44.4(4) ?
  W2 Ca As1 1_545 . 10_555 85.3(3) ?
  W2 Ca As1 1_545 . 11_555 128.5(3) ?
  W2 Ca P1 1_545 . 10_555 85.3(3) ?
  W2 Ca P1 1_545 . 11_555 128.5(3) ?
  W2 Ca O2 1_545 . 10_555 62.4(4) ?
  W2 Ca O2 1_545 . 11_555 120.6(6) ?
  W2 Ca O4a 1_545 . 6_546 60.8(5) ?
  W2 Ca O4a 1_545 . 7_555 44.9(5) ?
  W2 Ca O4b 1_545 . 6_546 64.8(6) ?
  W2 Ca O4b 1_545 . 7_555 45.4(6) ?
  W2 Ca As2 1_545 . . 59.9(7) ?
  W2 Ca As2 1_545 . 4_556 35.1(5) ?
  W2 Ca As2 1_545 . 6_546 29.3(3) ?
  W2 Ca As2 1_545 . 6_556 124.2(6) ?
  W2 Ca As2 1_545 . 7_545 30.7(3) ?
  W2 Ca As2 1_545 . 7_555 122.9(6) ?
  W2 Ca As3 1_545 . . 91.8(5) ?
  W2 Ca As3 1_545 . 10_554 51.6(3) ?
  W2 Ca As3 1_545 . 11_556 101.8(4) ?
  W2 Ca As3 1_545 . 4_556 31.0(3) ?
  W2 Ca As3 1_545 . 13_556 93.3(4) ?
  W2 Ca As3 1_545 . 6_546 38.3(3) ?
  W2 Ca As3 1_545 . 7_555 81.3(5) ?
  W2 Ca As3 1_545 . 16_544 58.6(4) ?
  W2 Ca Ca 1_545 . 6_546 43.2(4) ?
  W2 Ca Ca 1_545 . 6_556 136.8(7) ?
  W2 Ca Fe3 1_545 . 9_445 118.6(3) ?
  W2 Ca Fe3 1_545 . 12_455 144.0(3) ?
  W2 Ca O6 1_545 . . 112.8(8) ?
  W2 Ca O6 1_545 . 4_556 35.4(6) ?
  W2 Ca Ow2 1_545 . 9_445 133.2(3) ?
  W2 Ca W2 4_566 . 6_546 44.4(4) ?
  W2 Ca W2 4_566 . 7_555 49.3(4) ?
  W2 Ca As1 4_566 . 10_555 128.5(3) ?
  W2 Ca As1 4_566 . 11_555 85.3(3) ?
  W2 Ca P1 4_566 . 10_555 128.5(3) ?
  W2 Ca P1 4_566 . 11_555 85.3(3) ?
  W2 Ca O2 4_566 . 10_555 120.6(6) ?
  W2 Ca O2 4_566 . 11_555 62.4(4) ?
  W2 Ca O4a 4_566 . 6_546 44.9(5) ?
  W2 Ca O4a 4_566 . 7_555 60.8(5) ?
  W2 Ca O4b 4_566 . 6_546 45.4(6) ?
  W2 Ca O4b 4_566 . 7_555 64.8(6) ?
  W2 Ca As2 4_566 . . 35.1(5) ?
  W2 Ca As2 4_566 . 4_556 59.9(7) ?
  W2 Ca As2 4_566 . 6_546 122.9(6) ?
  W2 Ca As2 4_566 . 6_556 30.7(3) ?
  W2 Ca As2 4_566 . 7_545 124.2(6) ?
  W2 Ca As2 4_566 . 7_555 29.3(3) ?
  W2 Ca As3 4_566 . . 31.0(3) ?
  W2 Ca As3 4_566 . 10_554 101.8(4) ?
  W2 Ca As3 4_566 . 11_556 51.6(3) ?
  W2 Ca As3 4_566 . 4_556 91.8(5) ?
  W2 Ca As3 4_566 . 13_556 58.6(4) ?
  W2 Ca As3 4_566 . 6_546 81.3(5) ?
  W2 Ca As3 4_566 . 7_555 38.3(3) ?
  W2 Ca As3 4_566 . 16_544 93.3(4) ?
  W2 Ca Ca 4_566 . 6_546 136.8(7) ?
  W2 Ca Ca 4_566 . 6_556 43.2(4) ?
  W2 Ca Fe3 4_566 . 9_445 144.0(3) ?
  W2 Ca Fe3 4_566 . 12_455 118.6(3) ?
  W2 Ca O6 4_566 . . 35.4(6) ?
  W2 Ca O6 4_566 . 4_556 112.8(8) ?
  W2 Ca Ow2 4_566 . 9_445 133.2(3) ?
  W2 Ca W2 6_546 . 7_555 5.3(5) ?
  W2 Ca As1 6_546 . 10_555 113.8(5) ?
  W2 Ca As1 6_546 . 11_555 112.7(5) ?
  W2 Ca P1 6_546 . 10_555 113.8(5) ?
  W2 Ca P1 6_546 . 11_555 112.7(5) ?
  W2 Ca O2 6_546 . 10_555 92.9(7) ?
  W2 Ca O2 6_546 . 11_555 90.9(7) ?
  W2 Ca O4a 6_546 . 6_546 29.2(6) ?
  W2 Ca O4a 6_546 . 7_555 29.1(6) ?
  W2 Ca O4b 6_546 . 6_546 34.6(7) ?
  W2 Ca O4b 6_546 . 7_555 34.6(7) ?
  W2 Ca As2 6_546 . . 12.6(7) ?
  W2 Ca As2 6_546 . 4_556 17.8(7) ?
  W2 Ca As2 6_546 . 6_546 78.6(5) ?
  W2 Ca As2 6_546 . 6_556 75.0(4) ?
  W2 Ca As2 6_546 . 7_545 79.9(5) ?
  W2 Ca As2 6_546 . 7_555 73.6(5) ?
  W2 Ca As3 6_546 . . 50.4(5) ?
  W2 Ca As3 6_546 . 10_554 74.4(5) ?
  W2 Ca As3 6_546 . 11_556 70.0(5) ?
  W2 Ca As3 6_546 . 4_556 55.3(5) ?
  W2 Ca As3 6_546 . 13_556 68.4(5) ?
  W2 Ca As3 6_546 . 6_546 49.1(5) ?
  W2 Ca As3 6_546 . 7_555 44.7(5) ?
  W2 Ca As3 6_546 . 16_544 72.1(5) ?
  W2 Ca Ca 6_546 . 6_546 92.5(6) ?
  W2 Ca Ca 6_546 . 6_556 87.5(6) ?
  W2 Ca Fe3 6_546 . 9_445 161.0(4) ?
  W2 Ca Fe3 6_546 . 12_455 159.0(4) ?
  W2 Ca O6 6_546 . . 69.2(8) ?
  W2 Ca O6 6_546 . 4_556 74.4(8) ?
  W2 Ca Ow2 6_546 . 9_445 177.4(3) ?
  W2 Ca As1 7_555 . 10_555 112.7(5) ?
  W2 Ca As1 7_555 . 11_555 113.8(5) ?
  W2 Ca P1 7_555 . 10_555 112.7(5) ?
  W2 Ca P1 7_555 . 11_555 113.8(5) ?
  W2 Ca O2 7_555 . 10_555 90.9(7) ?
  W2 Ca O2 7_555 . 11_555 92.9(7) ?
  W2 Ca O4a 7_555 . 6_546 29.1(6) ?
  W2 Ca O4a 7_555 . 7_555 29.2(6) ?
  W2 Ca O4b 7_555 . 6_546 34.6(7) ?
  W2 Ca O4b 7_555 . 7_555 34.6(7) ?
  W2 Ca As2 7_555 . . 17.8(7) ?
  W2 Ca As2 7_555 . 4_556 12.6(7) ?
  W2 Ca As2 7_555 . 6_546 73.6(5) ?
  W2 Ca As2 7_555 . 6_556 79.9(5) ?
  W2 Ca As2 7_555 . 7_545 75.0(4) ?
  W2 Ca As2 7_555 . 7_555 78.6(5) ?
  W2 Ca As3 7_555 . . 55.3(5) ?
  W2 Ca As3 7_555 . 10_554 70.0(5) ?
  W2 Ca As3 7_555 . 11_556 74.4(5) ?
  W2 Ca As3 7_555 . 4_556 50.4(5) ?
  W2 Ca As3 7_555 . 13_556 72.1(5) ?
  W2 Ca As3 7_555 . 6_546 44.7(5) ?
  W2 Ca As3 7_555 . 7_555 49.1(5) ?
  W2 Ca As3 7_555 . 16_544 68.4(5) ?
  W2 Ca Ca 7_555 . 6_546 87.5(6) ?
  W2 Ca Ca 7_555 . 6_556 92.5(6) ?
  W2 Ca Fe3 7_555 . 9_445 159.0(4) ?
  W2 Ca Fe3 7_555 . 12_455 161.0(4) ?
  W2 Ca O6 7_555 . . 74.4(8) ?
  W2 Ca O6 7_555 . 4_556 69.2(8) ?
  W2 Ca Ow2 7_555 . 9_445 177.4(3) ?
  As1 Ca As1 10_555 . 11_555 133.4(6) ?
  As1 Ca P1 10_555 . 10_555 0.0(5) ?
  As1 Ca P1 10_555 . 11_555 133.4(6) ?
  As1 Ca O2 10_555 . 10_555 23.5(3) ?
  As1 Ca O2 10_555 . 11_555 152.9(8) ?
  As1 Ca O4a 10_555 . 6_546 141.2(6) ?
  As1 Ca O4a 10_555 . 7_555 85.0(4) ?
  As1 Ca O4b 10_555 . 6_546 146.6(8) ?
  As1 Ca O4b 10_555 . 7_555 79.5(5) ?
  As1 Ca As2 10_555 . . 111.8(5) ?
  As1 Ca As2 10_555 . 4_556 113.1(5) ?
  As1 Ca As2 10_555 . 6_546 69.14(12) ?
  As1 Ca As2 10_555 . 6_556 126.53(15) ?
  As1 Ca As2 10_555 . 7_545 64.98(11) ?
  As1 Ca As2 10_555 . 7_555 123.11(15) ?
  As1 Ca As3 10_555 . . 97.54(13) ?
  As1 Ca As3 10_555 . 10_554 116.45(9) ?
  As1 Ca As3 10_555 . 11_556 78.24(9) ?
  As1 Ca As3 10_555 . 4_556 110.26(14) ?
  As1 Ca As3 10_555 . 13_556 70.12(10) ?
  As1 Ca As3 10_555 . 6_546 121.2(2) ?
  As1 Ca As3 10_555 . 7_555 91.29(14) ?
  As1 Ca As3 10_555 . 16_544 127.44(10) ?
  As1 Ca Ca 10_555 . 6_546 60.33(18) ?
  As1 Ca Ca 10_555 . 6_556 119.7(3) ?
  As1 Ca Fe3 10_555 . 9_445 47.2(3) ?
  As1 Ca Fe3 10_555 . 12_455 86.3(4) ?
  As1 Ca O6 10_555 . . 98.8(4) ?
  As1 Ca O6 10_555 . 4_556 95.4(4) ?
  As1 Ca Ow2 10_555 . 9_445 66.7(3) ?
  As1 Ca P1 11_555 . 10_555 133.4(6) ?
  As1 Ca P1 11_555 . 11_555 0.0(5) ?
  As1 Ca O2 11_555 . 10_555 152.9(8) ?
  As1 Ca O2 11_555 . 11_555 23.5(3) ?
  As1 Ca O4a 11_555 . 6_546 85.0(4) ?
  As1 Ca O4a 11_555 . 7_555 141.2(6) ?
  As1 Ca O4b 11_555 . 6_546 79.5(5) ?
  As1 Ca O4b 11_555 . 7_555 146.6(8) ?
  As1 Ca As2 11_555 . . 113.1(5) ?
  As1 Ca As2 11_555 . 4_556 111.8(5) ?
  As1 Ca As2 11_555 . 6_546 123.11(15) ?
  As1 Ca As2 11_555 . 6_556 64.98(11) ?
  As1 Ca As2 11_555 . 7_545 126.53(15) ?
  As1 Ca As2 11_555 . 7_555 69.14(12) ?
  As1 Ca As3 11_555 . . 110.26(14) ?
  As1 Ca As3 11_555 . 10_554 78.24(9) ?
  As1 Ca As3 11_555 . 11_556 116.45(9) ?
  As1 Ca As3 11_555 . 4_556 97.54(13) ?
  As1 Ca As3 11_555 . 13_556 127.44(10) ?
  As1 Ca As3 11_555 . 6_546 91.29(14) ?
  As1 Ca As3 11_555 . 7_555 121.2(2) ?
  As1 Ca As3 11_555 . 16_544 70.12(10) ?
  As1 Ca Ca 11_555 . 6_546 119.7(3) ?
  As1 Ca Ca 11_555 . 6_556 60.33(18) ?
  As1 Ca Fe3 11_555 . 9_445 86.3(4) ?
  As1 Ca Fe3 11_555 . 12_455 47.2(3) ?
  As1 Ca O6 11_555 . . 95.4(4) ?
  As1 Ca O6 11_555 . 4_556 98.8(4) ?
  As1 Ca Ow2 11_555 . 9_445 66.7(3) ?
  P1 Ca P1 10_555 . 11_555 133.4(6) ?
  P1 Ca O2 10_555 . 10_555 23.5(3) ?
  P1 Ca O2 10_555 . 11_555 152.9(8) ?
  P1 Ca O4a 10_555 . 6_546 141.2(6) ?
  P1 Ca O4a 10_555 . 7_555 85.0(4) ?
  P1 Ca O4b 10_555 . 6_546 146.6(8) ?
  P1 Ca O4b 10_555 . 7_555 79.5(5) ?
  P1 Ca As2 10_555 . . 111.8(5) ?
  P1 Ca As2 10_555 . 4_556 113.1(5) ?
  P1 Ca As2 10_555 . 6_546 69.14(12) ?
  P1 Ca As2 10_555 . 6_556 126.53(15) ?
  P1 Ca As2 10_555 . 7_545 64.98(11) ?
  P1 Ca As2 10_555 . 7_555 123.11(15) ?
  P1 Ca As3 10_555 . . 97.54(13) ?
  P1 Ca As3 10_555 . 10_554 116.45(9) ?
  P1 Ca As3 10_555 . 11_556 78.24(9) ?
  P1 Ca As3 10_555 . 4_556 110.26(14) ?
  P1 Ca As3 10_555 . 13_556 70.12(10) ?
  P1 Ca As3 10_555 . 6_546 121.2(2) ?
  P1 Ca As3 10_555 . 7_555 91.29(14) ?
  P1 Ca As3 10_555 . 16_544 127.44(10) ?
  P1 Ca Ca 10_555 . 6_546 60.33(18) ?
  P1 Ca Ca 10_555 . 6_556 119.7(3) ?
  P1 Ca Fe3 10_555 . 9_445 47.2(3) ?
  P1 Ca Fe3 10_555 . 12_455 86.3(4) ?
  P1 Ca O6 10_555 . . 98.8(4) ?
  P1 Ca O6 10_555 . 4_556 95.4(4) ?
  P1 Ca Ow2 10_555 . 9_445 66.7(3) ?
  P1 Ca O2 11_555 . 10_555 152.9(8) ?
  P1 Ca O2 11_555 . 11_555 23.5(3) ?
  P1 Ca O4a 11_555 . 6_546 85.0(4) ?
  P1 Ca O4a 11_555 . 7_555 141.2(6) ?
  P1 Ca O4b 11_555 . 6_546 79.5(5) ?
  P1 Ca O4b 11_555 . 7_555 146.6(8) ?
  P1 Ca As2 11_555 . . 113.1(5) ?
  P1 Ca As2 11_555 . 4_556 111.8(5) ?
  P1 Ca As2 11_555 . 6_546 123.11(15) ?
  P1 Ca As2 11_555 . 6_556 64.98(11) ?
  P1 Ca As2 11_555 . 7_545 126.53(15) ?
  P1 Ca As2 11_555 . 7_555 69.14(12) ?
  P1 Ca As3 11_555 . . 110.26(14) ?
  P1 Ca As3 11_555 . 10_554 78.24(9) ?
  P1 Ca As3 11_555 . 11_556 116.45(9) ?
  P1 Ca As3 11_555 . 4_556 97.54(13) ?
  P1 Ca As3 11_555 . 13_556 127.44(10) ?
  P1 Ca As3 11_555 . 6_546 91.29(14) ?
  P1 Ca As3 11_555 . 7_555 121.2(2) ?
  P1 Ca As3 11_555 . 16_544 70.12(10) ?
  P1 Ca Ca 11_555 . 6_546 119.7(3) ?
  P1 Ca Ca 11_555 . 6_556 60.33(18) ?
  P1 Ca Fe3 11_555 . 9_445 86.3(4) ?
  P1 Ca Fe3 11_555 . 12_455 47.2(3) ?
  P1 Ca O6 11_555 . . 95.4(4) ?
  P1 Ca O6 11_555 . 4_556 98.8(4) ?
  P1 Ca Ow2 11_555 . 9_445 66.7(3) ?
  O2 Ca O2 10_555 . 11_555 176.2(10) ?
  O2 Ca O4a 10_555 . 6_546 118.3(8) ?
  O2 Ca O4a 10_555 . 7_555 65.5(5) ?
  O2 Ca O4b 10_555 . 6_546 123.5(9) ?
  O2 Ca O4b 10_555 . 7_555 60.3(6) ?
  O2 Ca As2 10_555 . . 93.9(7) ?
  O2 Ca As2 10_555 . 4_556 89.8(7) ?
  O2 Ca As2 10_555 . 6_546 51.5(2) ?
  O2 Ca As2 10_555 . 6_556 133.9(3) ?
  O2 Ca As2 10_555 . 7_545 47.2(2) ?
  O2 Ca As2 10_555 . 7_555 129.7(3) ?
  O2 Ca As3 10_555 . . 92.5(4) ?
  O2 Ca As3 10_555 . 10_554 101.7(3) ?
  O2 Ca As3 10_555 . 11_556 79.5(2) ?
  O2 Ca As3 10_555 . 4_556 89.8(4) ?
  O2 Ca As3 10_555 . 13_556 69.0(2) ?
  O2 Ca As3 10_555 . 6_546 99.7(4) ?
  O2 Ca As3 10_555 . 7_555 82.9(4) ?
  O2 Ca As3 10_555 . 16_544 112.4(3) ?
  O2 Ca Ca 10_555 . 6_546 47.29(17) ?
  O2 Ca Ca 10_555 . 6_556 132.71(17) ?
  O2 Ca Fe3 10_555 . 9_445 68.2(5) ?
  O2 Ca Fe3 10_555 . 12_455 108.0(6) ?
  O2 Ca O6 10_555 . . 102.0(5) ?
  O2 Ca O6 10_555 . 4_556 79.2(4) ?
  O2 Ca Ow2 10_555 . 9_445 88.1(5) ?
  O2 Ca O4a 11_555 . 6_546 65.5(5) ?
  O2 Ca O4a 11_555 . 7_555 118.3(8) ?
  O2 Ca O4b 11_555 . 6_546 60.3(6) ?
  O2 Ca O4b 11_555 . 7_555 123.5(9) ?
  O2 Ca As2 11_555 . . 89.8(7) ?
  O2 Ca As2 11_555 . 4_556 93.9(7) ?
  O2 Ca As2 11_555 . 6_546 129.7(3) ?
  O2 Ca As2 11_555 . 6_556 47.2(2) ?
  O2 Ca As2 11_555 . 7_545 133.9(3) ?
  O2 Ca As2 11_555 . 7_555 51.5(2) ?
  O2 Ca As3 11_555 . . 89.8(4) ?
  O2 Ca As3 11_555 . 10_554 79.5(2) ?
  O2 Ca As3 11_555 . 11_556 101.7(3) ?
  O2 Ca As3 11_555 . 4_556 92.5(4) ?
  O2 Ca As3 11_555 . 13_556 112.4(3) ?
  O2 Ca As3 11_555 . 6_546 82.9(4) ?
  O2 Ca As3 11_555 . 7_555 99.7(4) ?
  O2 Ca As3 11_555 . 16_544 69.0(2) ?
  O2 Ca Ca 11_555 . 6_546 132.71(17) ?
  O2 Ca Ca 11_555 . 6_556 47.29(17) ?
  O2 Ca Fe3 11_555 . 9_445 108.0(6) ?
  O2 Ca Fe3 11_555 . 12_455 68.2(5) ?
  O2 Ca O6 11_555 . . 79.2(4) ?
  O2 Ca O6 11_555 . 4_556 102.0(5) ?
  O2 Ca Ow2 11_555 . 9_445 88.1(5) ?
  O4a Ca O4a 6_546 . 7_555 58.1(7) ?
  O4a Ca O4b 6_546 . 6_546 5.5(6) ?
  O4a Ca O4b 6_546 . 7_555 63.5(8) ?
  O4a Ca As2 6_546 . . 36.0(7) ?
  O4a Ca As2 6_546 . 4_556 28.5(6) ?
  O4a Ca As2 6_546 . 6_546 85.8(5) ?
  O4a Ca As2 6_546 . 6_556 68.8(4) ?
  O4a Ca As2 6_546 . 7_545 88.9(5) ?
  O4a Ca As2 6_546 . 7_555 69.7(5) ?
  O4a Ca As3 6_546 . . 67.5(5) ?
  O4a Ca As3 6_546 . 10_554 57.7(4) ?
  O4a Ca As3 6_546 . 11_556 90.0(6) ?
  O4a Ca As3 6_546 . 4_556 47.7(4) ?
  O4a Ca As3 6_546 . 13_556 92.1(6) ?
  O4a Ca As3 6_546 . 6_546 36.7(4) ?
  O4a Ca As3 6_546 . 7_555 66.8(6) ?
  O4a Ca As3 6_546 . 16_544 51.0(4) ?
  O4a Ca Ca 6_546 . 6_546 99.1(6) ?
  O4a Ca Ca 6_546 . 6_556 80.9(5) ?
  O4a Ca Fe3 6_546 . 9_445 166.8(4) ?
  O4a Ca Fe3 6_546 . 12_455 132.1(4) ?
  O4a Ca O6 6_546 . . 79.6(8) ?
  O4a Ca O6 6_546 . 4_556 68.5(7) ?
  O4a Ca Ow2 6_546 . 9_445 151.0(4) ?
  O4a Ca O4b 7_555 . 6_546 63.5(8) ?
  O4a Ca O4b 7_555 . 7_555 5.5(6) ?
  O4a Ca As2 7_555 . . 28.5(6) ?
  O4a Ca As2 7_555 . 4_556 36.0(7) ?
  O4a Ca As2 7_555 . 6_546 69.7(5) ?
  O4a Ca As2 7_555 . 6_556 88.9(5) ?
  O4a Ca As2 7_555 . 7_545 68.8(4) ?
  O4a Ca As2 7_555 . 7_555 85.8(5) ?
  O4a Ca As3 7_555 . . 47.7(4) ?
  O4a Ca As3 7_555 . 10_554 90.0(6) ?
  O4a Ca As3 7_555 . 11_556 57.7(4) ?
  O4a Ca As3 7_555 . 4_556 67.5(5) ?
  O4a Ca As3 7_555 . 13_556 51.0(4) ?
  O4a Ca As3 7_555 . 6_546 66.8(6) ?
  O4a Ca As3 7_555 . 7_555 36.7(4) ?
  O4a Ca As3 7_555 . 16_544 92.1(6) ?
  O4a Ca Ca 7_555 . 6_546 80.9(5) ?
  O4a Ca Ca 7_555 . 6_556 99.1(6) ?
  O4a Ca Fe3 7_555 . 9_445 132.1(4) ?
  O4a Ca Fe3 7_555 . 12_455 166.8(4) ?
  O4a Ca O6 7_555 . . 68.5(7) ?
  O4a Ca O6 7_555 . 4_556 79.6(8) ?
  O4a Ca Ow2 7_555 . 9_445 151.0(4) ?
  O4b Ca O4b 6_546 . 7_555 69.0(9) ?
  O4b Ca As2 6_546 . . 40.7(8) ?
  O4b Ca As2 6_546 . 4_556 33.6(7) ?
  O4b Ca As2 6_546 . 6_546 88.5(6) ?
  O4b Ca As2 6_546 . 6_556 67.0(5) ?
  O4b Ca As2 6_546 . 7_545 91.8(6) ?
  O4b Ca As2 6_546 . 7_555 68.2(5) ?
  O4b Ca As3 6_546 . . 70.2(6) ?
  O4b Ca As3 6_546 . 10_554 56.5(5) ?
  O4b Ca As3 6_546 . 11_556 92.8(7) ?
  O4b Ca As3 6_546 . 4_556 49.0(5) ?
  O4b Ca As3 6_546 . 13_556 95.7(7) ?
  O4b Ca As3 6_546 . 6_546 37.5(5) ?
  O4b Ca As3 6_546 . 7_555 70.5(7) ?
  O4b Ca As3 6_546 . 16_544 48.8(5) ?
  O4b Ca Ca 6_546 . 6_546 101.4(7) ?
  O4b Ca Ca 6_546 . 6_556 78.6(6) ?
  O4b Ca Fe3 6_546 . 9_445 162.5(6) ?
  O4b Ca Fe3 6_546 . 12_455 126.7(5) ?
  O4b Ca O6 6_546 . . 80.6(9) ?
  O4b Ca O6 6_546 . 4_556 69.3(8) ?
  O4b Ca Ow2 6_546 . 9_445 145.5(6) ?
  O4b Ca As2 7_555 . . 33.6(7) ?
  O4b Ca As2 7_555 . 4_556 40.7(8) ?
  O4b Ca As2 7_555 . 6_546 68.2(5) ?
  O4b Ca As2 7_555 . 6_556 91.8(6) ?
  O4b Ca As2 7_555 . 7_545 67.0(5) ?
  O4b Ca As2 7_555 . 7_555 88.5(6) ?
  O4b Ca As3 7_555 . . 49.0(5) ?
  O4b Ca As3 7_555 . 10_554 92.8(7) ?
  O4b Ca As3 7_555 . 11_556 56.5(5) ?
  O4b Ca As3 7_555 . 4_556 70.2(6) ?
  O4b Ca As3 7_555 . 13_556 48.8(5) ?
  O4b Ca As3 7_555 . 6_546 70.5(7) ?
  O4b Ca As3 7_555 . 7_555 37.5(5) ?
  O4b Ca As3 7_555 . 16_544 95.7(7) ?
  O4b Ca Ca 7_555 . 6_546 78.6(6) ?
  O4b Ca Ca 7_555 . 6_556 101.4(7) ?
  O4b Ca Fe3 7_555 . 9_445 126.7(5) ?
  O4b Ca Fe3 7_555 . 12_455 162.5(6) ?
  O4b Ca O6 7_555 . . 69.3(8) ?
  O4b Ca O6 7_555 . 4_556 80.6(9) ?
  O4b Ca Ow2 7_555 . 9_445 145.5(6) ?
  As2 Ca As2 . . 4_556 30.4(10) ?
  As2 Ca As2 . . 6_546 88.9(8) ?
  As2 Ca As2 . . 6_556 65.5(4) ?
  As2 Ca As2 . . 7_545 89.7(7) ?
  As2 Ca As2 . . 7_555 63.5(4) ?
  As2 Ca As3 . . . 37.8(5) ?
  As2 Ca As3 . . 10_554 86.6(8) ?
  As2 Ca As3 . . 11_556 58.0(5) ?
  As2 Ca As3 . . 4_556 68.0(8) ?
  As2 Ca As3 . . 13_556 57.4(5) ?
  As2 Ca As3 . . 6_546 61.4(8) ?
  As2 Ca As3 . . 7_555 32.9(5) ?
  As2 Ca As3 . . 16_544 83.4(8) ?
  As2 Ca Ca . . 6_546 102.4(8) ?
  As2 Ca Ca . . 6_556 77.6(5) ?
  As2 Ca Fe3 . . 9_445 156.8(5) ?
  As2 Ca Fe3 . . 12_455 153.6(5) ?
  As2 Ca O6 . . . 56.6(7) ?
  As2 Ca O6 . . 4_556 86.9(11) ?
  As2 Ca Ow2 . . 9_445 164.8(6) ?
  As2 Ca As2 4_556 . 6_546 63.5(4) ?
  As2 Ca As2 4_556 . 6_556 89.7(7) ?
  As2 Ca As2 4_556 . 7_545 65.5(4) ?
  As2 Ca As2 4_556 . 7_555 88.9(8) ?
  As2 Ca As3 4_556 . . 68.0(8) ?
  As2 Ca As3 4_556 . 10_554 58.0(5) ?
  As2 Ca As3 4_556 . 11_556 86.6(8) ?
  As2 Ca As3 4_556 . 4_556 37.8(5) ?
  As2 Ca As3 4_556 . 13_556 83.4(8) ?
  As2 Ca As3 4_556 . 6_546 32.9(5) ?
  As2 Ca As3 4_556 . 7_555 61.4(8) ?
  As2 Ca As3 4_556 . 16_544 57.4(5) ?
  As2 Ca Ca 4_556 . 6_546 77.6(5) ?
  As2 Ca Ca 4_556 . 6_556 102.4(8) ?
  As2 Ca Fe3 4_556 . 9_445 153.6(5) ?
  As2 Ca Fe3 4_556 . 12_455 156.8(5) ?
  As2 Ca O6 4_556 . . 86.9(11) ?
  As2 Ca O6 4_556 . 4_556 56.6(7) ?
  As2 Ca Ow2 4_556 . 9_445 164.8(6) ?
  As2 Ca As2 6_546 . 6_556 153.2(7) ?
  As2 Ca As2 6_546 . 7_545 4.30(15) ?
  As2 Ca As2 6_546 . 7_555 152.2(7) ?
  As2 Ca As3 6_546 . . 117.2(5) ?
  As2 Ca As3 6_546 . 10_554 50.21(16) ?
  As2 Ca As3 6_546 . 11_556 119.5(3) ?
  As2 Ca As3 6_546 . 4_556 41.61(18) ?
  As2 Ca As3 6_546 . 13_556 108.9(3) ?
  As2 Ca As3 6_546 . 6_546 53.2(2) ?
  As2 Ca As3 6_546 . 7_555 105.7(5) ?
  As2 Ca As3 6_546 . 16_544 60.89(18) ?
  As2 Ca Ca 6_546 . 6_546 14.1(4) ?
  As2 Ca Ca 6_546 . 6_556 165.9(8) ?
  As2 Ca Fe3 6_546 . 9_445 90.7(3) ?
  As2 Ca Fe3 6_546 . 12_455 116.1(4) ?
  As2 Ca O6 6_546 . . 137.3(8) ?
  As2 Ca O6 6_546 . 4_556 27.7(4) ?
  As2 Ca Ow2 6_546 . 9_445 103.9(4) ?
  As2 Ca As2 6_556 . 7_545 154.8(6) ?
  As2 Ca As2 6_556 . 7_555 4.30(15) ?
  As2 Ca As3 6_556 . . 45.57(17) ?
  As2 Ca As3 6_556 . 10_554 116.6(3) ?
  As2 Ca As3 6_556 . 11_556 54.49(15) ?
  As2 Ca As3 6_556 . 4_556 115.9(4) ?
  As2 Ca As3 6_556 . 13_556 65.18(17) ?
  As2 Ca As3 6_556 . 6_546 104.3(4) ?
  As2 Ca As3 6_556 . 7_555 57.0(2) ?
  As2 Ca As3 6_556 . 16_544 105.8(3) ?
  As2 Ca Ca 6_556 . 6_546 167.3(7) ?
  As2 Ca Ca 6_556 . 6_556 12.7(4) ?
  As2 Ca Fe3 6_556 . 9_445 116.0(4) ?
  As2 Ca Fe3 6_556 . 12_455 88.4(3) ?
  As2 Ca O6 6_556 . . 32.0(4) ?
  As2 Ca O6 6_556 . 4_556 135.4(7) ?
  As2 Ca Ow2 6_556 . 9_445 102.6(3) ?
  As2 Ca As2 7_545 . 7_555 153.2(7) ?
  As2 Ca As3 7_545 . . 115.9(4) ?
  As2 Ca As3 7_545 . 10_554 54.49(15) ?
  As2 Ca As3 7_545 . 11_556 116.6(3) ?
  As2 Ca As3 7_545 . 4_556 45.57(17) ?
  As2 Ca As3 7_545 . 13_556 105.8(3) ?
  As2 Ca As3 7_545 . 6_546 57.0(2) ?
  As2 Ca As3 7_545 . 7_555 104.3(4) ?
  As2 Ca As3 7_545 . 16_544 65.18(17) ?
  As2 Ca Ca 7_545 . 6_546 12.7(4) ?
  As2 Ca Ca 7_545 . 6_556 167.3(7) ?
  As2 Ca Fe3 7_545 . 9_445 88.4(3) ?
  As2 Ca Fe3 7_545 . 12_455 116.0(4) ?
  As2 Ca O6 7_545 . . 135.4(7) ?
  As2 Ca O6 7_545 . 4_556 32.0(4) ?
  As2 Ca Ow2 7_545 . 9_445 102.6(3) ?
  As2 Ca As3 7_555 . . 41.61(18) ?
  As2 Ca As3 7_555 . 10_554 119.5(3) ?
  As2 Ca As3 7_555 . 11_556 50.21(16) ?
  As2 Ca As3 7_555 . 4_556 117.2(5) ?
  As2 Ca As3 7_555 . 13_556 60.89(18) ?
  As2 Ca As3 7_555 . 6_546 105.7(5) ?
  As2 Ca As3 7_555 . 7_555 53.2(2) ?
  As2 Ca As3 7_555 . 16_544 108.9(3) ?
  As2 Ca Ca 7_555 . 6_546 165.9(8) ?
  As2 Ca Ca 7_555 . 6_556 14.1(4) ?
  As2 Ca Fe3 7_555 . 9_445 116.1(4) ?
  As2 Ca Fe3 7_555 . 12_455 90.7(3) ?
  As2 Ca O6 7_555 . . 27.7(4) ?
  As2 Ca O6 7_555 . 4_556 137.3(8) ?
  As2 Ca Ow2 7_555 . 9_445 103.9(4) ?
  As3 Ca As3 . . 10_554 123.7(6) ?
  As3 Ca As3 . . 11_556 22.64(14) ?
  As3 Ca As3 . . 4_556 105.7(6) ?
  As3 Ca As3 . . 13_556 27.72(16) ?
  As3 Ca As3 . . 6_546 98.8(6) ?
  As3 Ca As3 . . 7_555 11.75(13) ?
  As3 Ca As3 . . 16_544 118.4(6) ?
  As3 Ca Ca . . 6_546 126.9(5) ?
  As3 Ca Ca . . 6_556 53.1(3) ?
  As3 Ca Fe3 . . 9_445 125.1(3) ?
  As3 Ca Fe3 . . 12_455 124.1(3) ?
  As3 Ca O6 . . . 21.0(5) ?
  As3 Ca O6 . . 4_556 123.8(9) ?
  As3 Ca Ow2 . . 9_445 127.1(3) ?
  As3 Ca As3 10_554 . 11_556 144.4(6) ?
  As3 Ca As3 10_554 . 4_556 22.64(14) ?
  As3 Ca As3 10_554 . 13_556 140.8(6) ?
  As3 Ca As3 10_554 . 6_546 25.35(15) ?
  As3 Ca As3 10_554 . 7_555 119.1(6) ?
  As3 Ca As3 10_554 . 16_544 11.04(11) ?
  As3 Ca Ca 10_554 . 6_546 56.34(16) ?
  As3 Ca Ca 10_554 . 6_556 123.7(2) ?
  As3 Ca Fe3 10_554 . 9_445 110.7(3) ?
  As3 Ca Fe3 10_554 . 12_455 102.8(3) ?
  As3 Ca O6 10_554 . . 137.1(8) ?
  As3 Ca O6 10_554 . 4_556 22.6(4) ?
  As3 Ca Ow2 10_554 . 9_445 107.8(3) ?
  As3 Ca As3 11_556 . 4_556 123.7(6) ?
  As3 Ca As3 11_556 . 13_556 11.04(11) ?
  As3 Ca As3 11_556 . 6_546 119.1(6) ?
  As3 Ca As3 11_556 . 7_555 25.35(15) ?
  As3 Ca As3 11_556 . 16_544 140.8(6) ?
  As3 Ca Ca 11_556 . 6_546 123.7(2) ?
  As3 Ca Ca 11_556 . 6_556 56.34(16) ?
  As3 Ca Fe3 11_556 . 9_445 102.8(3) ?
  As3 Ca Fe3 11_556 . 12_455 110.7(3) ?
  As3 Ca O6 11_556 . . 22.6(4) ?
  As3 Ca O6 11_556 . 4_556 137.1(8) ?
  As3 Ca Ow2 11_556 . 9_445 107.8(3) ?
  As3 Ca As3 4_556 . 13_556 118.4(6) ?
  As3 Ca As3 4_556 . 6_546 11.75(13) ?
  As3 Ca As3 4_556 . 7_555 98.8(6) ?
  As3 Ca As3 4_556 . 16_544 27.72(16) ?
  As3 Ca Ca 4_556 . 6_546 53.1(3) ?
  As3 Ca Ca 4_556 . 6_556 126.9(5) ?
  As3 Ca Fe3 4_556 . 9_445 124.1(3) ?
  As3 Ca Fe3 4_556 . 12_455 125.1(3) ?
  As3 Ca O6 4_556 . . 123.8(9) ?
  As3 Ca O6 4_556 . 4_556 21.0(5) ?
  As3 Ca Ow2 4_556 . 9_445 127.1(3) ?
  As3 Ca As3 13_556 . 6_546 116.2(6) ?
  As3 Ca As3 13_556 . 7_555 25.27(16) ?
  As3 Ca As3 13_556 . 16_544 140.4(7) ?
  As3 Ca Ca 13_556 . 6_546 112.6(2) ?
  As3 Ca Ca 13_556 . 6_556 67.38(17) ?
  As3 Ca Fe3 13_556 . 9_445 101.1(3) ?
  As3 Ca Fe3 13_556 . 12_455 116.4(4) ?
  As3 Ca O6 13_556 . . 33.3(4) ?
  As3 Ca O6 13_556 . 4_556 128.6(8) ?
  As3 Ca Ow2 13_556 . 9_445 109.8(3) ?
  As3 Ca As3 6_546 . 7_555 93.8(6) ?
  As3 Ca As3 6_546 . 16_544 25.27(16) ?
  As3 Ca Ca 6_546 . 6_546 64.8(3) ?
  As3 Ca Ca 6_546 . 6_556 115.2(5) ?
  As3 Ca Fe3 6_546 . 9_445 133.9(3) ?
  As3 Ca Fe3 6_546 . 12_455 126.3(3) ?
  As3 Ca O6 6_546 . . 114.9(9) ?
  As3 Ca O6 6_546 . 4_556 31.9(5) ?
  As3 Ca Ow2 6_546 . 9_445 133.1(3) ?
  As3 Ca As3 7_555 . 16_544 116.2(6) ?
  As3 Ca Ca 7_555 . 6_546 115.2(5) ?
  As3 Ca Ca 7_555 . 6_556 64.8(3) ?
  As3 Ca Fe3 7_555 . 9_445 126.3(3) ?
  As3 Ca Fe3 7_555 . 12_455 133.9(3) ?
  As3 Ca O6 7_555 . . 31.9(5) ?
  As3 Ca O6 7_555 . 4_556 114.9(9) ?
  As3 Ca Ow2 7_555 . 9_445 133.1(3) ?
  As3 Ca Ca 16_544 . 6_546 67.38(17) ?
  As3 Ca Ca 16_544 . 6_556 112.6(2) ?
  As3 Ca Fe3 16_544 . 9_445 116.4(4) ?
  As3 Ca Fe3 16_544 . 12_455 101.1(3) ?
  As3 Ca O6 16_544 . . 128.6(8) ?
  As3 Ca O6 16_544 . 4_556 33.3(4) ?
  As3 Ca Ow2 16_544 . 9_445 109.8(3) ?
  Ca Ca Ca 6_546 . 6_556 180.0(5) ?
  Ca Ca Fe3 6_546 . 9_445 76.7(4) ?
  Ca Ca Fe3 6_546 . 12_455 103.3(5) ?
  Ca Ca O6 6_546 . . 144.8(6) ?
  Ca Ca O6 6_546 . 4_556 35.2(4) ?
  Ca Ca Ow2 6_546 . 9_445 90.0(5) ?
  Ca Ca Fe3 6_556 . 9_445 103.3(5) ?
  Ca Ca Fe3 6_556 . 12_455 76.7(4) ?
  Ca Ca O6 6_556 . . 35.2(4) ?
  Ca Ca O6 6_556 . 4_556 144.8(6) ?
  Ca Ca Ow2 6_556 . 9_445 90.0(5) ?
  Fe3 Ca Fe3 9_445 . 12_455 39.7(3) ?
  Fe3 Ca O6 9_445 . . 111.2(7) ?
  Fe3 Ca O6 9_445 . 4_556 103.1(7) ?
  Fe3 Ca Ow2 9_445 . 9_445 19.87(15) ?
  Fe3 Ca O6 12_455 . . 103.1(7) ?
  Fe3 Ca O6 12_455 . 4_556 111.2(7) ?
  Fe3 Ca Ow2 12_455 . 9_445 19.87(15) ?
  O6 Ca O6 . . 4_556 143.5(13) ?
  O6 Ca Ow2 . . 9_445 108.2(7) ?
  O6 Ca Ow2 4_556 . 9_445 108.2(7) ?
  As1 Fe3 As1 . . 2_655 108.7(3) ?
  As1 Fe3 P1 . . . 0.0(5) ?
  As1 Fe3 P1 . . 2_655 108.7(3) ?
  As1 Fe3 O1 . . . 13.1(3) ?
  As1 Fe3 O1 . . 2_655 106.0(6) ?
  As1 Fe3 Ca . . 9_554 162.3(3) ?
  As1 Fe3 Ca . . 13_555 54.84(11) ?
  As1 Fe3 Fe3 . . 2_655 75.8(3) ?
  As1 Fe3 Fe3 . . 4_565 123.68(16) ?
  As1 Fe3 Ow1 . . . 76.9(7) ?
  As1 Fe3 Ow2 . . . 163.3(5) ?
  As1 Fe3 Ow2 . . 5_665 82.0(5) ?
  As1 Fe3 P1 2_655 . . 108.7(3) ?
  As1 Fe3 P1 2_655 . 2_655 0.0(5) ?
  As1 Fe3 O1 2_655 . . 106.0(6) ?
  As1 Fe3 O1 2_655 . 2_655 13.1(3) ?
  As1 Fe3 Ca 2_655 . 9_554 54.84(11) ?
  As1 Fe3 Ca 2_655 . 13_555 162.3(3) ?
  As1 Fe3 Fe3 2_655 . 2_655 75.8(3) ?
  As1 Fe3 Fe3 2_655 . 4_565 123.68(16) ?
  As1 Fe3 Ow1 2_655 . . 76.9(7) ?
  As1 Fe3 Ow2 2_655 . . 82.0(5) ?
  As1 Fe3 Ow2 2_655 . 5_665 163.3(5) ?
  P1 Fe3 P1 . . 2_655 108.7(3) ?
  P1 Fe3 O1 . . . 13.1(3) ?
  P1 Fe3 O1 . . 2_655 106.0(6) ?
  P1 Fe3 Ca . . 9_554 162.3(3) ?
  P1 Fe3 Ca . . 13_555 54.84(11) ?
  P1 Fe3 Fe3 . . 2_655 75.8(3) ?
  P1 Fe3 Fe3 . . 4_565 123.68(16) ?
  P1 Fe3 Ow1 . . . 76.9(7) ?
  P1 Fe3 Ow2 . . . 163.3(5) ?
  P1 Fe3 Ow2 . . 5_665 82.0(5) ?
  P1 Fe3 O1 2_655 . . 106.0(6) ?
  P1 Fe3 O1 2_655 . 2_655 13.1(3) ?
  P1 Fe3 Ca 2_655 . 9_554 54.84(11) ?
  P1 Fe3 Ca 2_655 . 13_555 162.3(3) ?
  P1 Fe3 Fe3 2_655 . 2_655 75.8(3) ?
  P1 Fe3 Fe3 2_655 . 4_565 123.68(16) ?
  P1 Fe3 Ow1 2_655 . . 76.9(7) ?
  P1 Fe3 Ow2 2_655 . . 82.0(5) ?
  P1 Fe3 Ow2 2_655 . 5_665 163.3(5) ?
  O1 Fe3 O1 . . 2_655 100.4(8) ?
  O1 Fe3 Ca . . 9_554 160.1(5) ?
  O1 Fe3 Ca . . 13_555 59.6(4) ?
  O1 Fe3 Fe3 . . 2_655 63.0(4) ?
  O1 Fe3 Fe3 . . 4_565 129.7(5) ?
  O1 Fe3 Ow1 . . . 88.3(9) ?
  O1 Fe3 Ow2 . . . 172.0(8) ?
  O1 Fe3 Ow2 . . 5_665 87.3(6) ?
  O1 Fe3 Ca 2_655 . 9_554 59.6(4) ?
  O1 Fe3 Ca 2_655 . 13_555 160.1(5) ?
  O1 Fe3 Fe3 2_655 . 2_655 63.0(4) ?
  O1 Fe3 Fe3 2_655 . 4_565 129.7(5) ?
  O1 Fe3 Ow1 2_655 . . 88.3(9) ?
  O1 Fe3 Ow2 2_655 . . 87.3(6) ?
  O1 Fe3 Ow2 2_655 . 5_665 172.0(8) ?
  Ca Fe3 Ca 9_554 . 13_555 140.3(3) ?
  Ca Fe3 Fe3 9_554 . 2_655 103.32(19) ?
  Ca Fe3 Fe3 9_554 . 4_565 70.13(15) ?
  Ca Fe3 Ow1 9_554 . . 91.7(4) ?
  Ca Fe3 Ow2 9_554 . . 27.7(5) ?
  Ca Fe3 Ow2 9_554 . 5_665 112.5(6) ?
  Ca Fe3 Fe3 13_555 . 2_655 103.32(19) ?
  Ca Fe3 Fe3 13_555 . 4_565 70.13(15) ?
  Ca Fe3 Ow1 13_555 . . 91.7(4) ?
  Ca Fe3 Ow2 13_555 . . 112.5(6) ?
  Ca Fe3 Ow2 13_555 . 5_665 27.7(5) ?
  Fe3 Fe3 Fe3 2_655 . 4_565 132.7(6) ?
  Fe3 Fe3 Ow1 2_655 . . 132.2(13) ?
  Fe3 Fe3 Ow2 2_655 . . 120.0(5) ?
  Fe3 Fe3 Ow2 2_655 . 5_665 120.0(5) ?
  Fe3 Fe3 Ow1 4_565 . . 95.1(12) ?
  Fe3 Fe3 Ow2 4_565 . . 42.4(5) ?
  Fe3 Fe3 Ow2 4_565 . 5_665 42.4(5) ?
  Ow1 Fe3 Ow2 . . . 93.8(9) ?
  Ow1 Fe3 Ow2 . . 5_665 93.8(9) ?
  Ow2 Fe3 Ow2 . . 5_665 84.8(7) ?
  As2 O6 As2 . . 4_556 1.3(3) ?
  As2 O6 As2 . . 6_556 118.2(9) ?
  As2 O6 As2 . . 7_555 119.0(10) ?
  As2 O6 As3 . . . 111.4(8) ?
  As2 O6 As3 . . 11_556 128.4(7) ?
  As2 O6 As3 . . 13_556 106.7(5) ?
  As2 O6 As3 . . 7_555 88.3(6) ?
  As2 O6 Ca . . . 23.0(6) ?
  As2 O6 Ca . . 6_556 119.2(9) ?
  As2 O6 As2 4_556 . 6_556 117.4(8) ?
  As2 O6 As2 4_556 . 7_555 118.2(9) ?
  As2 O6 As3 4_556 . . 112.6(7) ?
  As2 O6 As3 4_556 . 11_556 129.7(6) ?
  As2 O6 As3 4_556 . 13_556 107.9(4) ?
  As2 O6 As3 4_556 . 7_555 89.6(5) ?
  As2 O6 Ca 4_556 . . 22.1(6) ?
  As2 O6 Ca 4_556 . 6_556 118.0(8) ?
  As2 O6 As2 6_556 . 7_555 1.3(3) ?
  As2 O6 As3 6_556 . . 89.6(5) ?
  As2 O6 As3 6_556 . 11_556 107.9(4) ?
  As2 O6 As3 6_556 . 13_556 129.7(6) ?
  As2 O6 As3 6_556 . 7_555 112.6(7) ?
  As2 O6 Ca 6_556 . . 118.0(8) ?
  As2 O6 Ca 6_556 . 6_556 22.1(6) ?
  As2 O6 As3 7_555 . . 88.3(6) ?
  As2 O6 As3 7_555 . 11_556 106.7(5) ?
  As2 O6 As3 7_555 . 13_556 128.4(7) ?
  As2 O6 As3 7_555 . 7_555 111.4(8) ?
  As2 O6 Ca 7_555 . . 119.2(9) ?
  As2 O6 Ca 7_555 . 6_556 23.0(6) ?
  As3 O6 As3 . . 11_556 45.0(5) ?
  As3 O6 As3 . . 13_556 51.8(5) ?
  As3 O6 As3 . . 7_555 26.5(4) ?
  As3 O6 Ca . . . 133.1(8) ?
  As3 O6 Ca . . 6_556 108.0(6) ?
  As3 O6 As3 11_556 . 13_556 22.4(3) ?
  As3 O6 As3 11_556 . 7_555 51.8(5) ?
  As3 O6 Ca 11_556 . . 134.1(5) ?
  As3 O6 Ca 11_556 . 6_556 112.3(4) ?
  As3 O6 As3 13_556 . 7_555 45.0(5) ?
  As3 O6 Ca 13_556 . . 112.3(4) ?
  As3 O6 Ca 13_556 . 6_556 134.1(5) ?
  As3 O6 Ca 7_555 . . 108.0(6) ?
  As3 O6 Ca 7_555 . 6_556 133.1(8) ?
  Ca O6 Ca . . 6_556 109.5(8) ?
  Fe3 Ow1 Ow6 . . 9_554 118.1(13) ?
  Fe3 Ow1 Ow6 . . 10_564 118.1(13) ?
  Ow6 Ow1 Ow6 9_554 . 10_564 89.9(19) ?
  Ca Ow2 Fe3 9_554 . . 132.4(5) ?
  Ca Ow2 Fe3 9_554 . 4_565 132.4(5) ?
  Fe3 Ow2 Fe3 . . 4_565 95.2(9) ?
  Ow4 Ow3 Ow6 . . . 25(3) ?
  Ow3 Ow4 Ow6 . . . 16(2) ?
  Ow1 Ow6 Ow1 9_445 . 10_565 90.1(13) ?
  Ow1 Ow6 Ow3 9_445 . . 119(3) ?
  Ow1 Ow6 Ow4 9_445 . . 89(2) ?
  Ow1 Ow6 Ow3 10_565 . . 119(3) ?
  Ow1 Ow6 Ow4 10_565 . . 89(2) ?
  Ow3 Ow6 Ow4 . . . 138(5) ?

loop_
 _geom_torsion_atom_site_label_1
 _geom_torsion_atom_site_label_2
 _geom_torsion_atom_site_label_3
 _geom_torsion_atom_site_label_4
 _geom_torsion_site_symmetry_1
 _geom_torsion_site_symmetry_2
 _geom_torsion_site_symmetry_3
 _geom_torsion_site_symmetry_4
 _geom_torsion
 _geom_torsion_publ_flag
 ? ? ? ? ? ? ? ? ? ?

loop_
 _geom_hbond_atom_site_label_D
 _geom_hbond_atom_site_label_H
 _geom_hbond_atom_site_label_A
 _geom_hbond_site_symmetry_D
 _geom_hbond_site_symmetry_H
 _geom_hbond_site_symmetry_A
 _geom_hbond_distance_DH
 _geom_hbond_distance_HA
 _geom_hbond_distance_DA
 _geom_hbond_angle_DHA
 _geom_hbond_publ_flag
 ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 11. STRUCTURE-FACTOR LIST



